# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2015

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_K2MgTh3Mo8O32
_database_code_depnum_ccdc_archive 'CCDC 1430749'
_audit_update_record             
;
2015-10-12 deposited with the CCDC.
2015-11-12 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        K2MgTh3(MoO4)8
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'K2 Mg Mo8 O32 Th3'
_chemical_formula_weight         2078.15

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Th Th -7.2400 8.8979 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 2/c'
_symmetry_space_group_name_Hall  '-C 2yc'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   18.568(7)
_cell_length_b                   18.0282(19)
_cell_length_c                   9.4188(14)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.35(3)
_cell_angle_gamma                90.00
_cell_volume                     3152.8(13)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    5141
_cell_measurement_theta_min      3.0689
_cell_measurement_theta_max      32.4731
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.378
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3648
_exptl_absorpt_coefficient_mu    17.547
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.82583
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   
;
'Fri Sep 20 09:45:59 2013'
;

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Eos'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean 15.9834
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            5982
_diffrn_reflns_av_R_equivalents  0.0227
_diffrn_reflns_av_sigmaI/netI    0.0328
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_theta_min         3.13
_diffrn_reflns_theta_max         26.37
_reflns_number_total             3074
_reflns_number_gt                2882
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       
;
'Fri Sep 20 09:45:59 2013'
;
_computing_cell_refinement       
;
'Fri Sep 20 09:45:59 2013'
;
_computing_data_reduction        
;
'Fri Sep 20 09:45:59 2013'
;
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0140P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    .
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.000379(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         3074
_refine_ls_number_parameters     210
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0222
_refine_ls_R_factor_gt           0.0200
_refine_ls_wR_factor_ref         0.0434
_refine_ls_wR_factor_gt          0.0426
_refine_ls_goodness_of_fit_ref   1.059
_refine_ls_restrained_S_all      1.059
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Th1 Th 0.0000 0.131572(15) 0.7500 0.00802(7) Uani 1 2 d S . .
Th2 Th 0.248549(11) 0.119476(10) 1.338866(17) 0.00779(6) Uani 1 1 d . . .
Mo1 Mo 0.11742(2) 0.02400(3) 1.04738(4) 0.00842(10) Uani 1 1 d . . .
Mo2 Mo 0.09058(2) 0.25982(2) 0.46834(4) 0.00910(10) Uani 1 1 d . . .
Mo3 Mo 0.37913(3) 0.03438(2) 1.03543(4) 0.00872(11) Uani 1 1 d . . .
Mo4 Mo 0.21386(3) 0.17826(3) 0.75869(4) 0.01019(11) Uani 1 1 d . . .
K1 K 0.11719(8) 0.26030(9) 1.06220(14) 0.0347(4) Uani 1 1 d . . .
Mg1 Mg 0.5000 0.08907(13) 0.7500 0.0091(5) Uani 1 2 d S . .
O1 O 0.1196(2) 0.1796(2) 0.7975(4) 0.0194(9) Uani 1 1 d . . .
O2 O 0.0575(2) 0.3237(2) 0.3476(4) 0.0211(9) Uani 1 1 d . . .
O3 O 0.3283(2) 0.0900(2) 1.1545(3) 0.0178(9) Uani 1 1 d . . .
O4 O 0.2526(2) 0.2663(2) 0.7989(4) 0.0174(9) Uani 1 1 d . . .
O5 O 0.0176(2) 0.2212(2) 0.5653(3) 0.0182(9) Uani 1 1 d . . .
O6 O 0.4427(2) -0.0128(2) 1.1353(4) 0.0196(9) Uani 1 1 d . . .
O7 O 0.4239(2) 0.0923(2) 0.9145(3) 0.0166(9) Uani 1 1 d . . .
O8 O 0.0473(2) 0.0741(2) 0.9671(4) 0.0172(9) Uani 1 1 d . . .
O9 O 0.1722(2) 0.0867(2) 1.1422(4) 0.0176(9) Uani 1 1 d . . .
O10 O 0.1674(2) -0.0249(2) 0.9207(4) 0.0203(9) Uani 1 1 d . . .
O11 O 0.1523(2) 0.3015(2) 0.5865(4) 0.0212(9) Uani 1 1 d . . .
O12 O 0.3248(2) -0.0320(2) 0.9464(4) 0.0220(9) Uani 1 1 d . . .
O13 O 0.1325(2) 0.1893(2) 0.3697(4) 0.0237(9) Uani 1 1 d . . .
O14 O 0.2319(2) 0.1507(3) 0.5818(4) 0.0274(11) Uani 1 1 d . . .
O15 O 0.0813(2) -0.0406(2) 1.1687(3) 0.0217(10) Uani 1 1 d . . .
O16 O 0.2560(3) 0.1176(2) 0.8692(4) 0.0296(11) Uani 1 1 d . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Th1 O15 2.360(4) 5_557 ?
Th1 O15 2.360(4) 6 ?
Th1 O5 2.398(4) 2_556 ?
Th1 O5 2.398(4) . ?
Th1 O1 2.423(4) . ?
Th1 O1 2.423(4) 2_556 ?
Th1 O8 2.451(3) 2_556 ?
Th1 O8 2.451(3) . ?
Th1 K1 4.3231(16) . ?
Th1 K1 4.3231(16) 2_556 ?
Th2 O12 2.346(4) 6_556 ?
Th2 O3 2.350(4) . ?
Th2 O14 2.378(3) 1_556 ?
Th2 O9 2.400(4) . ?
Th2 O10 2.405(4) 6_556 ?
Th2 O11 2.429(4) 7_557 ?
Th2 O4 2.434(4) 7_557 ?
Th2 O13 2.513(4) 1_556 ?
Th2 K1 4.3711(18) . ?
Mo1 O8 1.752(4) . ?
Mo1 O10 1.754(4) . ?
Mo1 O9 1.759(4) . ?
Mo1 O15 1.767(4) . ?
Mo2 O2 1.730(4) . ?
Mo2 O11 1.760(4) . ?
Mo2 O13 1.760(4) . ?
Mo2 O5 1.781(4) . ?
Mo2 K1 3.8602(16) 1_554 ?
Mo2 K1 3.867(2) 2_556 ?
Mo3 O6 1.729(4) . ?
Mo3 O7 1.758(4) . ?
Mo3 O12 1.772(4) . ?
Mo3 O3 1.780(4) . ?
Mo3 K1 3.8147(18) 7_557 ?
Mo4 O16 1.697(4) . ?
Mo4 O14 1.773(4) . ?
Mo4 O4 1.783(4) . ?
Mo4 O1 1.790(4) . ?
Mo4 K1 3.6939(17) . ?
Mo4 K1 3.7213(19) 7_557 ?
K1 O7 2.774(4) 7_557 ?
K1 O4 2.784(4) 7_557 ?
K1 O5 2.858(4) 2_556 ?
K1 O1 2.887(4) . ?
K1 O2 3.130(4) 1_556 ?
K1 O13 3.178(4) 1_556 ?
K1 O16 3.284(5) 7_557 ?
K1 O9 3.376(4) . ?
K1 Mo4 3.7213(19) 7_557 ?
K1 Mo3 3.8147(18) 7_557 ?
K1 Mo2 3.8601(16) 1_556 ?
Mg1 O6 2.043(4) 6 ?
Mg1 O6 2.043(4) 5_657 ?
Mg1 O7 2.104(4) 2_656 ?
Mg1 O7 2.104(4) . ?
Mg1 O2 2.108(4) 7_556 ?
Mg1 O2 2.108(4) 8_556 ?
Mg1 K1 3.910(2) 7_557 ?
Mg1 K1 3.910(2) 8 ?
O2 Mg1 2.107(4) 7_556 ?
O2 K1 3.130(4) 1_554 ?
O4 Th2 2.434(4) 7_557 ?
O4 K1 2.784(4) 7_557 ?
O5 K1 2.858(4) 2_556 ?
O6 Mg1 2.043(4) 5_657 ?
O7 K1 2.774(4) 7_557 ?
O10 Th2 2.405(4) 6 ?
O11 Th2 2.429(4) 7_557 ?
O12 Th2 2.346(4) 6 ?
O13 Th2 2.513(4) 1_554 ?
O13 K1 3.178(4) 1_554 ?
O14 Th2 2.378(3) 1_554 ?
O15 Th1 2.360(4) 5_557 ?
O16 K1 3.284(5) 7_557 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O15 Th1 O15 92.0(2) 5_557 6 ?
O15 Th1 O5 98.17(14) 5_557 2_556 ?
O15 Th1 O5 142.56(13) 6 2_556 ?
O15 Th1 O5 142.55(13) 5_557 . ?
O15 Th1 O5 98.17(14) 6 . ?
O5 Th1 O5 95.31(18) 2_556 . ?
O15 Th1 O1 140.90(13) 5_557 . ?
O15 Th1 O1 73.79(14) 6 . ?
O5 Th1 O1 75.76(13) 2_556 . ?
O5 Th1 O1 76.35(13) . . ?
O15 Th1 O1 73.79(14) 5_557 2_556 ?
O15 Th1 O1 140.90(13) 6 2_556 ?
O5 Th1 O1 76.35(13) 2_556 2_556 ?
O5 Th1 O1 75.76(13) . 2_556 ?
O1 Th1 O1 138.1(2) . 2_556 ?
O15 Th1 O8 75.55(12) 5_557 2_556 ?
O15 Th1 O8 70.25(13) 6 2_556 ?
O5 Th1 O8 147.20(13) 2_556 2_556 ?
O5 Th1 O8 74.28(13) . 2_556 ?
O1 Th1 O8 128.95(13) . 2_556 ?
O1 Th1 O8 70.96(13) 2_556 2_556 ?
O15 Th1 O8 70.25(13) 5_557 . ?
O15 Th1 O8 75.55(12) 6 . ?
O5 Th1 O8 74.28(13) 2_556 . ?
O5 Th1 O8 147.20(13) . . ?
O1 Th1 O8 70.96(13) . . ?
O1 Th1 O8 128.95(13) 2_556 . ?
O8 Th1 O8 129.97(18) 2_556 . ?
O15 Th1 K1 118.20(9) 5_557 . ?
O15 Th1 K1 105.87(10) 6 . ?
O5 Th1 K1 38.29(9) 2_556 . ?
O5 Th1 K1 93.53(9) . . ?
O1 Th1 K1 39.24(9) . . ?
O1 Th1 K1 112.98(10) 2_556 . ?
O8 Th1 K1 166.16(9) 2_556 . ?
O8 Th1 K1 58.87(10) . . ?
O15 Th1 K1 105.87(10) 5_557 2_556 ?
O15 Th1 K1 118.20(9) 6 2_556 ?
O5 Th1 K1 93.53(9) 2_556 2_556 ?
O5 Th1 K1 38.29(9) . 2_556 ?
O1 Th1 K1 112.98(10) . 2_556 ?
O1 Th1 K1 39.24(9) 2_556 2_556 ?
O8 Th1 K1 58.87(9) 2_556 2_556 ?
O8 Th1 K1 166.16(9) . 2_556 ?
K1 Th1 K1 115.06(5) . 2_556 ?
O12 Th2 O3 77.61(13) 6_556 . ?
O12 Th2 O14 79.94(14) 6_556 1_556 ?
O3 Th2 O14 148.26(14) . 1_556 ?
O12 Th2 O9 121.32(14) 6_556 . ?
O3 Th2 O9 75.30(14) . . ?
O14 Th2 O9 136.16(15) 1_556 . ?
O12 Th2 O10 76.27(14) 6_556 6_556 ?
O3 Th2 O10 118.39(14) . 6_556 ?
O14 Th2 O10 76.94(14) 1_556 6_556 ?
O9 Th2 O10 72.80(13) . 6_556 ?
O12 Th2 O11 79.33(14) 6_556 7_557 ?
O3 Th2 O11 82.33(14) . 7_557 ?
O14 Th2 O11 71.65(14) 1_556 7_557 ?
O9 Th2 O11 144.23(12) . 7_557 ?
O10 Th2 O11 142.96(12) 6_556 7_557 ?
O12 Th2 O4 143.35(14) 6_556 7_557 ?
O3 Th2 O4 78.50(13) . 7_557 ?
O14 Th2 O4 108.18(14) 1_556 7_557 ?
O9 Th2 O4 78.11(12) . 7_557 ?
O10 Th2 O4 140.11(13) 6_556 7_557 ?
O11 Th2 O4 70.25(13) 7_557 7_557 ?
O12 Th2 O13 143.37(13) 6_556 1_556 ?
O3 Th2 O13 138.01(12) . 1_556 ?
O14 Th2 O13 69.74(14) 1_556 1_556 ?
O9 Th2 O13 73.13(13) . 1_556 ?
O10 Th2 O13 77.23(14) 6_556 1_556 ?
O11 Th2 O13 108.75(14) 7_557 1_556 ?
O4 Th2 O13 68.50(13) 7_557 1_556 ?
O12 Th2 K1 168.87(9) 6_556 . ?
O3 Th2 K1 92.45(9) . . ?
O14 Th2 K1 111.15(11) 1_556 . ?
O9 Th2 K1 50.07(10) . . ?
O10 Th2 K1 104.75(10) 6_556 . ?
O11 Th2 K1 104.54(10) 7_557 . ?
O4 Th2 K1 35.69(9) 7_557 . ?
O13 Th2 K1 45.78(9) 1_556 . ?
O8 Mo1 O10 111.15(17) . . ?
O8 Mo1 O9 108.26(19) . . ?
O10 Mo1 O9 111.19(19) . . ?
O8 Mo1 O15 109.57(19) . . ?
O10 Mo1 O15 108.2(2) . . ?
O9 Mo1 O15 108.39(16) . . ?
O2 Mo2 O11 111.04(19) . . ?
O2 Mo2 O13 106.93(18) . . ?
O11 Mo2 O13 110.70(19) . . ?
O2 Mo2 O5 109.24(19) . . ?
O11 Mo2 O5 109.69(17) . . ?
O13 Mo2 O5 109.19(19) . . ?
O2 Mo2 K1 52.69(13) . 1_554 ?
O11 Mo2 K1 122.60(13) . 1_554 ?
O13 Mo2 K1 54.46(13) . 1_554 ?
O5 Mo2 K1 127.70(12) . 1_554 ?
O2 Mo2 K1 66.36(15) . 2_556 ?
O11 Mo2 K1 133.72(14) . 2_556 ?
O13 Mo2 K1 114.03(14) . 2_556 ?
O5 Mo2 K1 43.70(12) . 2_556 ?
K1 Mo2 K1 93.44(4) 1_554 2_556 ?
O6 Mo3 O7 108.67(19) . . ?
O6 Mo3 O12 108.07(19) . . ?
O7 Mo3 O12 111.38(17) . . ?
O6 Mo3 O3 107.30(17) . . ?
O7 Mo3 O3 109.17(18) . . ?
O12 Mo3 O3 112.10(19) . . ?
O6 Mo3 K1 126.53(14) . 7_557 ?
O7 Mo3 K1 42.12(13) . 7_557 ?
O12 Mo3 K1 123.50(13) . 7_557 ?
O3 Mo3 K1 67.39(13) . 7_557 ?
O16 Mo4 O14 107.9(2) . . ?
O16 Mo4 O4 105.03(19) . . ?
O14 Mo4 O4 111.77(19) . . ?
O16 Mo4 O1 109.3(2) . . ?
O14 Mo4 O1 112.75(19) . . ?
O4 Mo4 O1 109.74(18) . . ?
O16 Mo4 K1 90.43(16) . . ?
O14 Mo4 K1 159.28(15) . . ?
O4 Mo4 K1 71.11(13) . . ?
O1 Mo4 K1 49.92(12) . . ?
O16 Mo4 K1 61.93(16) . 7_557 ?
O14 Mo4 K1 110.21(15) . 7_557 ?
O4 Mo4 K1 45.64(12) . 7_557 ?
O1 Mo4 K1 136.53(12) . 7_557 ?
K1 Mo4 K1 86.69(4) . 7_557 ?
O7 K1 O4 111.52(12) 7_557 7_557 ?
O7 K1 O5 91.65(12) 7_557 2_556 ?
O4 K1 O5 155.62(13) 7_557 2_556 ?
O7 K1 O1 123.82(12) 7_557 . ?
O4 K1 O1 107.51(12) 7_557 . ?
O5 K1 O1 62.03(11) 2_556 . ?
O7 K1 O2 58.86(10) 7_557 1_556 ?
O4 K1 O2 88.33(11) 7_557 1_556 ?
O5 K1 O2 97.87(11) 2_556 1_556 ?
O1 K1 O2 158.92(12) . 1_556 ?
O7 K1 O13 109.70(11) 7_557 1_556 ?
O4 K1 O13 55.21(11) 7_557 1_556 ?
O5 K1 O13 110.91(12) 2_556 1_556 ?
O1 K1 O13 125.62(12) . 1_556 ?
O2 K1 O13 52.76(10) 1_556 1_556 ?
O7 K1 O16 62.62(12) 7_557 7_557 ?
O4 K1 O16 53.38(11) 7_557 7_557 ?
O5 K1 O16 150.82(12) 2_556 7_557 ?
O1 K1 O16 119.50(12) . 7_557 ?
O2 K1 O16 81.01(12) 1_556 7_557 ?
O13 K1 O16 91.75(11) 1_556 7_557 ?
O7 K1 O9 162.46(10) 7_557 . ?
O4 K1 O9 58.32(10) 7_557 . ?
O5 K1 O9 97.33(11) 2_556 . ?
O1 K1 O9 73.71(10) . . ?
O2 K1 O9 104.79(10) 1_556 . ?
O13 K1 O9 52.97(9) 1_556 . ?
O16 K1 O9 111.22(11) 7_557 . ?
O7 K1 Mo4 125.46(9) 7_557 . ?
O4 K1 Mo4 82.52(9) 7_557 . ?
O5 K1 Mo4 90.25(8) 2_556 . ?
O1 K1 Mo4 28.32(8) . . ?
O2 K1 Mo4 170.83(9) 1_556 . ?
O13 K1 Mo4 120.18(8) 1_556 . ?
O16 K1 Mo4 93.97(9) 7_557 . ?
O9 K1 Mo4 69.75(7) . . ?
O7 K1 Mo4 84.88(9) 7_557 7_557 ?
O4 K1 Mo4 27.24(8) 7_557 7_557 ?
O5 K1 Mo4 176.05(9) 2_556 7_557 ?
O1 K1 Mo4 121.59(9) . 7_557 ?
O2 K1 Mo4 78.71(8) 1_556 7_557 ?
O13 K1 Mo4 68.66(8) 1_556 7_557 ?
O16 K1 Mo4 27.13(7) 7_557 7_557 ?
O9 K1 Mo4 85.52(7) . 7_557 ?
Mo4 K1 Mo4 93.31(4) . 7_557 ?
O7 K1 Mo3 25.16(8) 7_557 7_557 ?
O4 K1 Mo3 105.30(9) 7_557 7_557 ?
O5 K1 Mo3 98.93(9) 2_556 7_557 ?
O1 K1 Mo3 106.27(9) . 7_557 ?
O2 K1 Mo3 81.92(8) 1_556 7_557 ?
O13 K1 Mo3 127.52(8) 1_556 7_557 ?
O16 K1 Mo3 51.93(8) 7_557 7_557 ?
O9 K1 Mo3 161.37(8) . 7_557 ?
Mo4 K1 Mo3 101.10(4) . 7_557 ?
Mo4 K1 Mo3 78.71(3) 7_557 7_557 ?
O7 K1 Mo2 83.50(8) 7_557 1_556 ?
O4 K1 Mo2 69.52(8) 7_557 1_556 ?
O5 K1 Mo2 107.38(9) 2_556 1_556 ?
O1 K1 Mo2 149.04(10) . 1_556 ?
O2 K1 Mo2 26.07(7) 1_556 1_556 ?
O13 K1 Mo2 26.77(7) 1_556 1_556 ?
O16 K1 Mo2 84.41(8) 7_557 1_556 ?
O9 K1 Mo2 79.46(7) . 1_556 ?
Mo4 K1 Mo2 146.28(5) . 1_556 ?
Mo4 K1 Mo2 70.37(3) 7_557 1_556 ?
Mo3 K1 Mo2 104.10(4) 7_557 1_556 ?
O6 Mg1 O6 95.4(2) 6 5_657 ?
O6 Mg1 O7 88.79(15) 6 2_656 ?
O6 Mg1 O7 93.37(16) 5_657 2_656 ?
O6 Mg1 O7 93.36(16) 6 . ?
O6 Mg1 O7 88.79(15) 5_657 . ?
O7 Mg1 O7 176.8(2) 2_656 . ?
O6 Mg1 O2 90.64(16) 6 7_556 ?
O6 Mg1 O2 173.19(17) 5_657 7_556 ?
O7 Mg1 O2 89.91(16) 2_656 7_556 ?
O7 Mg1 O2 87.71(16) . 7_556 ?
O6 Mg1 O2 173.19(17) 6 8_556 ?
O6 Mg1 O2 90.64(16) 5_657 8_556 ?
O7 Mg1 O2 87.71(16) 2_656 8_556 ?
O7 Mg1 O2 89.91(16) . 8_556 ?
O2 Mg1 O2 83.5(2) 7_556 8_556 ?
O6 Mg1 K1 114.67(12) 6 7_557 ?
O6 Mg1 K1 121.17(11) 5_657 7_557 ?
O7 Mg1 K1 133.78(14) 2_656 7_557 ?
O7 Mg1 K1 43.06(11) . 7_557 ?
O2 Mg1 K1 52.95(11) 7_556 7_557 ?
O2 Mg1 K1 64.30(13) 8_556 7_557 ?
O6 Mg1 K1 121.17(11) 6 8 ?
O6 Mg1 K1 114.67(12) 5_657 8 ?
O7 Mg1 K1 43.06(11) 2_656 8 ?
O7 Mg1 K1 133.78(14) . 8 ?
O2 Mg1 K1 64.30(13) 7_556 8 ?
O2 Mg1 K1 52.95(11) 8_556 8 ?
K1 Mg1 K1 92.01(7) 7_557 8 ?
Mo4 O1 Th1 148.6(2) . . ?
Mo4 O1 K1 101.76(16) . . ?
Th1 O1 K1 108.69(13) . . ?
Mo2 O2 Mg1 163.9(2) . 7_556 ?
Mo2 O2 K1 101.24(17) . 1_554 ?
Mg1 O2 K1 94.54(12) 7_556 1_554 ?
Mo3 O3 Th2 158.8(2) . . ?
Mo4 O4 Th2 129.64(17) . 7_557 ?
Mo4 O4 K1 107.12(17) . 7_557 ?
Th2 O4 K1 113.64(15) 7_557 7_557 ?
Mo2 O5 Th1 138.0(2) . . ?
Mo2 O5 K1 110.80(15) . 2_556 ?
Th1 O5 K1 110.38(14) . 2_556 ?
Mo3 O6 Mg1 166.0(3) . 5_657 ?
Mo3 O7 Mg1 141.5(2) . . ?
Mo3 O7 K1 112.72(17) . 7_557 ?
Mg1 O7 K1 105.75(16) . 7_557 ?
Mo1 O8 Th1 147.1(2) . . ?
Mo1 O9 Th2 152.5(2) . . ?
Mo1 O9 K1 108.01(16) . . ?
Th2 O9 K1 96.90(12) . . ?
Mo1 O10 Th2 155.5(2) . 6 ?
Mo2 O11 Th2 157.3(2) . 7_557 ?
Mo3 O12 Th2 176.9(2) . 6 ?
Mo2 O13 Th2 143.7(2) . 1_554 ?
Mo2 O13 K1 98.76(16) . 1_554 ?
Th2 O13 K1 99.70(13) 1_554 1_554 ?
Mo4 O14 Th2 175.6(3) . 1_554 ?
Mo1 O15 Th1 156.1(2) . 5_557 ?
Mo4 O16 K1 90.94(17) . 7_557 ?

_diffrn_measured_fraction_theta_max 0.974
_diffrn_reflns_theta_full        26.37
_diffrn_measured_fraction_theta_full 0.974
_refine_diff_density_max         1.181
_refine_diff_density_min         -0.860
_refine_diff_density_rms         0.197
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_K2SrTh2Mo6O24
_database_code_depnum_ccdc_archive 'CCDC 1430750'
_audit_update_record             
;
2015-10-12 deposited with the CCDC.
2015-11-12 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        K2SrTh2(MoO4)6
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         K2SrTh2Mo6O24
_chemical_formula_sum            'K2 Mo6 O24 Sr Th2'
_chemical_formula_Weight         1589.52

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Th Th -7.2400 8.8979 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   8.0197(10)
_cell_length_b                   8.4470(17)
_cell_length_c                   16.030(2)
_cell_angle_alpha                101.550(15)
_cell_angle_beta                 102.893(12)
_cell_angle_gamma                97.388(13)
_cell_volume                     1019.9(3)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    1015
_cell_measurement_theta_min      3.2464
_cell_measurement_theta_max      30.5850

_exptl_crystal_description       
;
 ?
;
_exptl_crystal_colour            
;
 ?
;
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.09
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    5.176
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1404
_exptl_absorpt_coefficient_mu    21.315
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.12627
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   
;
 ?
;

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_Wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Eos'
_diffrn_measurement_method       '\Mo scans'
_diffrn_detector_area_resol_mean 15.9834
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            4424
_diffrn_reflns_av_R_equivalents  0.0455
_diffrn_reflns_av_sigmaI/netI    0.1132
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         3.25
_diffrn_reflns_theta_max         26.37
_reflns_number_total             4189
_reflns_number_gt                2656
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       
;
 ?
;
_computing_cell_refinement       
;
 ?
;
_computing_data_reduction        
;
 ?
;
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The Moeighted R-factor MoR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, Moith F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about tMoice as large as those based on F, and R-
 factors based on ALL data Moill be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_Moeighting_scheme     calc
_refine_ls_Moeighting_details    
'calc Mo=1/[σ²(Fo²)+(0.0591P)²+0.0000P] Mohere P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    .
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         3789
_refine_ls_number_parameters     316
_refine_ls_number_restraints     144
_refine_ls_R_factor_all          0.0893
_refine_ls_R_factor_gt           0.0526
_refine_ls_WR_factor_ref         0.1300
_refine_ls_WR_factor_gt          0.1129
_refine_ls_goodness_of_fit_ref   1.027
_refine_ls_restrained_S_all      1.006
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Th1 Th 0.30732(14) 0.30430(14) 0.50391(7) 0.0109(3) Uani 1 1 d . . .
Th2 Th 0.07471(14) 0.00516(14) 0.16407(7) 0.0096(3) Uani 1 1 d . . .
Mo1 Mo 0.52995(15) 0.00066(15) 0.34343(8) 0.0083(3) Uani 1 1 d . . .
Mo2 Mo -0.08758(15) -0.05415(15) 0.34733(8) 0.0084(3) Uani 1 1 d . . .
Mo3 Mo -0.14091(15) 0.32176(15) 0.33570(8) 0.0091(3) Uani 1 1 d . . .
Mo4 Mo 0.46295(15) 0.37230(15) 0.31897(8) 0.0092(3) Uani 1 1 d . . .
Mo5 Mo 0.61571(16) -0.16765(15) -0.01054(8) 0.0108(3) Uani 1 1 d . . .
Mo6 Mo 0.22226(15) -0.23380(16) -0.00449(8) 0.0111(3) Uani 1 1 d . . .
O1 O -0.280(3) 0.442(3) 0.4022(13) 0.013(5) Uani 1 1 d U . .
O2 O 0.595(3) 0.212(3) 0.2722(14) 0.015(5) Uani 1 1 d U . .
O3 O 0.658(3) -0.104(2) 0.2699(13) 0.011(4) Uani 1 1 d U . .
O4 O -0.085(2) 0.130(2) 0.2718(12) 0.007(4) Uani 1 1 d U . .
O5 O 0.515(3) -0.133(2) 0.4139(13) 0.012(5) Uani 1 1 d U . .
O6 O -0.027(3) -0.173(2) 0.2574(13) 0.010(4) Uani 1 1 d U . .
O7 O 0.129(2) -0.255(2) 0.0872(12) 0.004(4) Uani 1 1 d U . .
O8 O 0.407(2) 0.495(2) 0.4187(13) 0.009(4) Uani 1 1 d U . .
O9 O 0.119(2) 0.056(2) 0.4150(12) 0.008(4) Uani 1 1 d U . .
O10 O 0.044(3) -0.178(2) -0.0778(12) 0.008(4) Uani 1 1 d U . .
O11 O 0.487(3) 0.529(3) 0.2638(14) 0.015(5) Uani 1 1 d U . .
O12 O -0.206(2) 0.122(2) 0.4029(13) 0.007(4) Uani 1 1 d U . .
O13 O 0.465(2) 0.196(2) 0.4059(12) 0.004(4) Uani 1 1 d U . .
O14 O 0.388(3) -0.113(3) -0.0635(13) 0.015(5) Uani 1 1 d U . .
O15 O -0.139(3) -0.209(3) 0.4032(13) 0.013(5) Uani 1 1 d U . .
O16 O 0.792(3) -0.145(3) 0.0847(15) 0.022(5) Uani 1 1 d U . .
O17 O 0.195(3) -0.437(2) -0.0581(13) 0.011(4) Uani 1 1 d U . .
O18 O -0.102(3) 0.449(3) 0.2657(15) 0.020(5) Uani 1 1 d U . .
O19 O 0.252(3) 0.261(3) 0.2552(14) 0.014(5) Uani 1 1 d U . .
O20 O 0.467(3) -0.213(3) 0.0675(14) 0.020(5) Uani 1 1 d U . .
O21 O 0.336(2) -0.055(2) 0.2598(12) 0.007(4) Uani 1 1 d U . .
O22 O 0.599(3) -0.371(3) -0.0755(15) 0.024(6) Uani 1 1 d U . .
O23 O 0.722(2) -0.037(2) -0.0736(12) 0.008(4) Uani 1 1 d U . .
O24 O 0.057(3) 0.375(3) 0.4256(15) 0.022(5) Uani 1 1 d U . .
Sr1 Sr -0.3335(7) -0.3842(7) 0.1608(4) 0.0652(15) Uani 1 1 d . . .
K1 K 0.1924(10) -0.2872(10) 0.4337(5) 0.0270(18) Uani 1 1 d . . .
K2 K -0.1465(11) -0.5025(10) -0.1598(6) 0.032(2) Uani 1 1 d . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle betMoeen tMoo l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations betMoeen esds in cell parameters are only
 used Mohen they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Th1 O24 2.34(2) . ?
Th1 O13 2.351(19) . ?
Th1 O9 2.393(18) . ?
Th1 O15 2.41(2) 2_556 ?
Th1 O1 2.42(2) 2_566 ?
Th1 O8 2.48(2) . ?
Th1 O5 2.51(2) 2_656 ?
Th1 O8 2.557(19) 2_666 ?
Th1 Mo4 3.4906(18) 2_666 ?
Th1 Mo4 3.5812(18) . ?
Th1 K1 3.941(8) 2_656 ?
Th1 K1 3.992(8) 1_565 ?
Th2 O10 2.35(2) 2 ?
Th2 O16 2.39(2) 1_455 ?
Th2 O19 2.42(2) . ?
Th2 O23 2.43(2) 2_655 ?
Th2 O7 2.439(18) . ?
Th2 O21 2.482(19) . ?
Th2 O6 2.51(2) . ?
Th2 O4 2.518(19) . ?
Th2 Mo6 3.5543(17) . ?
Th2 Mo2 3.5641(17) . ?
Th2 K2 4.183(8) 2 ?
Th2 Sr1 4.316(6) . ?
Mo1 O21 1.749(18) . ?
Mo1 O5 1.76(2) . ?
Mo1 O3 1.89(2) . ?
Mo1 O13 1.943(18) . ?
Mo1 O12 2.145(19) 1_655 ?
Mo1 O2 2.37(2) . ?
Mo1 Mo2 3.1493(17) 1_655 ?
Mo1 K1 3.896(8) 2_656 ?
Mo1 K1 4.099(8) . ?
Mo2 O15 1.78(2) . ?
Mo2 O6 1.79(2) . ?
Mo2 O9 1.786(18) . ?
Mo2 O12 2.029(19) . ?
Mo2 O3 2.078(19) 1_455 ?
Mo2 O4 2.15(2) . ?
Mo2 Mo1 3.1492(17) 1_455 ?
Mo2 K1 3.417(8) . ?
Mo2 Sr1 3.635(6) . ?
Mo3 O18 1.75(2) . ?
Mo3 O24 1.82(2) . ?
Mo3 O4 1.898(19) . ?
Mo3 O1 1.95(2) . ?
Mo3 O2 2.13(2) 1_455 ?
Mo3 O12 2.24(2) . ?
Mo3 Mo4 3.2189(17) 1_455 ?
Mo3 K1 3.782(8) 1_565 ?
Mo3 K1 3.873(8) 2_556 ?
Mo4 O11 1.75(2) . ?
Mo4 O19 1.80(2) . ?
Mo4 O8 1.897(19) . ?
Mo4 O2 1.96(2) . ?
Mo4 O1 2.13(2) 1_655 ?
Mo4 O13 2.234(19) . ?
Mo4 Mo3 3.2189(17) 1_655 ?
Mo4 Th1 3.4905(18) 2_666 ?
Mo4 K2 3.621(8) 2 ?
Mo5 O22 1.79(2) . ?
Mo5 O16 1.79(2) . ?
Mo5 O23 1.89(2) . ?
Mo5 O20 1.97(2) . ?
Mo5 O14 1.99(2) . ?
Mo5 O14 2.44(2) 2_655 ?
Mo5 Mo6 3.1595(17) . ?
Mo5 Sr1 3.573(6) 1_655 ?
Mo6 O17 1.721(19) . ?
Mo6 O10 1.814(19) . ?
Mo6 O7 1.823(19) . ?
Mo6 O20 2.01(2) . ?
Mo6 O14 2.08(2) . ?
Mo6 O23 2.313(18) 2_655 ?
Mo6 K2 3.581(8) . ?
Mo6 K2 3.871(9) 2_545 ?
Mo6 Sr1 3.998(6) 2_545 ?
O1 Mo4 2.13(2) 1_455 ?
O1 Th1 2.42(2) 2_566 ?
O1 K1 3.15(2) 2_556 ?
O2 Mo3 2.13(2) 1_655 ?
O3 Mo2 2.078(19) 1_655 ?
O3 Sr1 2.66(2) 1_655 ?
O5 Th1 2.51(2) 2_656 ?
O5 K1 2.86(2) . ?
O6 Sr1 2.77(2) . ?
O6 K1 3.36(2) . ?
O7 K2 2.55(2) 2_545 ?
O8 Th1 2.557(18) 2_666 ?
O8 K1 2.69(2) 1_565 ?
O9 K1 3.09(2) . ?
O10 Th2 2.35(2) 2 ?
O10 K2 2.85(2) . ?
O11 Sr1 2.57(2) 1_665 ?
O11 K2 2.82(2) 2 ?
O12 Mo1 2.145(18) 1_455 ?
O12 K1 2.68(2) 2_556 ?
O13 K1 3.201(19) 2_656 ?
O14 Mo5 2.44(2) 2_655 ?
O15 Th1 2.41(2) 2_556 ?
O15 K1 2.78(2) . ?
O16 Th2 2.39(2) 1_655 ?
O16 Sr1 2.76(2) 1_655 ?
O17 Sr1 2.54(2) 2_545 ?
O17 K2 2.78(2) . ?
O18 Sr1 2.92(2) 1_565 ?
O18 K2 2.94(3) 2 ?
O18 K1 3.35(2) 1_565 ?
O19 K2 2.88(2) 2 ?
O20 Sr1 2.70(2) 1_655 ?
O22 Sr1 2.67(2) 2_545 ?
O22 K2 2.91(3) 1_655 ?
O23 Mo6 2.313(18) 2_655 ?
O23 Th2 2.43(2) 2_655 ?
O24 K1 2.88(2) 1_565 ?
Sr1 O17 2.54(2) 2_545 ?
Sr1 O11 2.57(2) 1_445 ?
Sr1 O3 2.66(2) 1_455 ?
Sr1 O22 2.67(2) 2_545 ?
Sr1 O20 2.70(2) 1_455 ?
Sr1 O16 2.76(2) 1_455 ?
Sr1 O18 2.92(2) 1_545 ?
Sr1 Mo5 3.573(6) 1_455 ?
Sr1 Mo6 3.998(6) 2_545 ?
Sr1 K2 4.087(10) 2_545 ?
K1 O12 2.68(2) 2_556 ?
K1 O8 2.69(2) 1_545 ?
K1 O24 2.88(2) 1_545 ?
K1 O1 3.15(2) 2_556 ?
K1 O13 3.201(19) 2_656 ?
K1 O18 3.35(2) 1_545 ?
K1 Mo3 3.782(8) 1_545 ?
K2 O7 2.55(2) 2_545 ?
K2 O11 2.82(2) 2 ?
K2 O19 2.88(2) 2 ?
K2 O22 2.91(3) 1_455 ?
K2 O18 2.94(3) 2 ?
K2 Mo4 3.621(8) 2 ?
K2 Mo6 3.871(9) 2_545 ?
K2 Sr1 4.087(10) 2_545 ?
K2 Sr1 4.153(10) 2_445 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O24 Th1 O13 109.7(7) . . ?
O24 Th1 O9 72.0(7) . . ?
O13 Th1 O9 76.0(6) . . ?
O24 Th1 O15 88.3(8) . 2_556 ?
O13 Th1 O15 138.2(7) . 2_556 ?
O9 Th1 O15 74.4(7) . 2_556 ?
O24 Th1 O1 76.0(7) . 2_566 ?
O13 Th1 O1 142.7(7) . 2_566 ?
O9 Th1 O1 137.3(7) . 2_566 ?
O15 Th1 O1 77.2(7) 2_556 2_566 ?
O24 Th1 O8 73.9(7) . . ?
O13 Th1 O8 65.2(6) . . ?
O9 Th1 O8 114.1(6) . . ?
O15 Th1 O8 155.6(7) 2_556 . ?
O1 Th1 O8 82.3(7) 2_566 . ?
O24 Th1 O5 156.8(7) . 2_656 ?
O13 Th1 O5 76.5(7) . 2_656 ?
O9 Th1 O5 88.6(6) . 2_656 ?
O15 Th1 O5 74.0(7) 2_556 2_656 ?
O1 Th1 O5 113.2(7) 2_566 2_656 ?
O8 Th1 O5 127.1(7) . 2_656 ?
O24 Th1 O8 124.7(7) . 2_666 ?
O13 Th1 O8 84.2(6) . 2_666 ?
O9 Th1 O8 158.1(6) . 2_666 ?
O15 Th1 O8 116.7(6) 2_556 2_666 ?
O1 Th1 O8 64.6(7) 2_566 2_666 ?
O8 Th1 O8 64.2(7) . 2_666 ?
O5 Th1 O8 77.5(6) 2_656 2_666 ?
O24 Th1 Mo4 111.1(5) . 2_666 ?
O13 Th1 Mo4 116.3(4) . 2_666 ?
O9 Th1 Mo4 163.5(5) . 2_666 ?
O15 Th1 Mo4 89.4(5) 2_556 2_666 ?
O1 Th1 Mo4 36.9(5) 2_566 2_666 ?
O8 Th1 Mo4 81.9(4) . 2_666 ?
O5 Th1 Mo4 84.0(4) 2_656 2_666 ?
O8 Th1 Mo4 32.1(4) 2_666 2_666 ?
O24 Th1 Mo4 82.2(6) . . ?
O13 Th1 Mo4 37.5(5) . . ?
O9 Th1 Mo4 90.6(5) . . ?
O15 Th1 Mo4 164.2(5) 2_556 . ?
O1 Th1 Mo4 112.4(5) 2_566 . ?
O8 Th1 Mo4 30.0(4) . . ?
O5 Th1 Mo4 111.3(5) 2_656 . ?
O8 Th1 Mo4 79.0(5) 2_666 . ?
Mo4 Th1 Mo4 105.79(4) 2_666 . ?
O24 Th1 K1 154.8(6) . 2_656 ?
O13 Th1 K1 54.3(4) . 2_656 ?
O9 Th1 K1 116.0(5) . 2_656 ?
O15 Th1 K1 116.6(5) 2_556 2_656 ?
O1 Th1 K1 105.0(5) 2_566 2_656 ?
O8 Th1 K1 81.2(5) . 2_656 ?
O5 Th1 K1 46.3(5) 2_656 2_656 ?
O8 Th1 K1 42.6(5) 2_666 2_656 ?
Mo4 Th1 K1 68.49(12) 2_666 2_656 ?
Mo4 Th1 K1 74.12(13) . 2_656 ?
O24 Th1 K1 45.5(6) . 1_565 ?
O13 Th1 K1 104.6(5) . 1_565 ?
O9 Th1 K1 114.5(5) . 1_565 ?
O15 Th1 K1 114.3(5) 2_556 1_565 ?
O1 Th1 K1 52.1(5) 2_566 1_565 ?
O8 Th1 K1 41.4(5) . 1_565 ?
O5 Th1 K1 156.6(5) 2_656 1_565 ?
O8 Th1 K1 79.4(5) 2_666 1_565 ?
Mo4 Th1 K1 74.43(12) 2_666 1_565 ?
Mo4 Th1 K1 67.10(12) . 1_565 ?
K1 Th1 K1 114.92(13) 2_656 1_565 ?
O10 Th2 O16 75.8(7) 2 1_455 ?
O10 Th2 O19 82.8(7) 2 . ?
O16 Th2 O19 148.0(8) 1_455 . ?
O10 Th2 O23 77.1(7) 2 2_655 ?
O16 Th2 O23 114.6(7) 1_455 2_655 ?
O19 Th2 O23 82.7(7) . 2_655 ?
O10 Th2 O7 117.6(6) 2 . ?
O16 Th2 O7 75.7(7) 1_455 . ?
O19 Th2 O7 136.0(7) . . ?
O23 Th2 O7 66.6(6) 2_655 . ?
O10 Th2 O21 147.6(6) 2 . ?
O16 Th2 O21 135.7(7) 1_455 . ?
O19 Th2 O21 71.1(7) . . ?
O23 Th2 O21 80.7(6) 2_655 . ?
O7 Th2 O21 73.3(6) . . ?
O10 Th2 O6 137.0(7) 2 . ?
O16 Th2 O6 72.4(7) 1_455 . ?
O19 Th2 O6 110.7(7) . . ?
O23 Th2 O6 143.1(7) 2_655 . ?
O7 Th2 O6 81.6(6) . . ?
O21 Th2 O6 72.3(6) . . ?
O10 Th2 O4 85.2(7) 2 . ?
O16 Th2 O4 83.4(7) 1_455 . ?
O19 Th2 O4 71.2(7) . . ?
O23 Th2 O4 150.0(6) 2_655 . ?
O7 Th2 O4 143.3(6) . . ?
O21 Th2 O4 103.5(6) . . ?
O6 Th2 O4 63.2(6) . . ?
O10 Th2 Mo6 95.4(5) 2 . ?
O16 Th2 Mo6 85.3(6) 1_455 . ?
O19 Th2 Mo6 120.5(5) . . ?
O23 Th2 Mo6 40.2(4) 2_655 . ?
O7 Th2 Mo6 28.3(4) . . ?
O21 Th2 Mo6 82.2(4) . . ?
O6 Th2 Mo6 109.9(5) . . ?
O4 Th2 Mo6 168.3(4) . . ?
O10 Th2 Mo2 119.7(5) 2 . ?
O16 Th2 Mo2 81.7(6) 1_455 . ?
O19 Th2 Mo2 88.8(5) . . ?
O23 Th2 Mo2 160.1(4) 2_655 . ?
O7 Th2 Mo2 109.4(4) . . ?
O21 Th2 Mo2 79.6(5) . . ?
O6 Th2 Mo2 27.9(5) . . ?
O4 Th2 Mo2 36.7(4) . . ?
Mo6 Th2 Mo2 137.72(5) . . ?
O10 Th2 K2 40.8(5) 2 2 ?
O16 Th2 K2 113.9(6) 1_455 2 ?
O19 Th2 K2 42.0(5) . 2 ?
O23 Th2 K2 74.5(5) 2_655 2 ?
O7 Th2 K2 140.0(5) . 2 ?
O21 Th2 K2 110.2(4) . 2 ?
O6 Th2 K2 138.2(5) . 2 ?
O4 Th2 K2 76.2(5) . 2 ?
Mo6 Th2 K2 111.69(14) . 2 ?
Mo2 Th2 K2 110.36(14) . 2 ?
O10 Th2 Sr1 109.2(5) 2 . ?
O16 Th2 Sr1 35.7(6) 1_455 . ?
O19 Th2 Sr1 142.3(5) . . ?
O23 Th2 Sr1 134.3(4) 2_655 . ?
O7 Th2 Sr1 71.1(4) . . ?
O21 Th2 Sr1 103.3(4) . . ?
O6 Th2 Sr1 37.3(4) . . ?
O4 Th2 Sr1 74.3(4) . . ?
Mo6 Th2 Sr1 94.50(8) . . ?
Mo2 Th2 Sr1 53.93(8) . . ?
K2 Th2 Sr1 139.52(14) 2 . ?
O21 Mo1 O5 106.6(9) . . ?
O21 Mo1 O3 92.8(9) . . ?
O5 Mo1 O3 101.6(9) . . ?
O21 Mo1 O13 94.8(8) . . ?
O5 Mo1 O13 102.0(9) . . ?
O3 Mo1 O13 152.0(8) . . ?
O21 Mo1 O12 154.5(8) . 1_655 ?
O5 Mo1 O12 98.1(8) . 1_655 ?
O3 Mo1 O12 75.7(8) . 1_655 ?
O13 Mo1 O12 86.1(7) . 1_655 ?
O21 Mo1 O2 84.4(8) . . ?
O5 Mo1 O2 168.6(8) . . ?
O3 Mo1 O2 80.5(8) . . ?
O13 Mo1 O2 73.5(8) . . ?
O12 Mo1 O2 71.5(7) 1_655 . ?
O21 Mo1 Mo2 132.4(6) . 1_655 ?
O5 Mo1 Mo2 89.8(7) . 1_655 ?
O3 Mo1 Mo2 39.6(6) . 1_655 ?
O13 Mo1 Mo2 125.7(5) . 1_655 ?
O12 Mo1 Mo2 39.6(5) 1_655 1_655 ?
O2 Mo1 Mo2 84.8(5) . 1_655 ?
O21 Mo1 K1 149.6(6) . 2_656 ?
O5 Mo1 K1 80.0(6) . 2_656 ?
O3 Mo1 K1 115.4(6) . 2_656 ?
O13 Mo1 K1 54.9(5) . 2_656 ?
O12 Mo1 K1 41.1(5) 1_655 2_656 ?
O2 Mo1 K1 89.0(5) . 2_656 ?
Mo2 Mo1 K1 76.16(12) 1_655 2_656 ?
O21 Mo1 K1 74.4(7) . . ?
O5 Mo1 K1 35.7(7) . . ?
O3 Mo1 K1 118.3(6) . . ?
O13 Mo1 K1 89.7(6) . . ?
O12 Mo1 K1 131.1(6) 1_655 . ?
O2 Mo1 K1 151.8(5) . . ?
Mo2 Mo1 K1 123.25(12) 1_655 . ?
K1 Mo1 K1 99.84(15) 2_656 . ?
O15 Mo2 O6 100.4(10) . . ?
O15 Mo2 O9 103.0(9) . . ?
O6 Mo2 O9 101.6(9) . . ?
O15 Mo2 O12 99.6(9) . . ?
O6 Mo2 O12 153.9(9) . . ?
O9 Mo2 O12 90.1(8) . . ?
O15 Mo2 O3 90.6(9) . 1_455 ?
O6 Mo2 O3 88.6(8) . 1_455 ?
O9 Mo2 O3 161.1(8) . 1_455 ?
O12 Mo2 O3 74.5(8) . 1_455 ?
O15 Mo2 O4 167.7(8) . . ?
O6 Mo2 O4 83.4(8) . . ?
O9 Mo2 O4 87.5(8) . . ?
O12 Mo2 O4 73.7(8) . . ?
O3 Mo2 O4 77.7(8) 1_455 . ?
O15 Mo2 Mo1 83.7(7) . 1_455 ?
O6 Mo2 Mo1 124.1(6) . 1_455 ?
O9 Mo2 Mo1 132.1(6) . 1_455 ?
O12 Mo2 Mo1 42.4(5) . 1_455 ?
O3 Mo2 Mo1 35.5(6) 1_455 1_455 ?
O4 Mo2 Mo1 84.5(5) . 1_455 ?
O15 Mo2 K1 54.2(7) . . ?
O6 Mo2 K1 73.1(7) . . ?
O9 Mo2 K1 64.3(6) . . ?
O12 Mo2 K1 132.8(6) . . ?
O3 Mo2 K1 134.5(6) 1_455 . ?
O4 Mo2 K1 137.7(5) . . ?
Mo1 Mo2 K1 137.78(15) 1_455 . ?
O15 Mo2 Th2 141.4(7) . . ?
O6 Mo2 Th2 41.1(7) . . ?
O9 Mo2 Th2 86.5(6) . . ?
O12 Mo2 Th2 117.9(6) . . ?
O3 Mo2 Th2 90.9(6) 1_455 . ?
O4 Mo2 Th2 44.2(5) . . ?
Mo1 Mo2 Th2 117.43(5) 1_455 . ?
K1 Mo2 Th2 100.28(14) . . ?
O15 Mo2 Sr1 79.9(6) . . ?
O6 Mo2 Sr1 47.8(6) . . ?
O9 Mo2 Sr1 148.5(6) . . ?
O12 Mo2 Sr1 120.6(5) . . ?
O3 Mo2 Sr1 46.3(6) 1_455 . ?
O4 Mo2 Sr1 94.5(5) . . ?
Mo1 Mo2 Sr1 79.27(10) 1_455 . ?
K1 Mo2 Sr1 94.95(17) . . ?
Th2 Mo2 Sr1 73.65(9) . . ?
O18 Mo3 O24 104.1(10) . . ?
O18 Mo3 O4 96.9(10) . . ?
O24 Mo3 O4 96.9(9) . . ?
O18 Mo3 O1 101.8(10) . . ?
O24 Mo3 O1 95.2(10) . . ?
O4 Mo3 O1 154.4(9) . . ?
O18 Mo3 O2 99.9(9) . 1_455 ?
O24 Mo3 O2 155.3(10) . 1_455 ?
O4 Mo3 O2 85.7(8) . 1_455 ?
O1 Mo3 O2 74.2(8) . 1_455 ?
O18 Mo3 O12 169.5(9) . . ?
O24 Mo3 O12 82.8(9) . . ?
O4 Mo3 O12 74.2(8) . . ?
O1 Mo3 O12 85.2(8) . . ?
O2 Mo3 O12 74.3(8) 1_455 . ?
O18 Mo3 Mo4 94.6(8) . 1_455 ?
O24 Mo3 Mo4 134.5(7) . 1_455 ?
O4 Mo3 Mo4 121.9(6) . 1_455 ?
O1 Mo3 Mo4 39.8(6) . 1_455 ?
O2 Mo3 Mo4 36.2(6) 1_455 1_455 ?
O12 Mo3 Mo4 85.8(5) . 1_455 ?
O18 Mo3 K1 62.2(7) . 1_565 ?
O24 Mo3 K1 47.5(7) . 1_565 ?
O4 Mo3 K1 121.6(6) . 1_565 ?
O1 Mo3 K1 82.9(6) . 1_565 ?
O2 Mo3 K1 147.4(6) 1_455 1_565 ?
O12 Mo3 K1 127.1(5) . 1_565 ?
Mo4 Mo3 K1 114.17(12) 1_455 1_565 ?
O18 Mo3 K1 148.0(7) . 2_556 ?
O24 Mo3 K1 63.1(8) . 2_556 ?
O4 Mo3 K1 113.2(6) . 2_556 ?
O1 Mo3 K1 54.0(6) . 2_556 ?
O2 Mo3 K1 93.2(6) 1_455 2_556 ?
O12 Mo3 K1 42.3(5) . 2_556 ?
Mo4 Mo3 K1 79.07(12) 1_455 2_556 ?
K1 Mo3 K1 91.56(18) 1_565 2_556 ?
O11 Mo4 O19 99.8(10) . . ?
O11 Mo4 O8 98.2(9) . . ?
O19 Mo4 O8 101.2(9) . . ?
O11 Mo4 O2 104.8(10) . . ?
O19 Mo4 O2 96.3(9) . . ?
O8 Mo4 O2 148.2(9) . . ?
O11 Mo4 O1 94.1(9) . 1_655 ?
O19 Mo4 O1 164.9(9) . 1_655 ?
O8 Mo4 O1 82.6(8) . 1_655 ?
O2 Mo4 O1 74.1(8) . 1_655 ?
O11 Mo4 O13 171.4(8) . . ?
O19 Mo4 O13 88.5(8) . . ?
O8 Mo4 O13 77.7(8) . . ?
O2 Mo4 O13 76.4(8) . . ?
O1 Mo4 O13 77.9(7) 1_655 . ?
O11 Mo4 Mo3 92.7(7) . 1_655 ?
O19 Mo4 Mo3 136.3(7) . 1_655 ?
O8 Mo4 Mo3 118.4(6) . 1_655 ?
O2 Mo4 Mo3 40.0(6) . 1_655 ?
O1 Mo4 Mo3 36.0(6) 1_655 1_655 ?
O13 Mo4 Mo3 82.9(5) . 1_655 ?
O11 Mo4 Th1 80.1(6) . 2_666 ?
O19 Mo4 Th1 145.7(7) . 2_666 ?
O8 Mo4 Th1 45.7(6) . 2_666 ?
O2 Mo4 Th1 117.1(6) . 2_666 ?
O1 Mo4 Th1 43.1(6) 1_655 2_666 ?
O13 Mo4 Th1 91.7(4) . 2_666 ?
Mo3 Mo4 Th1 77.63(4) 1_655 2_666 ?
O11 Mo4 Th1 138.1(7) . . ?
O19 Mo4 Th1 84.5(7) . . ?
O8 Mo4 Th1 40.8(6) . . ?
O2 Mo4 Th1 116.2(6) . . ?
O1 Mo4 Th1 89.3(6) 1_655 . ?
O13 Mo4 Th1 39.8(5) . . ?
Mo3 Mo4 Th1 112.98(4) 1_655 . ?
Th1 Mo4 Th1 74.21(4) 2_666 . ?
O11 Mo4 K2 49.4(7) . 2 ?
O19 Mo4 K2 51.9(7) . 2 ?
O8 Mo4 K2 94.8(6) . 2 ?
O2 Mo4 K2 116.9(6) . 2 ?
O1 Mo4 K2 142.9(6) 1_655 2 ?
O13 Mo4 K2 137.9(5) . 2 ?
Mo3 Mo4 K2 134.18(16) 1_655 2 ?
Th1 Mo4 K2 112.60(14) 2_666 2 ?
Th1 Mo4 K2 112.75(16) . 2 ?
O22 Mo5 O16 105.4(10) . . ?
O22 Mo5 O23 101.9(10) . . ?
O16 Mo5 O23 100.4(9) . . ?
O22 Mo5 O20 100.5(10) . . ?
O16 Mo5 O20 84.7(10) . . ?
O23 Mo5 O20 154.7(9) . . ?
O22 Mo5 O14 101.4(9) . . ?
O16 Mo5 O14 148.8(10) . . ?
O23 Mo5 O14 89.3(8) . . ?
O20 Mo5 O14 74.8(9) . . ?
O22 Mo5 O14 173.2(9) . 2_655 ?
O16 Mo5 O14 81.4(9) . 2_655 ?
O23 Mo5 O14 76.1(8) . 2_655 ?
O20 Mo5 O14 80.3(8) . 2_655 ?
O14 Mo5 O14 72.2(8) . 2_655 ?
O22 Mo5 Mo6 92.4(8) . . ?
O16 Mo5 Mo6 122.3(8) . . ?
O23 Mo5 Mo6 129.3(6) . . ?
O20 Mo5 Mo6 37.8(6) . . ?
O14 Mo5 Mo6 40.0(6) . . ?
O14 Mo5 Mo6 84.2(5) 2_655 . ?
O22 Mo5 Sr1 80.8(8) . 1_655 ?
O16 Mo5 Sr1 49.2(7) . 1_655 ?
O23 Mo5 Sr1 147.9(6) . 1_655 ?
O20 Mo5 Sr1 48.4(7) . 1_655 ?
O14 Mo5 Sr1 121.9(6) . 1_655 ?
O14 Mo5 Sr1 104.5(5) 2_655 1_655 ?
Mo6 Mo5 Sr1 82.07(10) . 1_655 ?
O17 Mo6 O10 98.2(9) . . ?
O17 Mo6 O7 100.2(9) . . ?
O10 Mo6 O7 101.1(9) . . ?
O17 Mo6 O20 97.0(9) . . ?
O10 Mo6 O20 156.9(9) . . ?
O7 Mo6 O20 93.2(9) . . ?
O17 Mo6 O14 103.7(9) . . ?
O10 Mo6 O14 87.5(9) . . ?
O7 Mo6 O14 153.2(8) . . ?
O20 Mo6 O14 72.1(9) . . ?
O17 Mo6 O23 175.8(8) . 2_655 ?
O10 Mo6 O23 85.9(8) . 2_655 ?
O7 Mo6 O23 79.7(7) . 2_655 ?
O20 Mo6 O23 78.9(8) . 2_655 ?
O14 Mo6 O23 75.6(8) . 2_655 ?
O17 Mo6 Mo5 91.9(7) . . ?
O10 Mo6 Mo5 125.1(6) . . ?
O7 Mo6 Mo5 130.0(6) . . ?
O20 Mo6 Mo5 37.0(7) . . ?
O14 Mo6 Mo5 37.9(6) . . ?
O23 Mo6 Mo5 85.1(5) 2_655 . ?
O17 Mo6 Th2 138.2(7) . . ?
O10 Mo6 Th2 83.9(6) . . ?
O7 Mo6 Th2 39.4(6) . . ?
O20 Mo6 Th2 96.2(6) . . ?
O14 Mo6 Th2 118.2(6) . . ?
O23 Mo6 Th2 42.8(5) 2_655 . ?
Mo5 Mo6 Th2 121.05(5) . . ?
O17 Mo6 K2 49.3(7) . . ?
O10 Mo6 K2 52.1(6) . . ?
O7 Mo6 K2 91.6(6) . . ?
O20 Mo6 K2 146.2(6) . . ?
O14 Mo6 K2 113.2(6) . . ?
O23 Mo6 K2 134.9(5) 2_655 . ?
Mo5 Mo6 K2 130.19(16) . . ?
Th2 Mo6 K2 108.46(16) . . ?
O17 Mo6 K2 72.3(7) . 2_545 ?
O10 Mo6 K2 122.1(6) . 2_545 ?
O7 Mo6 K2 33.3(6) . 2_545 ?
O20 Mo6 K2 79.2(7) . 2_545 ?
O14 Mo6 K2 150.4(6) . 2_545 ?
O23 Mo6 K2 106.3(5) 2_655 2_545 ?
Mo5 Mo6 K2 112.48(13) . 2_545 ?
Th2 Mo6 K2 71.52(14) . 2_545 ?
K2 Mo6 K2 86.88(19) . 2_545 ?
O17 Mo6 Sr1 24.9(7) . 2_545 ?
O10 Mo6 Sr1 102.6(6) . 2_545 ?
O7 Mo6 Sr1 122.4(6) . 2_545 ?
O20 Mo6 Sr1 84.4(6) . 2_545 ?
O14 Mo6 Sr1 79.4(6) . 2_545 ?
O23 Mo6 Sr1 153.2(5) 2_655 2_545 ?
Mo5 Mo6 Sr1 69.13(9) . 2_545 ?
Th2 Mo6 Sr1 161.84(9) . 2_545 ?
K2 Mo6 Sr1 64.98(17) . 2_545 ?
K2 Mo6 Sr1 90.86(16) 2_545 2_545 ?
Mo3 O1 Mo4 104.2(9) . 1_455 ?
Mo3 O1 Th1 148.5(10) . 2_566 ?
Mo4 O1 Th1 100.0(8) 1_455 2_566 ?
Mo3 O1 K1 95.9(8) . 2_556 ?
Mo4 O1 K1 117.5(8) 1_455 2_556 ?
Th1 O1 K1 90.5(6) 2_566 2_556 ?
Mo4 O2 Mo3 103.8(9) . 1_655 ?
Mo4 O2 Mo1 100.5(9) . . ?
Mo3 O2 Mo1 105.1(9) 1_655 . ?
Mo1 O3 Mo2 104.8(9) . 1_655 ?
Mo1 O3 Sr1 144.3(10) . 1_655 ?
Mo2 O3 Sr1 99.4(8) 1_655 1_655 ?
Mo3 O4 Mo2 108.6(9) . . ?
Mo3 O4 Th2 148.3(10) . . ?
Mo2 O4 Th2 99.1(7) . . ?
Mo1 O5 Th1 141.1(11) . 2_656 ?
Mo1 O5 K1 123.3(10) . . ?
Th1 O5 K1 94.2(7) 2_656 . ?
Mo2 O6 Th2 111.0(9) . . ?
Mo2 O6 Sr1 103.7(9) . . ?
Th2 O6 Sr1 109.5(7) . . ?
Mo2 O6 K1 76.4(7) . . ?
Th2 O6 K1 131.1(7) . . ?
Sr1 O6 K1 115.5(7) . . ?
Mo6 O7 Th2 112.2(8) . . ?
Mo6 O7 K2 123.6(9) . 2_545 ?
Th2 O7 K2 121.1(8) . 2_545 ?
Mo4 O8 Th1 109.1(8) . . ?
Mo4 O8 Th1 102.2(8) . 2_666 ?
Th1 O8 Th1 115.8(7) . 2_666 ?
Mo4 O8 K1 131.7(10) . 1_565 ?
Th1 O8 K1 101.0(7) . 1_565 ?
Th1 O8 K1 97.3(6) 2_666 1_565 ?
Mo2 O9 Th1 151.7(10) . . ?
Mo2 O9 K1 84.4(7) . . ?
Th1 O9 K1 122.2(7) . . ?
Mo6 O10 Th2 152.3(10) . 2 ?
Mo6 O10 K2 97.7(8) . . ?
Th2 O10 K2 106.5(7) 2 . ?
Mo4 O11 Sr1 138.4(11) . 1_665 ?
Mo4 O11 K2 102.5(9) . 2 ?
Sr1 O11 K2 100.7(7) 1_665 2 ?
Mo2 O12 Mo1 97.9(8) . 1_455 ?
Mo2 O12 Mo3 100.8(8) . . ?
Mo1 O12 Mo3 109.1(8) 1_455 . ?
Mo2 O12 K1 136.7(9) . 2_556 ?
Mo1 O12 K1 107.1(8) 1_455 2_556 ?
Mo3 O12 K1 103.4(7) . 2_556 ?
Mo1 O13 Mo4 105.8(8) . . ?
Mo1 O13 Th1 147.0(9) . . ?
Mo4 O13 Th1 102.7(7) . . ?
Mo1 O13 K1 95.3(7) . 2_656 ?
Mo4 O13 K1 112.2(7) . 2_656 ?
Th1 O13 K1 89.1(6) . 2_656 ?
Mo5 O14 Mo6 102.1(9) . . ?
Mo5 O14 Mo5 107.8(8) . 2_655 ?
Mo6 O14 Mo5 97.9(8) . 2_655 ?
Mo2 O15 Th1 147.4(11) . 2_556 ?
Mo2 O15 K1 94.5(9) . . ?
Th1 O15 K1 113.1(8) 2_556 . ?
Mo5 O16 Th2 144.7(13) . 1_655 ?
Mo5 O16 Sr1 101.3(9) . 1_655 ?
Th2 O16 Sr1 113.9(9) 1_655 1_655 ?
Mo6 O17 Sr1 138.5(11) . 2_545 ?
Mo6 O17 K2 102.8(9) . . ?
Sr1 O17 K2 100.2(7) 2_545 . ?
Mo3 O18 Sr1 130.9(11) . 1_565 ?
Mo3 O18 K2 137.9(12) . 2 ?
Sr1 O18 K2 88.5(7) 1_565 2 ?
Mo3 O18 K1 90.2(8) . 1_565 ?
Sr1 O18 K1 112.0(7) 1_565 1_565 ?
K2 O18 K1 86.3(6) 2 1_565 ?
Mo4 O19 Th2 148.1(11) . . ?
Mo4 O19 K2 98.7(9) . 2 ?
Th2 O19 K2 103.8(7) . 2 ?
Mo5 O20 Mo6 105.3(10) . . ?
Mo5 O20 Sr1 98.6(9) . 1_655 ?
Mo6 O20 Sr1 140.1(10) . 1_655 ?
Mo1 O21 Th2 153.4(10) . . ?
Mo5 O22 Sr1 134.0(12) . 2_545 ?
Mo5 O22 K2 128.0(11) . 1_655 ?
Sr1 O22 K2 96.3(7) 2_545 1_655 ?
Mo5 O23 Mo6 108.3(9) . 2_655 ?
Mo5 O23 Th2 148.6(10) . 2_655 ?
Mo6 O23 Th2 96.9(7) 2_655 2_655 ?
Mo3 O24 Th1 150.1(12) . . ?
Mo3 O24 K1 104.6(10) . 1_565 ?
Th1 O24 K1 99.2(7) . 1_565 ?
O17 Sr1 O11 128.4(7) 2_545 1_445 ?
O17 Sr1 O3 152.8(7) 2_545 1_455 ?
O11 Sr1 O3 75.2(7) 1_445 1_455 ?
O17 Sr1 O22 78.4(7) 2_545 2_545 ?
O11 Sr1 O22 68.0(7) 1_445 2_545 ?
O3 Sr1 O22 127.5(7) 1_455 2_545 ?
O17 Sr1 O20 108.7(7) 2_545 1_455 ?
O11 Sr1 O20 104.1(7) 1_445 1_455 ?
O3 Sr1 O20 72.0(7) 1_455 1_455 ?
O22 Sr1 O20 81.9(7) 2_545 1_455 ?
O17 Sr1 O16 82.2(7) 2_545 1_455 ?
O11 Sr1 O16 149.2(7) 1_445 1_455 ?
O3 Sr1 O16 76.2(6) 1_455 1_455 ?
O22 Sr1 O16 123.5(7) 2_545 1_455 ?
O20 Sr1 O16 55.4(7) 1_455 1_455 ?
O17 Sr1 O6 95.8(6) 2_545 . ?
O11 Sr1 O6 110.6(6) 1_445 . ?
O3 Sr1 O6 59.7(6) 1_455 . ?
O22 Sr1 O6 169.9(7) 2_545 . ?
O20 Sr1 O6 108.0(6) 1_455 . ?
O16 Sr1 O6 63.2(6) 1_455 . ?
O17 Sr1 O18 72.0(7) 2_545 1_545 ?
O11 Sr1 O18 77.6(7) 1_445 1_545 ?
O3 Sr1 O18 105.7(6) 1_455 1_545 ?
O22 Sr1 O18 101.5(7) 2_545 1_545 ?
O20 Sr1 O18 176.5(7) 1_455 1_545 ?
O16 Sr1 O18 121.7(7) 1_455 1_545 ?
O6 Sr1 O18 68.6(6) . 1_545 ?
O17 Sr1 Mo5 81.9(5) 2_545 1_455 ?
O11 Sr1 Mo5 137.0(5) 1_445 1_455 ?
O3 Sr1 Mo5 87.2(5) 1_455 1_455 ?
O22 Sr1 Mo5 95.0(5) 2_545 1_455 ?
O20 Sr1 Mo5 33.0(5) 1_455 1_455 ?
O16 Sr1 Mo5 29.5(5) 1_455 1_455 ?
O6 Sr1 Mo5 92.4(5) . 1_455 ?
O18 Sr1 Mo5 145.3(5) 1_545 1_455 ?
O17 Sr1 Mo2 123.9(5) 2_545 . ?
O11 Sr1 Mo2 86.9(5) 1_445 . ?
O3 Sr1 Mo2 34.3(4) 1_455 . ?
O22 Sr1 Mo2 154.4(6) 2_545 . ?
O20 Sr1 Mo2 99.9(5) 1_455 . ?
O16 Sr1 Mo2 75.9(5) 1_455 . ?
O6 Sr1 Mo2 28.5(4) . . ?
O18 Sr1 Mo2 77.1(4) 1_545 . ?
Mo5 Sr1 Mo2 100.26(14) 1_455 . ?
O17 Sr1 Mo6 16.6(4) 2_545 2_545 ?
O11 Sr1 Mo6 113.0(5) 1_445 2_545 ?
O3 Sr1 Mo6 168.7(5) 1_455 2_545 ?
O22 Sr1 Mo6 63.7(5) 2_545 2_545 ?
O20 Sr1 Mo6 111.8(5) 1_455 2_545 ?
O16 Sr1 Mo6 97.0(5) 1_455 2_545 ?
O6 Sr1 Mo6 109.3(5) . 2_545 ?
O18 Sr1 Mo6 69.8(4) 1_545 2_545 ?
Mo5 Sr1 Mo6 91.19(12) 1_455 2_545 ?
Mo2 Sr1 Mo6 135.64(16) . 2_545 ?
O17 Sr1 K2 42.1(5) 2_545 2_545 ?
O11 Sr1 K2 123.5(5) 1_445 2_545 ?
O3 Sr1 K2 116.7(5) 1_455 2_545 ?
O22 Sr1 K2 114.6(6) 2_545 2_545 ?
O20 Sr1 K2 132.4(5) 1_455 2_545 ?
O16 Sr1 K2 80.2(5) 1_455 2_545 ?
O6 Sr1 K2 57.2(4) . 2_545 ?
O18 Sr1 K2 45.9(5) 1_545 2_545 ?
Mo5 Sr1 K2 99.44(17) 1_455 2_545 ?
Mo2 Sr1 K2 83.20(16) . 2_545 ?
Mo6 Sr1 K2 52.56(14) 2_545 2_545 ?
O12 K1 O8 116.9(7) 2_556 1_545 ?
O12 K1 O15 80.9(6) 2_556 . ?
O8 K1 O15 151.2(6) 1_545 . ?
O12 K1 O5 99.9(6) 2_556 . ?
O8 K1 O5 69.6(6) 1_545 . ?
O15 K1 O5 132.5(7) . . ?
O12 K1 O24 105.2(7) 2_556 1_545 ?
O8 K1 O24 62.5(7) 1_545 1_545 ?
O15 K1 O24 91.9(7) . 1_545 ?
O5 K1 O24 131.9(7) . 1_545 ?
O12 K1 O9 74.8(6) 2_556 . ?
O8 K1 O9 146.6(6) 1_545 . ?
O15 K1 O9 56.5(6) . . ?
O5 K1 O9 77.7(6) . . ?
O24 K1 O9 148.3(7) 1_545 . ?
O12 K1 O1 57.7(6) 2_556 2_556 ?
O8 K1 O1 66.5(6) 1_545 2_556 ?
O15 K1 O1 112.6(6) . 2_556 ?
O5 K1 O1 107.1(6) . 2_556 ?
O24 K1 O1 57.9(6) 1_545 2_556 ?
O9 K1 O1 132.5(6) . 2_556 ?
O12 K1 O13 55.9(5) 2_556 2_656 ?
O8 K1 O13 67.4(5) 1_545 2_656 ?
O15 K1 O13 136.4(6) . 2_656 ?
O5 K1 O13 59.3(5) . 2_656 ?
O24 K1 O13 103.9(6) 1_545 2_656 ?
O9 K1 O13 101.9(5) . 2_656 ?
O1 K1 O13 51.2(5) 2_556 2_656 ?
O12 K1 O18 137.4(6) 2_556 1_545 ?
O8 K1 O18 87.2(6) 1_545 1_545 ?
O15 K1 O18 65.7(6) . 1_545 ?
O5 K1 O18 122.0(6) . 1_545 ?
O24 K1 O18 53.2(6) 1_545 1_545 ?
O9 K1 O18 104.9(6) . 1_545 ?
O1 K1 O18 110.8(6) 2_556 1_545 ?
O13 K1 O18 152.8(6) 2_656 1_545 ?
O12 K1 O6 120.4(6) 2_556 . ?
O8 K1 O6 121.7(6) 1_545 . ?
O15 K1 O6 51.9(6) . . ?
O5 K1 O6 90.8(6) . . ?
O24 K1 O6 109.9(6) 1_545 . ?
O9 K1 O6 50.5(5) . . ?
O1 K1 O6 162.2(6) 2_556 . ?
O13 K1 O6 145.1(6) 2_656 . ?
O18 K1 O6 57.1(5) 1_545 . ?
O12 K1 Mo2 90.3(5) 2_556 . ?
O8 K1 Mo2 152.2(5) 1_545 . ?
O15 K1 Mo2 31.3(4) . . ?
O5 K1 Mo2 101.6(5) . . ?
O24 K1 Mo2 118.3(5) 1_545 . ?
O9 K1 Mo2 31.3(4) . . ?
O1 K1 Mo2 139.8(5) 2_556 . ?
O13 K1 Mo2 132.1(4) 2_656 . ?
O18 K1 Mo2 75.1(4) 1_545 . ?
O6 K1 Mo2 30.5(4) . . ?
O12 K1 Mo3 117.7(5) 2_556 1_545 ?
O8 K1 Mo3 80.6(4) 1_545 1_545 ?
O15 K1 Mo3 70.9(4) . 1_545 ?
O5 K1 Mo3 139.8(5) . 1_545 ?
O24 K1 Mo3 27.8(4) 1_545 1_545 ?
O9 K1 Mo3 123.6(4) . 1_545 ?
O1 K1 Mo3 83.7(4) 2_556 1_545 ?
O13 K1 Mo3 131.7(4) 2_656 1_545 ?
O18 K1 Mo3 27.6(4) 1_545 1_545 ?
O6 K1 Mo3 82.4(4) . 1_545 ?
Mo2 K1 Mo3 92.27(18) . 1_545 ?
O7 K2 O17 76.6(6) 2_545 . ?
O7 K2 O11 110.0(7) 2_545 2 ?
O17 K2 O11 173.2(7) . 2 ?
O7 K2 O10 123.7(6) 2_545 . ?
O17 K2 O10 56.6(6) . . ?
O11 K2 O10 116.8(6) 2 . ?
O7 K2 O19 166.7(7) 2_545 2 ?
O17 K2 O19 116.6(6) . 2 ?
O11 K2 O19 56.8(6) 2 2 ?
O10 K2 O19 66.8(6) . 2 ?
O7 K2 O22 95.9(7) 2_545 1_455 ?
O17 K2 O22 116.6(7) . 1_455 ?
O11 K2 O22 61.6(6) 2 1_455 ?
O10 K2 O22 80.9(6) . 1_455 ?
O19 K2 O22 76.8(7) 2 1_455 ?
O7 K2 O18 116.7(7) 2_545 2 ?
O17 K2 O18 68.5(6) . 2 ?
O11 K2 O18 109.1(7) 2 2 ?
O10 K2 O18 75.7(6) . 2 ?
O19 K2 O18 72.4(7) 2 2 ?
O22 K2 O18 146.7(7) 1_455 2 ?
O7 K2 Mo6 95.9(5) 2_545 . ?
O17 K2 Mo6 28.0(4) . . ?
O11 K2 Mo6 146.0(5) 2 . ?
O10 K2 Mo6 30.1(4) . . ?
O19 K2 Mo6 95.8(4) 2 . ?
O22 K2 Mo6 95.0(5) 1_455 . ?
O18 K2 Mo6 76.3(4) 2 . ?
O7 K2 Mo4 137.7(5) 2_545 2 ?
O17 K2 Mo4 145.6(5) . 2 ?
O11 K2 Mo4 28.1(5) 2 2 ?
O10 K2 Mo4 94.5(4) . 2 ?
O19 K2 Mo4 29.4(4) 2 2 ?
O22 K2 Mo4 70.7(5) 1_455 2 ?
O18 K2 Mo4 87.7(5) 2 2 ?
Mo6 K2 Mo4 124.5(2) . 2 ?
O7 K2 Mo6 23.1(4) 2_545 2_545 ?
O17 K2 Mo6 83.2(5) . 2_545 ?
O11 K2 Mo6 102.1(5) 2 2_545 ?
O10 K2 Mo6 114.0(5) . 2_545 ?
O19 K2 Mo6 149.4(5) 2 2_545 ?
O22 K2 Mo6 73.3(5) 1_455 2_545 ?
O18 K2 Mo6 138.3(5) 2 2_545 ?
Mo6 K2 Mo6 93.12(19) . 2_545 ?
Mo4 K2 Mo6 129.1(2) 2 2_545 ?
O7 K2 Sr1 74.8(5) 2_545 2_545 ?
O17 K2 Sr1 37.8(4) . 2_545 ?
O11 K2 Sr1 144.6(5) 2 2_545 ?
O10 K2 Sr1 84.1(4) . 2_545 ?
O19 K2 Sr1 116.5(5) 2 2_545 ?
O22 K2 Sr1 153.7(5) 1_455 2_545 ?
O18 K2 Sr1 45.5(5) 2 2_545 ?
Mo6 K2 Sr1 62.45(15) . 2_545 ?
Mo4 K2 Sr1 132.2(3) 2 2_545 ?
Mo6 K2 Sr1 93.58(19) 2_545 2_545 ?
O7 K2 Sr1 81.5(5) 2_545 2_445 ?
O17 K2 Sr1 145.4(5) . 2_445 ?
O11 K2 Sr1 37.5(5) 2 2_445 ?
O10 K2 Sr1 119.6(5) . 2_445 ?
O19 K2 Sr1 85.8(5) 2 2_445 ?
O22 K2 Sr1 39.7(4) 1_455 2_445 ?
O18 K2 Sr1 146.0(5) 2 2_445 ?
Mo6 K2 Sr1 133.1(3) . 2_445 ?
Mo4 K2 Sr1 62.33(15) 2 2_445 ?
Mo6 K2 Sr1 66.92(16) 2_545 2_445 ?
Sr1 K2 Sr1 153.5(3) 2_545 2_445 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O10 Th2 Mo2 O15 141.7(12) 2 . . . ?
O16 Th2 Mo2 O15 73.3(12) 1_455 . . . ?
O19 Th2 Mo2 O15 -137.4(12) . . . . ?
O23 Th2 Mo2 O15 -73.1(16) 2_655 . . . ?
O7 Th2 Mo2 O15 1.7(11) . . . . ?
O21 Th2 Mo2 O15 -66.3(11) . . . . ?
O6 Th2 Mo2 O15 5.4(14) . . . . ?
O4 Th2 Mo2 O15 163.4(13) . . . . ?
Mo6 Th2 Mo2 O15 -0.3(10) . . . . ?
K2 Th2 Mo2 O15 -174.2(10) 2 . . . ?
Sr1 Th2 Mo2 O15 48.7(10) . . . . ?
O10 Th2 Mo2 O6 136.2(11) 2 . . . ?
O16 Th2 Mo2 O6 67.9(11) 1_455 . . . ?
O19 Th2 Mo2 O6 -142.8(11) . . . . ?
O23 Th2 Mo2 O6 -78.6(16) 2_655 . . . ?
O7 Th2 Mo2 O6 -3.7(10) . . . . ?
O21 Th2 Mo2 O6 -71.7(10) . . . . ?
O4 Th2 Mo2 O6 158.0(12) . . . . ?
Mo6 Th2 Mo2 O6 -5.7(9) . . . . ?
K2 Th2 Mo2 O6 -179.6(10) 2 . . . ?
Sr1 Th2 Mo2 O6 43.2(9) . . . . ?
O10 Th2 Mo2 O9 -111.7(8) 2 . . . ?
O16 Th2 Mo2 O9 179.9(8) 1_455 . . . ?
O19 Th2 Mo2 O9 -30.8(8) . . . . ?
O23 Th2 Mo2 O9 33.5(14) 2_655 . . . ?
O7 Th2 Mo2 O9 108.3(8) . . . . ?
O21 Th2 Mo2 O9 40.3(8) . . . . ?
O6 Th2 Mo2 O9 112.0(11) . . . . ?
O4 Th2 Mo2 O9 -90.0(9) . . . . ?
Mo6 Th2 Mo2 O9 106.3(6) . . . . ?
K2 Th2 Mo2 O9 -67.6(6) 2 . . . ?
Sr1 Th2 Mo2 O9 155.3(6) . . . . ?
O10 Th2 Mo2 O12 -23.5(8) 2 . . . ?
O16 Th2 Mo2 O12 -91.8(8) 1_455 . . . ?
O19 Th2 Mo2 O12 57.5(8) . . . . ?
O23 Th2 Mo2 O12 121.7(14) 2_655 . . . ?
O7 Th2 Mo2 O12 -163.4(7) . . . . ?
O21 Th2 Mo2 O12 128.5(7) . . . . ?
O6 Th2 Mo2 O12 -159.7(11) . . . . ?
O4 Th2 Mo2 O12 -1.7(9) . . . . ?
Mo6 Th2 Mo2 O12 -165.4(6) . . . . ?
K2 Th2 Mo2 O12 20.7(6) 2 . . . ?
Sr1 Th2 Mo2 O12 -116.5(6) . . . . ?
O10 Th2 Mo2 O3 49.5(7) 2 . . 1_455 ?
O16 Th2 Mo2 O3 -18.9(8) 1_455 . . 1_455 ?
O19 Th2 Mo2 O3 130.4(7) . . . 1_455 ?
O23 Th2 Mo2 O3 -165.3(14) 2_655 . . 1_455 ?
O7 Th2 Mo2 O3 -90.5(7) . . . 1_455 ?
O21 Th2 Mo2 O3 -158.5(7) . . . 1_455 ?
O6 Th2 Mo2 O3 -86.8(11) . . . 1_455 ?
O4 Th2 Mo2 O3 71.3(9) . . . 1_455 ?
Mo6 Th2 Mo2 O3 -92.5(6) . . . 1_455 ?
K2 Th2 Mo2 O3 93.7(6) 2 . . 1_455 ?
Sr1 Th2 Mo2 O3 -43.5(6) . . . 1_455 ?
O10 Th2 Mo2 O4 -21.8(9) 2 . . . ?
O16 Th2 Mo2 O4 -90.1(9) 1_455 . . . ?
O19 Th2 Mo2 O4 59.2(9) . . . . ?
O23 Th2 Mo2 O4 123.4(15) 2_655 . . . ?
O7 Th2 Mo2 O4 -161.7(8) . . . . ?
O21 Th2 Mo2 O4 130.2(8) . . . . ?
O6 Th2 Mo2 O4 -158.0(12) . . . . ?
Mo6 Th2 Mo2 O4 -163.7(7) . . . . ?
K2 Th2 Mo2 O4 22.4(7) 2 . . . ?
Sr1 Th2 Mo2 O4 -114.8(7) . . . . ?
O10 Th2 Mo2 Mo1 24.8(5) 2 . . 1_455 ?
O16 Th2 Mo2 Mo1 -43.6(6) 1_455 . . 1_455 ?
O19 Th2 Mo2 Mo1 105.7(5) . . . 1_455 ?
O23 Th2 Mo2 Mo1 170.0(13) 2_655 . . 1_455 ?
O7 Th2 Mo2 Mo1 -115.2(4) . . . 1_455 ?
O21 Th2 Mo2 Mo1 176.8(4) . . . 1_455 ?
O6 Th2 Mo2 Mo1 -111.5(9) . . . 1_455 ?
O4 Th2 Mo2 Mo1 46.5(7) . . . 1_455 ?
Mo6 Th2 Mo2 Mo1 -117.19(7) . . . 1_455 ?
K2 Th2 Mo2 Mo1 68.94(13) 2 . . 1_455 ?
Sr1 Th2 Mo2 Mo1 -68.23(11) . . . 1_455 ?
O10 Th2 Mo2 K1 -174.8(5) 2 . . . ?
O16 Th2 Mo2 K1 116.8(6) 1_455 . . . ?
O19 Th2 Mo2 K1 -93.8(5) . . . . ?
O23 Th2 Mo2 K1 -29.6(13) 2_655 . . . ?
O7 Th2 Mo2 K1 45.2(5) . . . . ?
O21 Th2 Mo2 K1 -22.8(5) . . . . ?
O6 Th2 Mo2 K1 48.9(10) . . . . ?
O4 Th2 Mo2 K1 -153.0(7) . . . . ?
Mo6 Th2 Mo2 K1 43.23(15) . . . . ?
K2 Th2 Mo2 K1 -130.64(18) 2 . . . ?
Sr1 Th2 Mo2 K1 92.18(17) . . . . ?
O10 Th2 Mo2 Sr1 93.0(5) 2 . . . ?
O16 Th2 Mo2 Sr1 24.6(6) 1_455 . . . ?
O19 Th2 Mo2 Sr1 174.0(5) . . . . ?
O23 Th2 Mo2 Sr1 -121.8(13) 2_655 . . . ?
O7 Th2 Mo2 Sr1 -47.0(4) . . . . ?
O21 Th2 Mo2 Sr1 -115.0(4) . . . . ?
O6 Th2 Mo2 Sr1 -43.2(9) . . . . ?
O4 Th2 Mo2 Sr1 114.8(7) . . . . ?
Mo6 Th2 Mo2 Sr1 -48.96(11) . . . . ?
K2 Th2 Mo2 Sr1 137.17(15) 2 . . . ?
O24 Th1 Mo4 O11 55.4(11) . . . . ?
O13 Th1 Mo4 O11 -167.2(12) . . . . ?
O9 Th1 Mo4 O11 127.1(11) . . . . ?
O15 Th1 Mo4 O11 109(2) 2_556 . . . ?
O1 Th1 Mo4 O11 -15.9(11) 2_566 . . . ?
O8 Th1 Mo4 O11 -15.8(13) . . . . ?
O5 Th1 Mo4 O11 -144.1(11) 2_656 . . . ?
O8 Th1 Mo4 O11 -72.3(11) 2_666 . . . ?
Mo4 Th1 Mo4 O11 -54.4(10) 2_666 . . . ?
K1 Th1 Mo4 O11 -115.9(10) 2_656 . . . ?
K1 Th1 Mo4 O11 10.6(10) 1_565 . . . ?
O24 Th1 Mo4 O19 -43.1(9) . . . . ?
O13 Th1 Mo4 O19 94.4(9) . . . . ?
O9 Th1 Mo4 O19 28.7(8) . . . . ?
O15 Th1 Mo4 O19 11(2) 2_556 . . . ?
O1 Th1 Mo4 O19 -114.3(8) 2_566 . . . ?
O8 Th1 Mo4 O19 -114.3(11) . . . . ?
O5 Th1 Mo4 O19 117.5(8) 2_656 . . . ?
O8 Th1 Mo4 O19 -170.8(8) 2_666 . . . ?
Mo4 Th1 Mo4 O19 -152.8(7) 2_666 . . . ?
K1 Th1 Mo4 O19 145.6(7) 2_656 . . . ?
K1 Th1 Mo4 O19 -87.8(7) 1_565 . . . ?
O24 Th1 Mo4 O8 71.2(10) . . . . ?
O13 Th1 Mo4 O8 -151.3(11) . . . . ?
O9 Th1 Mo4 O8 143.0(10) . . . . ?
O15 Th1 Mo4 O8 125(2) 2_556 . . . ?
O1 Th1 Mo4 O8 -0.1(10) 2_566 . . . ?
O5 Th1 Mo4 O8 -128.2(10) 2_656 . . . ?
O8 Th1 Mo4 O8 -56.5(12) 2_666 . . . ?
Mo4 Th1 Mo4 O8 -38.6(9) 2_666 . . . ?
K1 Th1 Mo4 O8 -100.1(9) 2_656 . . . ?
K1 Th1 Mo4 O8 26.5(9) 1_565 . . . ?
O24 Th1 Mo4 O2 -137.4(8) . . . . ?
O13 Th1 Mo4 O2 0.1(10) . . . . ?
O9 Th1 Mo4 O2 -65.6(8) . . . . ?
O15 Th1 Mo4 O2 -84(2) 2_556 . . . ?
O1 Th1 Mo4 O2 151.3(8) 2_566 . . . ?
O8 Th1 Mo4 O2 151.4(11) . . . . ?
O5 Th1 Mo4 O2 23.1(8) 2_656 . . . ?
O8 Th1 Mo4 O2 94.9(8) 2_666 . . . ?
Mo4 Th1 Mo4 O2 112.8(7) 2_666 . . . ?
K1 Th1 Mo4 O2 51.3(7) 2_656 . . . ?
K1 Th1 Mo4 O2 177.9(7) 1_565 . . . ?
O24 Th1 Mo4 O1 150.7(8) . . . 1_655 ?
O13 Th1 Mo4 O1 -71.8(9) . . . 1_655 ?
O9 Th1 Mo4 O1 -137.5(7) . . . 1_655 ?
O15 Th1 Mo4 O1 -155.6(19) 2_556 . . 1_655 ?
O1 Th1 Mo4 O1 79.5(9) 2_566 . . 1_655 ?
O8 Th1 Mo4 O1 79.5(10) . . . 1_655 ?
O5 Th1 Mo4 O1 -48.7(7) 2_656 . . 1_655 ?
O8 Th1 Mo4 O1 23.0(7) 2_666 . . 1_655 ?
Mo4 Th1 Mo4 O1 41.0(6) 2_666 . . 1_655 ?
K1 Th1 Mo4 O1 -20.6(6) 2_656 . . 1_655 ?
K1 Th1 Mo4 O1 106.0(6) 1_565 . . 1_655 ?
O24 Th1 Mo4 O13 -137.4(9) . . . . ?
O9 Th1 Mo4 O13 -65.7(8) . . . . ?
O15 Th1 Mo4 O13 -84(2) 2_556 . . . ?
O1 Th1 Mo4 O13 151.3(9) 2_566 . . . ?
O8 Th1 Mo4 O13 151.3(11) . . . . ?
O5 Th1 Mo4 O13 23.1(8) 2_656 . . . ?
O8 Th1 Mo4 O13 94.8(8) 2_666 . . . ?
Mo4 Th1 Mo4 O13 112.8(7) 2_666 . . . ?
K1 Th1 Mo4 O13 51.2(7) 2_656 . . . ?
K1 Th1 Mo4 O13 177.8(7) 1_565 . . . ?
O24 Th1 Mo4 Mo3 178.6(5) . . . 1_655 ?
O13 Th1 Mo4 Mo3 -44.0(7) . . . 1_655 ?
O9 Th1 Mo4 Mo3 -109.7(5) . . . 1_655 ?
O15 Th1 Mo4 Mo3 -127.8(19) 2_556 . . 1_655 ?
O1 Th1 Mo4 Mo3 107.3(5) 2_566 . . 1_655 ?
O8 Th1 Mo4 Mo3 107.4(9) . . . 1_655 ?
O5 Th1 Mo4 Mo3 -20.9(5) 2_656 . . 1_655 ?
O8 Th1 Mo4 Mo3 50.9(5) 2_666 . . 1_655 ?
Mo4 Th1 Mo4 Mo3 68.80(5) 2_666 . . 1_655 ?
K1 Th1 Mo4 Mo3 7.25(13) 2_656 . . 1_655 ?
K1 Th1 Mo4 Mo3 133.82(13) 1_565 . . 1_655 ?
O24 Th1 Mo4 Th1 109.8(5) . . . 2_666 ?
O13 Th1 Mo4 Th1 -112.8(7) . . . 2_666 ?
O9 Th1 Mo4 Th1 -178.5(5) . . . 2_666 ?
O15 Th1 Mo4 Th1 163.4(19) 2_556 . . 2_666 ?
O1 Th1 Mo4 Th1 38.5(5) 2_566 . . 2_666 ?
O8 Th1 Mo4 Th1 38.6(9) . . . 2_666 ?
O5 Th1 Mo4 Th1 -89.7(5) 2_656 . . 2_666 ?
O8 Th1 Mo4 Th1 -17.9(5) 2_666 . . 2_666 ?
Mo4 Th1 Mo4 Th1 0.000(2) 2_666 . . 2_666 ?
K1 Th1 Mo4 Th1 -61.54(12) 2_656 . . 2_666 ?
K1 Th1 Mo4 Th1 65.02(12) 1_565 . . 2_666 ?
O24 Th1 Mo4 K2 1.4(5) . . . 2 ?
O13 Th1 Mo4 K2 138.9(7) . . . 2 ?
O9 Th1 Mo4 K2 73.2(5) . . . 2 ?
O15 Th1 Mo4 K2 55.1(19) 2_556 . . 2 ?
O1 Th1 Mo4 K2 -69.8(5) 2_566 . . 2 ?
O8 Th1 Mo4 K2 -69.8(9) . . . 2 ?
O5 Th1 Mo4 K2 162.0(5) 2_656 . . 2 ?
O8 Th1 Mo4 K2 -126.3(5) 2_666 . . 2 ?
Mo4 Th1 Mo4 K2 -108.33(15) 2_666 . . 2 ?
K1 Th1 Mo4 K2 -169.87(19) 2_656 . . 2 ?
K1 Th1 Mo4 K2 -43.31(19) 1_565 . . 2 ?
O22 Mo5 Mo6 O17 5.0(10) . . . . ?
O16 Mo5 Mo6 O17 -104.9(11) . . . . ?
O23 Mo5 Mo6 O17 112.5(10) . . . . ?
O20 Mo5 Mo6 O17 -99.1(13) . . . . ?
O14 Mo5 Mo6 O17 110.0(11) . . . . ?
O14 Mo5 Mo6 O17 179.2(8) 2_655 . . . ?
Sr1 Mo5 Mo6 O17 -75.3(7) 1_655 . . . ?
O22 Mo5 Mo6 O10 -96.3(11) . . . . ?
O16 Mo5 Mo6 O10 153.8(11) . . . . ?
O23 Mo5 Mo6 O10 11.1(10) . . . . ?
O20 Mo5 Mo6 O10 159.5(13) . . . . ?
O14 Mo5 Mo6 O10 8.7(12) . . . . ?
O14 Mo5 Mo6 O10 77.8(9) 2_655 . . . ?
Sr1 Mo5 Mo6 O10 -176.7(7) 1_655 . . . ?
O22 Mo5 Mo6 O7 110.1(11) . . . . ?
O16 Mo5 Mo6 O7 0.2(11) . . . . ?
O23 Mo5 Mo6 O7 -142.4(10) . . . . ?
O20 Mo5 Mo6 O7 5.9(13) . . . . ?
O14 Mo5 Mo6 O7 -144.9(12) . . . . ?
O14 Mo5 Mo6 O7 -75.8(9) 2_655 . . . ?
Sr1 Mo5 Mo6 O7 29.8(7) 1_655 . . . ?
O22 Mo5 Mo6 O20 104.1(13) . . . . ?
O16 Mo5 Mo6 O20 -5.8(13) . . . . ?
O23 Mo5 Mo6 O20 -148.4(13) . . . . ?
O14 Mo5 Mo6 O20 -150.8(14) . . . . ?
O14 Mo5 Mo6 O20 -81.7(12) 2_655 . . . ?
Sr1 Mo5 Mo6 O20 23.8(11) 1_655 . . . ?
O22 Mo5 Mo6 O14 -105.0(12) . . . . ?
O16 Mo5 Mo6 O14 145.1(13) . . . . ?
O23 Mo5 Mo6 O14 2.5(12) . . . . ?
O20 Mo5 Mo6 O14 150.8(14) . . . . ?
O14 Mo5 Mo6 O14 69.2(12) 2_655 . . . ?
Sr1 Mo5 Mo6 O14 174.7(9) 1_655 . . . ?
O22 Mo5 Mo6 O23 -177.8(9) . . . 2_655 ?
O16 Mo5 Mo6 O23 72.3(10) . . . 2_655 ?
O23 Mo5 Mo6 O23 -70.3(10) . . . 2_655 ?
O20 Mo5 Mo6 O23 78.0(12) . . . 2_655 ?
O14 Mo5 Mo6 O23 -72.8(10) . . . 2_655 ?
O14 Mo5 Mo6 O23 -3.7(7) 2_655 . . 2_655 ?
Sr1 Mo5 Mo6 O23 101.8(5) 1_655 . . 2_655 ?
O22 Mo5 Mo6 Th2 157.9(8) . . . . ?
O16 Mo5 Mo6 Th2 48.0(9) . . . . ?
O23 Mo5 Mo6 Th2 -94.6(7) . . . . ?
O20 Mo5 Mo6 Th2 53.7(11) . . . . ?
O14 Mo5 Mo6 Th2 -97.1(9) . . . . ?
O14 Mo5 Mo6 Th2 -27.9(5) 2_655 . . . ?
Sr1 Mo5 Mo6 Th2 77.57(10) 1_655 . . . ?
O22 Mo5 Mo6 K2 -29.2(8) . . . . ?
O16 Mo5 Mo6 K2 -139.1(9) . . . . ?
O23 Mo5 Mo6 K2 78.3(7) . . . . ?
O20 Mo5 Mo6 K2 -133.3(11) . . . . ?
O14 Mo5 Mo6 K2 75.8(9) . . . . ?
O14 Mo5 Mo6 K2 145.0(5) 2_655 . . . ?
Sr1 Mo5 Mo6 K2 -109.5(2) 1_655 . . . ?
O22 Mo5 Mo6 K2 76.6(8) . . . 2_545 ?
O16 Mo5 Mo6 K2 -33.3(9) . . . 2_545 ?
O23 Mo5 Mo6 K2 -175.9(7) . . . 2_545 ?
O20 Mo5 Mo6 K2 -27.5(11) . . . 2_545 ?
O14 Mo5 Mo6 K2 -178.4(9) . . . 2_545 ?
O14 Mo5 Mo6 K2 -109.2(5) 2_655 . . 2_545 ?
Sr1 Mo5 Mo6 K2 -3.72(17) 1_655 . . 2_545 ?
O22 Mo5 Mo6 Sr1 -5.3(8) . . . 2_545 ?
O16 Mo5 Mo6 Sr1 -115.2(9) . . . 2_545 ?
O23 Mo5 Mo6 Sr1 102.1(7) . . . 2_545 ?
O20 Mo5 Mo6 Sr1 -109.5(11) . . . 2_545 ?
O14 Mo5 Mo6 Sr1 99.7(9) . . . 2_545 ?
O14 Mo5 Mo6 Sr1 168.8(5) 2_655 . . 2_545 ?
Sr1 Mo5 Mo6 Sr1 -85.66(13) 1_655 . . 2_545 ?
O10 Th2 Mo6 O17 -123.3(11) 2 . . . ?
O16 Th2 Mo6 O17 -48.1(11) 1_455 . . . ?
O19 Th2 Mo6 O17 151.9(12) . . . . ?
O23 Th2 Mo6 O17 174.0(12) 2_655 . . . ?
O7 Th2 Mo6 O17 20.2(13) . . . . ?
O21 Th2 Mo6 O17 89.2(11) . . . . ?
O6 Th2 Mo6 O17 21.3(11) . . . . ?
O4 Th2 Mo6 O17 -31(2) . . . . ?
Mo2 Th2 Mo6 O17 24.1(10) . . . . ?
K2 Th2 Mo6 O17 -162.0(10) 2 . . . ?
Sr1 Th2 Mo6 O17 -13.6(10) . . . . ?
O10 Th2 Mo6 O10 -27.9(10) 2 . . . ?
O16 Th2 Mo6 O10 47.4(8) 1_455 . . . ?
O19 Th2 Mo6 O10 -112.6(8) . . . . ?
O23 Th2 Mo6 O10 -90.5(9) 2_655 . . . ?
O7 Th2 Mo6 O10 115.6(11) . . . . ?
O21 Th2 Mo6 O10 -175.3(8) . . . . ?
O6 Th2 Mo6 O10 116.8(8) . . . . ?
O4 Th2 Mo6 O10 64(2) . . . . ?
Mo2 Th2 Mo6 O10 119.6(6) . . . . ?
K2 Th2 Mo6 O10 -66.6(6) 2 . . . ?
Sr1 Th2 Mo6 O10 81.9(6) . . . . ?
O10 Th2 Mo6 O7 -143.5(10) 2 . . . ?
O16 Th2 Mo6 O7 -68.3(10) 1_455 . . . ?
O19 Th2 Mo6 O7 131.7(11) . . . . ?
O23 Th2 Mo6 O7 153.8(11) 2_655 . . . ?
O21 Th2 Mo6 O7 69.1(10) . . . . ?
O6 Th2 Mo6 O7 1.1(10) . . . . ?
O4 Th2 Mo6 O7 -51(2) . . . . ?
Mo2 Th2 Mo6 O7 4.0(9) . . . . ?
K2 Th2 Mo6 O7 177.8(9) 2 . . . ?
Sr1 Th2 Mo6 O7 -33.7(9) . . . . ?
O10 Th2 Mo6 O20 128.9(8) 2 . . . ?
O16 Th2 Mo6 O20 -155.8(9) 1_455 . . . ?
O19 Th2 Mo6 O20 44.2(9) . . . . ?
O23 Th2 Mo6 O20 66.3(10) 2_655 . . . ?
O7 Th2 Mo6 O20 -87.5(11) . . . . ?
O21 Th2 Mo6 O20 -18.5(8) . . . . ?
O6 Th2 Mo6 O20 -86.4(8) . . . . ?
O4 Th2 Mo6 O20 -139(2) . . . . ?
Mo2 Th2 Mo6 O20 -83.6(7) . . . . ?
K2 Th2 Mo6 O20 90.2(7) 2 . . . ?
Sr1 Th2 Mo6 O20 -121.3(7) . . . . ?
O10 Th2 Mo6 O14 56.0(8) 2 . . . ?
O16 Th2 Mo6 O14 131.2(9) 1_455 . . . ?
O19 Th2 Mo6 O14 -28.8(9) . . . . ?
O23 Th2 Mo6 O14 -6.7(9) 2_655 . . . ?
O7 Th2 Mo6 O14 -160.5(11) . . . . ?
O21 Th2 Mo6 O14 -91.5(8) . . . . ?
O6 Th2 Mo6 O14 -159.4(8) . . . . ?
O4 Th2 Mo6 O14 148(2) . . . . ?
Mo2 Th2 Mo6 O14 -156.5(7) . . . . ?
K2 Th2 Mo6 O14 17.3(7) 2 . . . ?
Sr1 Th2 Mo6 O14 165.7(7) . . . . ?
O10 Th2 Mo6 O23 62.7(8) 2 . . 2_655 ?
O16 Th2 Mo6 O23 137.9(9) 1_455 . . 2_655 ?
O19 Th2 Mo6 O23 -22.1(9) . . . 2_655 ?
O7 Th2 Mo6 O23 -153.8(11) . . . 2_655 ?
O21 Th2 Mo6 O23 -84.8(8) . . . 2_655 ?
O6 Th2 Mo6 O23 -152.7(8) . . . 2_655 ?
O4 Th2 Mo6 O23 155(2) . . . 2_655 ?
Mo2 Th2 Mo6 O23 -149.9(7) . . . 2_655 ?
K2 Th2 Mo6 O23 24.0(7) 2 . . 2_655 ?
Sr1 Th2 Mo6 O23 172.4(7) . . . 2_655 ?
O10 Th2 Mo6 Mo5 99.8(5) 2 . . . ?
O16 Th2 Mo6 Mo5 175.0(6) 1_455 . . . ?
O19 Th2 Mo6 Mo5 15.0(6) . . . . ?
O23 Th2 Mo6 Mo5 37.1(7) 2_655 . . . ?
O7 Th2 Mo6 Mo5 -116.7(9) . . . . ?
O21 Th2 Mo6 Mo5 -47.7(4) . . . . ?
O6 Th2 Mo6 Mo5 -115.6(5) . . . . ?
O4 Th2 Mo6 Mo5 -168(2) . . . . ?
Mo2 Th2 Mo6 Mo5 -112.77(7) . . . . ?
K2 Th2 Mo6 Mo5 61.04(13) 2 . . . ?
Sr1 Th2 Mo6 Mo5 -150.47(9) . . . . ?
O10 Th2 Mo6 K2 -74.5(5) 2 . . . ?
O16 Th2 Mo6 K2 0.7(6) 1_455 . . . ?
O19 Th2 Mo6 K2 -159.3(6) . . . . ?
O23 Th2 Mo6 K2 -137.2(7) 2_655 . . . ?
O7 Th2 Mo6 K2 69.0(9) . . . . ?
O21 Th2 Mo6 K2 138.0(5) . . . . ?
O6 Th2 Mo6 K2 70.1(5) . . . . ?
O4 Th2 Mo6 K2 18(2) . . . . ?
Mo2 Th2 Mo6 K2 72.94(15) . . . . ?
K2 Th2 Mo6 K2 -113.25(15) 2 . . . ?
Sr1 Th2 Mo6 K2 35.23(16) . . . . ?
O10 Th2 Mo6 K2 -154.6(5) 2 . . 2_545 ?
O16 Th2 Mo6 K2 -79.4(6) 1_455 . . 2_545 ?
O19 Th2 Mo6 K2 120.6(6) . . . 2_545 ?
O23 Th2 Mo6 K2 142.7(7) 2_655 . . 2_545 ?
O7 Th2 Mo6 K2 -11.1(9) . . . 2_545 ?
O21 Th2 Mo6 K2 57.9(5) . . . 2_545 ?
O6 Th2 Mo6 K2 -10.0(5) . . . 2_545 ?
O4 Th2 Mo6 K2 -62(2) . . . 2_545 ?
Mo2 Th2 Mo6 K2 -7.15(13) . . . 2_545 ?
K2 Th2 Mo6 K2 166.7(2) 2 . . 2_545 ?
Sr1 Th2 Mo6 K2 -44.85(15) . . . 2_545 ?
O10 Th2 Mo6 Sr1 -140.1(5) 2 . . 2_545 ?
O16 Th2 Mo6 Sr1 -64.9(6) 1_455 . . 2_545 ?
O19 Th2 Mo6 Sr1 135.1(6) . . . 2_545 ?
O23 Th2 Mo6 Sr1 157.2(8) 2_655 . . 2_545 ?
O7 Th2 Mo6 Sr1 3.4(9) . . . 2_545 ?
O21 Th2 Mo6 Sr1 72.4(5) . . . 2_545 ?
O6 Th2 Mo6 Sr1 4.5(5) . . . 2_545 ?
O4 Th2 Mo6 Sr1 -48(2) . . . 2_545 ?
Mo2 Th2 Mo6 Sr1 7.3(3) . . . 2_545 ?
K2 Th2 Mo6 Sr1 -178.9(3) 2 . . 2_545 ?
Sr1 Th2 Mo6 Sr1 -30.4(4) . . . 2_545 ?
O18 Mo3 O1 Mo4 82.9(10) . . . 1_455 ?
O24 Mo3 O1 Mo4 -171.4(10) . . . 1_455 ?
O4 Mo3 O1 Mo4 -53(2) . . . 1_455 ?
O2 Mo3 O1 Mo4 -14.1(9) 1_455 . . 1_455 ?
O12 Mo3 O1 Mo4 -89.2(9) . . . 1_455 ?
K1 Mo3 O1 Mo4 142.5(8) 1_565 . . 1_455 ?
K1 Mo3 O1 Mo4 -120.3(10) 2_556 . . 1_455 ?
O18 Mo3 O1 Th1 -56(2) . . . 2_566 ?
O24 Mo3 O1 Th1 50(2) . . . 2_566 ?
O4 Mo3 O1 Th1 167.7(15) . . . 2_566 ?
O2 Mo3 O1 Th1 -153(2) 1_455 . . 2_566 ?
O12 Mo3 O1 Th1 132(2) . . . 2_566 ?
Mo4 Mo3 O1 Th1 -139(3) 1_455 . . 2_566 ?
K1 Mo3 O1 Th1 3.6(19) 1_565 . . 2_566 ?
K1 Mo3 O1 Th1 101(2) 2_556 . . 2_566 ?
O18 Mo3 O1 K1 -156.8(8) . . . 2_556 ?
O24 Mo3 O1 K1 -51.1(9) . . . 2_556 ?
O4 Mo3 O1 K1 67(2) . . . 2_556 ?
O2 Mo3 O1 K1 106.2(8) 1_455 . . 2_556 ?
O12 Mo3 O1 K1 31.2(6) . . . 2_556 ?
Mo4 Mo3 O1 K1 120.3(10) 1_455 . . 2_556 ?
K1 Mo3 O1 K1 -97.2(5) 1_565 . . 2_556 ?
O11 Mo4 O2 Mo3 76.1(11) . . . 1_655 ?
O19 Mo4 O2 Mo3 177.9(10) . . . 1_655 ?
O8 Mo4 O2 Mo3 -58.8(19) . . . 1_655 ?
O1 Mo4 O2 Mo3 -14.1(9) 1_655 . . 1_655 ?
O13 Mo4 O2 Mo3 -95.1(9) . . . 1_655 ?
Th1 Mo4 O2 Mo3 -10.2(11) 2_666 . . 1_655 ?
Th1 Mo4 O2 Mo3 -95.2(8) . . . 1_655 ?
K2 Mo4 O2 Mo3 127.7(6) 2 . . 1_655 ?
O11 Mo4 O2 Mo1 -175.3(8) . . . . ?
O19 Mo4 O2 Mo1 -73.5(9) . . . . ?
O8 Mo4 O2 Mo1 49.8(18) . . . . ?
O1 Mo4 O2 Mo1 94.5(9) 1_655 . . . ?
O13 Mo4 O2 Mo1 13.5(6) . . . . ?
Mo3 Mo4 O2 Mo1 108.6(11) 1_655 . . . ?
Th1 Mo4 O2 Mo1 98.4(6) 2_666 . . . ?
Th1 Mo4 O2 Mo1 13.4(9) . . . . ?
K2 Mo4 O2 Mo1 -123.7(5) 2 . . . ?
O21 Mo1 O2 Mo4 81.0(9) . . . . ?
O5 Mo1 O2 Mo4 -84(4) . . . . ?
O3 Mo1 O2 Mo4 174.8(9) . . . . ?
O13 Mo1 O2 Mo4 -15.8(8) . . . . ?
O12 Mo1 O2 Mo4 -107.2(9) 1_655 . . . ?
Mo2 Mo1 O2 Mo4 -145.4(7) 1_655 . . . ?
K1 Mo1 O2 Mo4 -69.2(7) 2_656 . . . ?
K1 Mo1 O2 Mo4 40.0(15) . . . . ?
O21 Mo1 O2 Mo3 -171.4(10) . . . 1_655 ?
O5 Mo1 O2 Mo3 24(5) . . . 1_655 ?
O3 Mo1 O2 Mo3 -77.6(9) . . . 1_655 ?
O13 Mo1 O2 Mo3 91.8(9) . . . 1_655 ?
O12 Mo1 O2 Mo3 0.4(8) 1_655 . . 1_655 ?
Mo2 Mo1 O2 Mo3 -37.9(7) 1_655 . . 1_655 ?
K1 Mo1 O2 Mo3 38.3(7) 2_656 . . 1_655 ?
K1 Mo1 O2 Mo3 147.6(6) . . . 1_655 ?
O21 Mo1 O3 Mo2 177.2(9) . . . 1_655 ?
O5 Mo1 O3 Mo2 -75.3(10) . . . 1_655 ?
O13 Mo1 O3 Mo2 71.3(19) . . . 1_655 ?
O12 Mo1 O3 Mo2 20.2(8) 1_655 . . 1_655 ?
O2 Mo1 O3 Mo2 93.3(9) . . . 1_655 ?
K1 Mo1 O3 Mo2 9.0(10) 2_656 . . 1_655 ?
K1 Mo1 O3 Mo2 -109.0(7) . . . 1_655 ?
O21 Mo1 O3 Sr1 -51.6(18) . . . 1_655 ?
O5 Mo1 O3 Sr1 55.9(18) . . . 1_655 ?
O13 Mo1 O3 Sr1 -157.5(13) . . . 1_655 ?
O12 Mo1 O3 Sr1 151.4(18) 1_655 . . 1_655 ?
O2 Mo1 O3 Sr1 -135.5(17) . . . 1_655 ?
Mo2 Mo1 O3 Sr1 131(2) 1_655 . . 1_655 ?
K1 Mo1 O3 Sr1 140.2(14) 2_656 . . 1_655 ?
K1 Mo1 O3 Sr1 22.1(19) . . . 1_655 ?
O18 Mo3 O4 Mo2 173.1(9) . . . . ?
O24 Mo3 O4 Mo2 67.8(11) . . . . ?
O1 Mo3 O4 Mo2 -50(2) . . . . ?
O2 Mo3 O4 Mo2 -87.5(9) 1_455 . . . ?
O12 Mo3 O4 Mo2 -12.6(7) . . . . ?
Mo4 Mo3 O4 Mo2 -87.2(8) 1_455 . . . ?
K1 Mo3 O4 Mo2 111.5(7) 1_565 . . . ?
K1 Mo3 O4 Mo2 4.2(9) 2_556 . . . ?
O18 Mo3 O4 Th2 23.3(19) . . . . ?
O24 Mo3 O4 Th2 -81.9(19) . . . . ?
O1 Mo3 O4 Th2 160.4(16) . . . . ?
O2 Mo3 O4 Th2 122.8(18) 1_455 . . . ?
O12 Mo3 O4 Th2 -162.3(19) . . . . ?
Mo4 Mo3 O4 Th2 123.1(15) 1_455 . . . ?
K1 Mo3 O4 Th2 -38(2) 1_565 . . . ?
K1 Mo3 O4 Th2 -145.5(15) 2_556 . . . ?
O15 Mo2 O4 Mo3 72(4) . . . . ?
O6 Mo2 O4 Mo3 -178.8(10) . . . . ?
O9 Mo2 O4 Mo3 -76.9(10) . . . . ?
O12 Mo2 O4 Mo3 14.0(8) . . . . ?
O3 Mo2 O4 Mo3 91.2(10) 1_455 . . . ?
Mo1 Mo2 O4 Mo3 55.9(7) 1_455 . . . ?
K1 Mo2 O4 Mo3 -122.9(7) . . . . ?
Th2 Mo2 O4 Mo3 -164.4(12) . . . . ?
Sr1 Mo2 O4 Mo3 134.6(7) . . . . ?
O15 Mo2 O4 Th2 -123(4) . . . . ?
O6 Mo2 O4 Th2 -14.3(8) . . . . ?
O9 Mo2 O4 Th2 87.6(8) . . . . ?
O12 Mo2 O4 Th2 178.4(8) . . . . ?
O3 Mo2 O4 Th2 -104.3(8) 1_455 . . . ?
Mo1 Mo2 O4 Th2 -139.7(5) 1_455 . . . ?
K1 Mo2 O4 Th2 41.5(10) . . . . ?
Sr1 Mo2 O4 Th2 -60.9(5) . . . . ?
O10 Th2 O4 Mo3 -47.8(18) 2 . . . ?
O16 Th2 O4 Mo3 -124.0(19) 1_455 . . . ?
O19 Th2 O4 Mo3 36.2(17) . . . . ?
O23 Th2 O4 Mo3 6(3) 2_655 . . . ?
O7 Th2 O4 Mo3 -179.4(14) . . . . ?
O21 Th2 O4 Mo3 100.5(18) . . . . ?
O6 Th2 O4 Mo3 162(2) . . . . ?
Mo6 Th2 O4 Mo3 -141.1(13) . . . . ?
Mo2 Th2 O4 Mo3 151(2) . . . . ?
K2 Th2 O4 Mo3 -7.4(16) 2 . . . ?
Sr1 Th2 O4 Mo3 -159.3(19) . . . . ?
O10 Th2 O4 Mo2 161.1(7) 2 . . . ?
O16 Th2 O4 Mo2 84.9(8) 1_455 . . . ?
O19 Th2 O4 Mo2 -114.9(8) . . . . ?
O23 Th2 O4 Mo2 -145.4(10) 2_655 . . . ?
O7 Th2 O4 Mo2 29.6(13) . . . . ?
O21 Th2 O4 Mo2 -50.6(8) . . . . ?
O6 Th2 O4 Mo2 11.3(6) . . . . ?
Mo6 Th2 O4 Mo2 68(2) . . . . ?
K2 Th2 O4 Mo2 -158.4(7) 2 . . . ?
Sr1 Th2 O4 Mo2 49.7(5) . . . . ?
O21 Mo1 O5 Th1 136.1(15) . . . 2_656 ?
O3 Mo1 O5 Th1 39.6(17) . . . 2_656 ?
O13 Mo1 O5 Th1 -125.0(15) . . . 2_656 ?
O12 Mo1 O5 Th1 -37.4(16) 1_655 . . 2_656 ?
O2 Mo1 O5 Th1 -60(5) . . . 2_656 ?
Mo2 Mo1 O5 Th1 1.5(15) 1_655 . . 2_656 ?
K1 Mo1 O5 Th1 -74.4(14) 2_656 . . 2_656 ?
K1 Mo1 O5 Th1 163(2) . . . 2_656 ?
O21 Mo1 O5 K1 -26.5(13) . . . . ?
O3 Mo1 O5 K1 -123.0(10) . . . . ?
O13 Mo1 O5 K1 72.4(11) . . . . ?
O12 Mo1 O5 K1 160.0(10) 1_655 . . . ?
O2 Mo1 O5 K1 137(4) . . . . ?
Mo2 Mo1 O5 K1 -161.1(9) 1_655 . . . ?
K1 Mo1 O5 K1 123.0(10) 2_656 . . . ?
O15 Mo2 O6 Th2 -176.6(9) . . . . ?
O9 Mo2 O6 Th2 -70.8(10) . . . . ?
O12 Mo2 O6 Th2 44(2) . . . . ?
O3 Mo2 O6 Th2 93.1(9) 1_455 . . . ?
O4 Mo2 O6 Th2 15.2(8) . . . . ?
Mo1 Mo2 O6 Th2 94.0(8) 1_455 . . . ?
K1 Mo2 O6 Th2 -129.2(8) . . . . ?
Sr1 Mo2 O6 Th2 117.4(11) . . . . ?
O15 Mo2 O6 Sr1 66.0(9) . . . . ?
O9 Mo2 O6 Sr1 171.7(8) . . . . ?
O12 Mo2 O6 Sr1 -73(2) . . . . ?
O3 Mo2 O6 Sr1 -24.4(8) 1_455 . . . ?
O4 Mo2 O6 Sr1 -102.2(8) . . . . ?
Mo1 Mo2 O6 Sr1 -23.4(10) 1_455 . . . ?
K1 Mo2 O6 Sr1 113.4(7) . . . . ?
Th2 Mo2 O6 Sr1 -117.4(11) . . . . ?
O15 Mo2 O6 K1 -47.4(7) . . . . ?
O9 Mo2 O6 K1 58.3(7) . . . . ?
O12 Mo2 O6 K1 173.2(16) . . . . ?
O3 Mo2 O6 K1 -137.8(6) 1_455 . . . ?
O4 Mo2 O6 K1 144.4(6) . . . . ?
Mo1 Mo2 O6 K1 -136.8(4) 1_455 . . . ?
Th2 Mo2 O6 K1 129.2(8) . . . . ?
Sr1 Mo2 O6 K1 -113.4(7) . . . . ?
O10 Th2 O6 Mo2 -61.7(13) 2 . . . ?
O16 Th2 O6 Mo2 -105.9(11) 1_455 . . . ?
O19 Th2 O6 Mo2 40.3(11) . . . . ?
O23 Th2 O6 Mo2 146.3(9) 2_655 . . . ?
O7 Th2 O6 Mo2 176.5(10) . . . . ?
O21 Th2 O6 Mo2 101.4(10) . . . . ?
O4 Th2 O6 Mo2 -14.5(8) . . . . ?
Mo6 Th2 O6 Mo2 175.9(7) . . . . ?
K2 Th2 O6 Mo2 0.6(13) 2 . . . ?
Sr1 Th2 O6 Mo2 -113.9(12) . . . . ?
O10 Th2 O6 Sr1 52.1(12) 2 . . . ?
O16 Th2 O6 Sr1 7.9(8) 1_455 . . . ?
O19 Th2 O6 Sr1 154.1(7) . . . . ?
O23 Th2 O6 Sr1 -99.8(11) 2_655 . . . ?
O7 Th2 O6 Sr1 -69.7(7) . . . . ?
O21 Th2 O6 Sr1 -144.8(9) . . . . ?
O4 Th2 O6 Sr1 99.4(8) . . . . ?
Mo6 Th2 O6 Sr1 -70.2(7) . . . . ?
Mo2 Th2 O6 Sr1 113.9(12) . . . . ?
K2 Th2 O6 Sr1 114.5(6) 2 . . . ?
O10 Th2 O6 K1 -151.7(8) 2 . . . ?
O16 Th2 O6 K1 164.1(11) 1_455 . . . ?
O19 Th2 O6 K1 -49.7(11) . . . . ?
O23 Th2 O6 K1 56.3(14) 2_655 . . . ?
O7 Th2 O6 K1 86.5(10) . . . . ?
O21 Th2 O6 K1 11.4(9) . . . . ?
O4 Th2 O6 K1 -104.5(10) . . . . ?
Mo6 Th2 O6 K1 85.9(9) . . . . ?
Mo2 Th2 O6 K1 -90.0(12) . . . . ?
K2 Th2 O6 K1 -89.4(10) 2 . . . ?
Sr1 Th2 O6 K1 156.1(14) . . . . ?
O17 Mo6 O7 Th2 -166.5(9) . . . . ?
O10 Mo6 O7 Th2 -66.0(9) . . . . ?
O20 Mo6 O7 Th2 95.8(9) . . . . ?
O14 Mo6 O7 Th2 41(2) . . . . ?
O23 Mo6 O7 Th2 17.7(8) 2_655 . . . ?
Mo5 Mo6 O7 Th2 92.2(8) . . . . ?
K2 Mo6 O7 Th2 -117.7(7) . . . . ?
K2 Mo6 O7 Th2 160.5(15) 2_545 . . . ?
Sr1 Mo6 O7 Th2 -178.8(3) 2_545 . . . ?
O17 Mo6 O7 K2 33.0(12) . . . 2_545 ?
O10 Mo6 O7 K2 133.5(10) . . . 2_545 ?
O20 Mo6 O7 K2 -64.7(11) . . . 2_545 ?
O14 Mo6 O7 K2 -119.8(17) . . . 2_545 ?
O23 Mo6 O7 K2 -142.8(10) 2_655 . . 2_545 ?
Mo5 Mo6 O7 K2 -68.3(11) . . . 2_545 ?
Th2 Mo6 O7 K2 -160.5(15) . . . 2_545 ?
K2 Mo6 O7 K2 81.8(9) . . . 2_545 ?
Sr1 Mo6 O7 K2 20.7(12) 2_545 . . 2_545 ?
O10 Th2 O7 Mo6 41.9(11) 2 . . . ?
O16 Th2 O7 Mo6 107.2(10) 1_455 . . . ?
O19 Th2 O7 Mo6 -67.7(13) . . . . ?
O23 Th2 O7 Mo6 -18.1(8) 2_655 . . . ?
O21 Th2 O7 Mo6 -105.0(9) . . . . ?
O6 Th2 O7 Mo6 -178.9(9) . . . . ?
O4 Th2 O7 Mo6 164.6(8) . . . . ?
Mo2 Th2 O7 Mo6 -177.2(6) . . . . ?
K2 Th2 O7 Mo6 -3.2(13) 2 . . . ?
Sr1 Th2 O7 Mo6 144.2(9) . . . . ?
O10 Th2 O7 K2 -157.0(8) 2 . . 2_545 ?
O16 Th2 O7 K2 -91.8(10) 1_455 . . 2_545 ?
O19 Th2 O7 K2 93.4(11) . . . 2_545 ?
O23 Th2 O7 K2 143.0(10) 2_655 . . 2_545 ?
O21 Th2 O7 K2 56.1(8) . . . 2_545 ?
O6 Th2 O7 K2 -17.8(8) . . . 2_545 ?
O4 Th2 O7 K2 -34.3(14) . . . 2_545 ?
Mo6 Th2 O7 K2 161.1(15) . . . 2_545 ?
Mo2 Th2 O7 K2 -16.1(9) . . . 2_545 ?
K2 Th2 O7 K2 157.9(5) 2 . . 2_545 ?
Sr1 Th2 O7 K2 -54.7(7) . . . 2_545 ?
O11 Mo4 O8 Th1 169.4(9) . . . . ?
O19 Mo4 O8 Th1 67.7(10) . . . . ?
O2 Mo4 O8 Th1 -54.5(19) . . . . ?
O1 Mo4 O8 Th1 -97.5(9) 1_655 . . . ?
O13 Mo4 O8 Th1 -18.3(7) . . . . ?
Mo3 Mo4 O8 Th1 -93.1(7) 1_655 . . . ?
Th1 Mo4 O8 Th1 -123.1(11) 2_666 . . . ?
K2 Mo4 O8 Th1 119.7(7) 2 . . . ?
O11 Mo4 O8 Th1 -67.5(9) . . . 2_666 ?
O19 Mo4 O8 Th1 -169.2(8) . . . 2_666 ?
O2 Mo4 O8 Th1 68.6(18) . . . 2_666 ?
O1 Mo4 O8 Th1 25.6(8) 1_655 . . 2_666 ?
O13 Mo4 O8 Th1 104.8(8) . . . 2_666 ?
Mo3 Mo4 O8 Th1 30.0(9) 1_655 . . 2_666 ?
Th1 Mo4 O8 Th1 123.1(11) . . . 2_666 ?
K2 Mo4 O8 Th1 -117.1(6) 2 . . 2_666 ?
O11 Mo4 O8 K1 44.0(13) . . . 1_565 ?
O19 Mo4 O8 K1 -57.7(14) . . . 1_565 ?
O2 Mo4 O8 K1 -179.9(12) . . . 1_565 ?
O1 Mo4 O8 K1 137.1(12) 1_655 . . 1_565 ?
O13 Mo4 O8 K1 -143.7(13) . . . 1_565 ?
Mo3 Mo4 O8 K1 141.5(9) 1_655 . . 1_565 ?
Th1 Mo4 O8 K1 111.5(14) 2_666 . . 1_565 ?
Th1 Mo4 O8 K1 -125.4(15) . . . 1_565 ?
K2 Mo4 O8 K1 -5.7(11) 2 . . 1_565 ?
O24 Th1 O8 Mo4 -102.5(10) . . . . ?
O13 Th1 O8 Mo4 18.8(7) . . . . ?
O9 Th1 O8 Mo4 -41.3(11) . . . . ?
O15 Th1 O8 Mo4 -147.2(13) 2_556 . . . ?
O1 Th1 O8 Mo4 179.9(10) 2_566 . . . ?
O5 Th1 O8 Mo4 66.6(11) 2_656 . . . ?
O8 Th1 O8 Mo4 114.6(13) 2_666 . . . ?
Mo4 Th1 O8 Mo4 142.7(8) 2_666 . . . ?
K1 Th1 O8 Mo4 73.4(8) 2_656 . . . ?
K1 Th1 O8 Mo4 -141.7(12) 1_565 . . . ?
O24 Th1 O8 Th1 142.9(10) . . . 2_666 ?
O13 Th1 O8 Th1 -95.8(9) . . . 2_666 ?
O9 Th1 O8 Th1 -155.9(7) . . . 2_666 ?
O15 Th1 O8 Th1 98.2(16) 2_556 . . 2_666 ?
O1 Th1 O8 Th1 65.4(8) 2_566 . . 2_666 ?
O5 Th1 O8 Th1 -48.0(11) 2_656 . . 2_666 ?
O8 Th1 O8 Th1 0.0 2_666 . . 2_666 ?
Mo4 Th1 O8 Th1 28.2(7) 2_666 . . 2_666 ?
Mo4 Th1 O8 Th1 -114.6(13) . . . 2_666 ?
K1 Th1 O8 Th1 -41.2(7) 2_656 . . 2_666 ?
K1 Th1 O8 Th1 103.8(10) 1_565 . . 2_666 ?
O24 Th1 O8 K1 39.1(7) . . . 1_565 ?
O13 Th1 O8 K1 160.4(8) . . . 1_565 ?
O9 Th1 O8 K1 100.4(7) . . . 1_565 ?
O15 Th1 O8 K1 -5.6(19) 2_556 . . 1_565 ?
O1 Th1 O8 K1 -38.4(7) 2_566 . . 1_565 ?
O5 Th1 O8 K1 -151.8(6) 2_656 . . 1_565 ?
O8 Th1 O8 K1 -103.8(10) 2_666 . . 1_565 ?
Mo4 Th1 O8 K1 -75.6(5) 2_666 . . 1_565 ?
Mo4 Th1 O8 K1 141.7(12) . . . 1_565 ?
K1 Th1 O8 K1 -145.0(5) 2_656 . . 1_565 ?
O15 Mo2 O9 Th1 -122(2) . . . . ?
O6 Mo2 O9 Th1 134(2) . . . . ?
O12 Mo2 O9 Th1 -22(2) . . . . ?
O3 Mo2 O9 Th1 13(4) 1_455 . . . ?
O4 Mo2 O9 Th1 52(2) . . . . ?
Mo1 Mo2 O9 Th1 -29(3) 1_455 . . . ?
K1 Mo2 O9 Th1 -161(2) . . . . ?
Th2 Mo2 O9 Th1 96(2) . . . . ?
Sr1 Mo2 O9 Th1 146.1(14) . . . . ?
O15 Mo2 O9 K1 39.0(8) . . . . ?
O6 Mo2 O9 K1 -64.7(8) . . . . ?
O12 Mo2 O9 K1 138.9(7) . . . . ?
O3 Mo2 O9 K1 174(2) 1_455 . . . ?
O4 Mo2 O9 K1 -147.5(6) . . . . ?
Mo1 Mo2 O9 K1 132.3(5) 1_455 . . . ?
Th2 Mo2 O9 K1 -103.2(4) . . . . ?
Sr1 Mo2 O9 K1 -52.9(13) . . . . ?
O24 Th1 O9 Mo2 -14(2) . . . . ?
O13 Th1 O9 Mo2 -130(2) . . . . ?
O15 Th1 O9 Mo2 80(2) 2_556 . . . ?
O1 Th1 O9 Mo2 30(3) 2_566 . . . ?
O8 Th1 O9 Mo2 -76(2) . . . . ?
O5 Th1 O9 Mo2 153(2) 2_656 . . . ?
O8 Th1 O9 Mo2 -156.5(17) 2_666 . . . ?
Mo4 Th1 O9 Mo2 90(3) 2_666 . . . ?
Mo4 Th1 O9 Mo2 -95(2) . . . . ?
K1 Th1 O9 Mo2 -168(2) 2_656 . . . ?
K1 Th1 O9 Mo2 -30(2) 1_565 . . . ?
O24 Th1 O9 K1 -171.1(11) . . . . ?
O13 Th1 O9 K1 72.4(9) . . . . ?
O15 Th1 O9 K1 -77.7(9) 2_556 . . . ?
O1 Th1 O9 K1 -127.7(10) 2_566 . . . ?
O8 Th1 O9 K1 126.6(8) . . . . ?
O5 Th1 O9 K1 -4.0(9) 2_656 . . . ?
O8 Th1 O9 K1 46(2) 2_666 . . . ?
Mo4 Th1 O9 K1 -68(2) 2_666 . . . ?
Mo4 Th1 O9 K1 107.3(8) . . . . ?
K1 Th1 O9 K1 34.7(10) 2_656 . . . ?
K1 Th1 O9 K1 172.3(6) 1_565 . . . ?
O17 Mo6 O10 Th2 -132(2) . . . 2 ?
O7 Mo6 O10 Th2 126(2) . . . 2 ?
O20 Mo6 O10 Th2 -2(4) . . . 2 ?
O14 Mo6 O10 Th2 -29(2) . . . 2 ?
O23 Mo6 O10 Th2 47(2) 2_655 . . 2 ?
Mo5 Mo6 O10 Th2 -34(2) . . . 2 ?
Th2 Mo6 O10 Th2 90(2) . . . 2 ?
K2 Mo6 O10 Th2 -151(3) . . . 2 ?
K2 Mo6 O10 Th2 153.7(18) 2_545 . . 2 ?
Sr1 Mo6 O10 Th2 -107(2) 2_545 . . 2 ?
O17 Mo6 O10 K2 18.8(9) . . . . ?
O7 Mo6 O10 K2 -83.4(8) . . . . ?
O20 Mo6 O10 K2 149.4(19) . . . . ?
O14 Mo6 O10 K2 122.3(8) . . . . ?
O23 Mo6 O10 K2 -162.0(8) 2_655 . . . ?
Mo5 Mo6 O10 K2 116.9(5) . . . . ?
Th2 Mo6 O10 K2 -119.1(6) . . . . ?
K2 Mo6 O10 K2 -55.4(8) 2_545 . . . ?
Sr1 Mo6 O10 K2 43.8(6) 2_545 . . . ?
O19 Mo4 O11 Sr1 -108.9(15) . . . 1_665 ?
O8 Mo4 O11 Sr1 148.1(15) . . . 1_665 ?
O2 Mo4 O11 Sr1 -9.6(17) . . . 1_665 ?
O1 Mo4 O11 Sr1 65.0(15) 1_655 . . 1_665 ?
O13 Mo4 O11 Sr1 87(6) . . . 1_665 ?
Mo3 Mo4 O11 Sr1 29.0(14) 1_655 . . 1_665 ?
Th1 Mo4 O11 Sr1 106.0(14) 2_666 . . 1_665 ?
Th1 Mo4 O11 Sr1 158.5(8) . . . 1_665 ?
K2 Mo4 O11 Sr1 -122.5(18) 2 . . 1_665 ?
O19 Mo4 O11 K2 13.6(10) . . . 2 ?
O8 Mo4 O11 K2 -89.4(8) . . . 2 ?
O2 Mo4 O11 K2 112.9(8) . . . 2 ?
O1 Mo4 O11 K2 -172.5(8) 1_655 . . 2 ?
O13 Mo4 O11 K2 -150(5) . . . 2 ?
Mo3 Mo4 O11 K2 151.5(6) 1_655 . . 2 ?
Th1 Mo4 O11 K2 -131.6(7) 2_666 . . 2 ?
Th1 Mo4 O11 K2 -79.0(10) . . . 2 ?
O15 Mo2 O12 Mo1 -69.5(9) . . . 1_455 ?
O6 Mo2 O12 Mo1 70(2) . . . 1_455 ?
O9 Mo2 O12 Mo1 -172.8(9) . . . 1_455 ?
O3 Mo2 O12 Mo1 18.4(8) 1_455 . . 1_455 ?
O4 Mo2 O12 Mo1 99.9(8) . . . 1_455 ?
K1 Mo2 O12 Mo1 -118.9(6) . . . 1_455 ?
Th2 Mo2 O12 Mo1 101.1(6) . . . 1_455 ?
Sr1 Mo2 O12 Mo1 14.4(10) . . . 1_455 ?
O15 Mo2 O12 Mo3 179.2(8) . . . . ?
O6 Mo2 O12 Mo3 -41(2) . . . . ?
O9 Mo2 O12 Mo3 75.9(9) . . . . ?
O3 Mo2 O12 Mo3 -92.9(9) 1_455 . . . ?
O4 Mo2 O12 Mo3 -11.4(7) . . . . ?
Mo1 Mo2 O12 Mo3 -111.3(10) 1_455 . . . ?
K1 Mo2 O12 Mo3 129.8(5) . . . . ?
Th2 Mo2 O12 Mo3 -10.2(8) . . . . ?
Sr1 Mo2 O12 Mo3 -96.9(6) . . . . ?
O15 Mo2 O12 K1 56.0(14) . . . 2_556 ?
O6 Mo2 O12 K1 -164.5(15) . . . 2_556 ?
O9 Mo2 O12 K1 -47.2(14) . . . 2_556 ?
O3 Mo2 O12 K1 144.0(14) 1_455 . . 2_556 ?
O4 Mo2 O12 K1 -134.5(14) . . . 2_556 ?
Mo1 Mo2 O12 K1 125.5(17) 1_455 . . 2_556 ?
K1 Mo2 O12 K1 6.7(17) . . . 2_556 ?
Th2 Mo2 O12 K1 -133.3(11) . . . 2_556 ?
Sr1 Mo2 O12 K1 139.9(10) . . . 2_556 ?
O18 Mo3 O12 Mo2 45(5) . . . . ?
O24 Mo3 O12 Mo2 -86.4(10) . . . . ?
O4 Mo3 O12 Mo2 12.9(8) . . . . ?
O1 Mo3 O12 Mo2 177.7(9) . . . . ?
O2 Mo3 O12 Mo2 102.8(9) 1_455 . . . ?
Mo4 Mo3 O12 Mo2 137.8(6) 1_455 . . . ?
K1 Mo3 O12 Mo2 -104.9(6) 1_565 . . . ?
K1 Mo3 O12 Mo2 -143.8(11) 2_556 . . . ?
O18 Mo3 O12 Mo1 -57(5) . . . 1_455 ?
O24 Mo3 O12 Mo1 171.2(11) . . . 1_455 ?
O4 Mo3 O12 Mo1 -89.5(9) . . . 1_455 ?
O1 Mo3 O12 Mo1 75.3(9) . . . 1_455 ?
O2 Mo3 O12 Mo1 0.4(8) 1_455 . . 1_455 ?
Mo4 Mo3 O12 Mo1 35.4(7) 1_455 . . 1_455 ?
K1 Mo3 O12 Mo1 152.7(4) 1_565 . . 1_455 ?
K1 Mo3 O12 Mo1 113.8(11) 2_556 . . 1_455 ?
O18 Mo3 O12 K1 -171(5) . . . 2_556 ?
O24 Mo3 O12 K1 57.4(9) . . . 2_556 ?
O4 Mo3 O12 K1 156.8(9) . . . 2_556 ?
O1 Mo3 O12 K1 -38.4(8) . . . 2_556 ?
O2 Mo3 O12 K1 -113.3(9) 1_455 . . 2_556 ?
Mo4 Mo3 O12 K1 -78.4(6) 1_455 . . 2_556 ?
K1 Mo3 O12 K1 38.9(9) 1_565 . . 2_556 ?
O21 Mo1 O13 Mo4 -68.6(9) . . . . ?
O5 Mo1 O13 Mo4 -176.7(8) . . . . ?
O3 Mo1 O13 Mo4 37(2) . . . . ?
O12 Mo1 O13 Mo4 85.9(8) 1_655 . . . ?
O2 Mo1 O13 Mo4 14.1(7) . . . . ?
Mo2 Mo1 O13 Mo4 84.8(8) 1_655 . . . ?
K1 Mo1 O13 Mo4 114.8(9) 2_656 . . . ?
K1 Mo1 O13 Mo4 -142.9(6) . . . . ?
O21 Mo1 O13 Th1 80.0(17) . . . . ?
O5 Mo1 O13 Th1 -28.1(18) . . . . ?
O3 Mo1 O13 Th1 -174.7(14) . . . . ?
O12 Mo1 O13 Th1 -125.5(17) 1_655 . . . ?
O2 Mo1 O13 Th1 162.7(18) . . . . ?
Mo2 Mo1 O13 Th1 -126.6(14) 1_655 . . . ?
K1 Mo1 O13 Th1 -96.6(17) 2_656 . . . ?
K1 Mo1 O13 Th1 5.7(16) . . . . ?
O21 Mo1 O13 K1 176.6(7) . . . 2_656 ?
O5 Mo1 O13 K1 68.5(8) . . . 2_656 ?
O3 Mo1 O13 K1 -78.1(17) . . . 2_656 ?
O12 Mo1 O13 K1 -29.0(7) 1_655 . . 2_656 ?
O2 Mo1 O13 K1 -100.8(7) . . . 2_656 ?
Mo2 Mo1 O13 K1 -30.0(8) 1_655 . . 2_656 ?
K1 Mo1 O13 K1 102.2(4) . . . 2_656 ?
O11 Mo4 O13 Mo1 -116(6) . . . . ?
O19 Mo4 O13 Mo1 80.0(10) . . . . ?
O8 Mo4 O13 Mo1 -178.2(9) . . . . ?
O2 Mo4 O13 Mo1 -16.9(8) . . . . ?
O1 Mo4 O13 Mo1 -93.2(9) 1_655 . . . ?
Mo3 Mo4 O13 Mo1 -57.0(6) 1_655 . . . ?
Th1 Mo4 O13 Mo1 -134.3(6) 2_666 . . . ?
Th1 Mo4 O13 Mo1 163.1(12) . . . . ?
K2 Mo4 O13 Mo1 98.3(8) 2 . . . ?
O11 Mo4 O13 Th1 81(6) . . . . ?
O19 Mo4 O13 Th1 -83.1(8) . . . . ?
O8 Mo4 O13 Th1 18.7(7) . . . . ?
O2 Mo4 O13 Th1 -180.0(9) . . . . ?
O1 Mo4 O13 Th1 103.7(8) 1_655 . . . ?
Mo3 Mo4 O13 Th1 139.9(6) 1_655 . . . ?
Th1 Mo4 O13 Th1 62.6(5) 2_666 . . . ?
K2 Mo4 O13 Th1 -64.8(9) 2 . . . ?
O11 Mo4 O13 K1 -13(6) . . . 2_656 ?
O19 Mo4 O13 K1 -177.3(9) . . . 2_656 ?
O8 Mo4 O13 K1 -75.5(8) . . . 2_656 ?
O2 Mo4 O13 K1 85.8(8) . . . 2_656 ?
O1 Mo4 O13 K1 9.5(7) 1_655 . . 2_656 ?
Mo3 Mo4 O13 K1 45.6(5) 1_655 . . 2_656 ?
Th1 Mo4 O13 K1 -31.7(6) 2_666 . . 2_656 ?
Th1 Mo4 O13 K1 -94.2(8) . . . 2_656 ?
K2 Mo4 O13 K1 -159.0(3) 2 . . 2_656 ?
O24 Th1 O13 Mo1 -103.7(17) . . . . ?
O9 Th1 O13 Mo1 -39.0(16) . . . . ?
O15 Th1 O13 Mo1 7(2) 2_556 . . . ?
O1 Th1 O13 Mo1 163.8(13) 2_566 . . . ?
O8 Th1 O13 Mo1 -164.4(19) . . . . ?
O5 Th1 O13 Mo1 53.0(16) 2_656 . . . ?
O8 Th1 O13 Mo1 131.4(17) 2_666 . . . ?
Mo4 Th1 O13 Mo1 129.3(15) 2_666 . . . ?
Mo4 Th1 O13 Mo1 -149(2) . . . . ?
K1 Th1 O13 Mo1 98.4(17) 2_656 . . . ?
K1 Th1 O13 Mo1 -151.1(15) 1_565 . . . ?
O24 Th1 O13 Mo4 45.4(9) . . . . ?
O9 Th1 O13 Mo4 110.1(8) . . . . ?
O15 Th1 O13 Mo4 156.1(8) 2_556 . . . ?
O1 Th1 O13 Mo4 -47.2(13) 2_566 . . . ?
O8 Th1 O13 Mo4 -15.3(6) . . . . ?
O5 Th1 O13 Mo4 -157.9(8) 2_656 . . . ?
O8 Th1 O13 Mo4 -79.5(7) 2_666 . . . ?
Mo4 Th1 O13 Mo4 -81.7(6) 2_666 . . . ?
K1 Th1 O13 Mo4 -112.5(7) 2_656 . . . ?
K1 Th1 O13 Mo4 -2.1(7) 1_565 . . . ?
O24 Th1 O13 K1 157.9(6) . . . 2_656 ?
O9 Th1 O13 K1 -137.4(6) . . . 2_656 ?
O15 Th1 O13 K1 -91.4(9) 2_556 . . 2_656 ?
O1 Th1 O13 K1 65.3(11) 2_566 . . 2_656 ?
O8 Th1 O13 K1 97.2(6) . . . 2_656 ?
O5 Th1 O13 K1 -45.4(5) 2_656 . . 2_656 ?
O8 Th1 O13 K1 33.0(6) 2_666 . . 2_656 ?
Mo4 Th1 O13 K1 30.9(6) 2_666 . . 2_656 ?
Mo4 Th1 O13 K1 112.5(7) . . . 2_656 ?
K1 Th1 O13 K1 110.4(3) 1_565 . . 2_656 ?
O22 Mo5 O14 Mo6 79.9(11) . . . . ?
O16 Mo5 O14 Mo6 -69(2) . . . . ?
O23 Mo5 O14 Mo6 -178.1(9) . . . . ?
O20 Mo5 O14 Mo6 -18.0(8) . . . . ?
O14 Mo5 O14 Mo6 -102.5(11) 2_655 . . . ?
Sr1 Mo5 O14 Mo6 -6.2(11) 1_655 . . . ?
O22 Mo5 O14 Mo5 -177.6(10) . . . 2_655 ?
O16 Mo5 O14 Mo5 34(2) . . . 2_655 ?
O23 Mo5 O14 Mo5 -75.6(9) . . . 2_655 ?
O20 Mo5 O14 Mo5 84.5(10) . . . 2_655 ?
O14 Mo5 O14 Mo5 -0.002(1) 2_655 . . 2_655 ?
Mo6 Mo5 O14 Mo5 102.5(11) . . . 2_655 ?
Sr1 Mo5 O14 Mo5 96.3(8) 1_655 . . 2_655 ?
O17 Mo6 O14 Mo5 -75.1(10) . . . . ?
O10 Mo6 O14 Mo5 -172.9(9) . . . . ?
O7 Mo6 O14 Mo5 77(2) . . . . ?
O20 Mo6 O14 Mo5 17.9(8) . . . . ?
O23 Mo6 O14 Mo5 100.7(9) 2_655 . . . ?
Th2 Mo6 O14 Mo5 105.4(7) . . . . ?
K2 Mo6 O14 Mo5 -126.3(6) . . . . ?
K2 Mo6 O14 Mo5 3.0(17) 2_545 . . . ?
Sr1 Mo6 O14 Mo5 -69.6(7) 2_545 . . . ?
O17 Mo6 O14 Mo5 174.7(8) . . . 2_655 ?
O10 Mo6 O14 Mo5 76.9(8) . . . 2_655 ?
O7 Mo6 O14 Mo5 -33(2) . . . 2_655 ?
O20 Mo6 O14 Mo5 -92.2(9) . . . 2_655 ?
O23 Mo6 O14 Mo5 -9.5(7) 2_655 . . 2_655 ?
Mo5 Mo6 O14 Mo5 -110.2(10) . . . 2_655 ?
Th2 Mo6 O14 Mo5 -4.8(9) . . . 2_655 ?
K2 Mo6 O14 Mo5 123.5(5) . . . 2_655 ?
K2 Mo6 O14 Mo5 -107.2(10) 2_545 . . 2_655 ?
Sr1 Mo6 O14 Mo5 -179.7(7) 2_545 . . 2_655 ?
O6 Mo2 O15 Th1 -151.2(19) . . . 2_556 ?
O9 Mo2 O15 Th1 104.2(19) . . . 2_556 ?
O12 Mo2 O15 Th1 12(2) . . . 2_556 ?
O3 Mo2 O15 Th1 -62.6(19) 1_455 . . 2_556 ?
O4 Mo2 O15 Th1 -44(5) . . . 2_556 ?
Mo1 Mo2 O15 Th1 -27.6(18) 1_455 . . 2_556 ?
K1 Mo2 O15 Th1 149(2) . . . 2_556 ?
Th2 Mo2 O15 Th1 -154.9(12) . . . 2_556 ?
Sr1 Mo2 O15 Th1 -107.8(19) . . . 2_556 ?
O6 Mo2 O15 K1 60.3(8) . . . . ?
O9 Mo2 O15 K1 -44.3(9) . . . . ?
O12 Mo2 O15 K1 -136.7(7) . . . . ?
O3 Mo2 O15 K1 148.9(8) 1_455 . . . ?
O4 Mo2 O15 K1 167(3) . . . . ?
Mo1 Mo2 O15 K1 -176.1(5) 1_455 . . . ?
Th2 Mo2 O15 K1 56.6(11) . . . . ?
Sr1 Mo2 O15 K1 103.7(5) . . . . ?
O22 Mo5 O16 Th2 117(2) . . . 1_655 ?
O23 Mo5 O16 Th2 12(2) . . . 1_655 ?
O20 Mo5 O16 Th2 -143(2) . . . 1_655 ?
O14 Mo5 O16 Th2 -94(3) . . . 1_655 ?
O14 Mo5 O16 Th2 -62(2) 2_655 . . 1_655 ?
Mo6 Mo5 O16 Th2 -139.7(17) . . . 1_655 ?
Sr1 Mo5 O16 Th2 -180(3) 1_655 . . 1_655 ?
O22 Mo5 O16 Sr1 -62.7(11) . . . 1_655 ?
O23 Mo5 O16 Sr1 -168.3(8) . . . 1_655 ?
O20 Mo5 O16 Sr1 36.7(9) . . . 1_655 ?
O14 Mo5 O16 Sr1 85.5(19) . . . 1_655 ?
O14 Mo5 O16 Sr1 117.7(9) 2_655 . . 1_655 ?
Mo6 Mo5 O16 Sr1 40.3(10) . . . 1_655 ?
O10 Mo6 O17 Sr1 102.3(16) . . . 2_545 ?
O7 Mo6 O17 Sr1 -154.8(15) . . . 2_545 ?
O20 Mo6 O17 Sr1 -60.2(17) . . . 2_545 ?
O14 Mo6 O17 Sr1 13.0(17) . . . 2_545 ?
O23 Mo6 O17 Sr1 -67(13) 2_655 . . 2_545 ?
Mo5 Mo6 O17 Sr1 -23.5(15) . . . 2_545 ?
Th2 Mo6 O17 Sr1 -167.6(8) . . . 2_545 ?
K2 Mo6 O17 Sr1 122.0(19) . . . 2_545 ?
K2 Mo6 O17 Sr1 -136.5(16) 2_545 . . 2_545 ?
O10 Mo6 O17 K2 -19.6(10) . . . . ?
O7 Mo6 O17 K2 83.2(9) . . . . ?
O20 Mo6 O17 K2 177.8(8) . . . . ?
O14 Mo6 O17 K2 -109.0(8) . . . . ?
O23 Mo6 O17 K2 171(12) 2_655 . . . ?
Mo5 Mo6 O17 K2 -145.5(6) . . . . ?
Th2 Mo6 O17 K2 70.4(11) . . . . ?
K2 Mo6 O17 K2 101.5(7) 2_545 . . . ?
Sr1 Mo6 O17 K2 -122.0(19) 2_545 . . . ?
O24 Mo3 O18 Sr1 -143.2(13) . . . 1_565 ?
O4 Mo3 O18 Sr1 117.9(13) . . . 1_565 ?
O1 Mo3 O18 Sr1 -44.6(14) . . . 1_565 ?
O2 Mo3 O18 Sr1 31.1(14) 1_455 . . 1_565 ?
O12 Mo3 O18 Sr1 86(5) . . . 1_565 ?
Mo4 Mo3 O18 Sr1 -5.0(12) 1_455 . . 1_565 ?
K1 Mo3 O18 Sr1 -120.0(14) 1_565 . . 1_565 ?
K1 Mo3 O18 Sr1 -81.6(17) 2_556 . . 1_565 ?
O24 Mo3 O18 K2 61.5(17) . . . 2 ?
O4 Mo3 O18 K2 -37.4(16) . . . 2 ?
O1 Mo3 O18 K2 160.1(14) . . . 2 ?
O2 Mo3 O18 K2 -124.2(14) 1_455 . . 2 ?
O12 Mo3 O18 K2 -69(5) . . . 2 ?
Mo4 Mo3 O18 K2 -160.3(13) 1_455 . . 2 ?
K1 Mo3 O18 K2 84.7(14) 1_565 . . 2 ?
K1 Mo3 O18 K2 123.0(13) 2_556 . . 2 ?
O24 Mo3 O18 K1 -23.2(10) . . . 1_565 ?
O4 Mo3 O18 K1 -122.1(7) . . . 1_565 ?
O1 Mo3 O18 K1 75.3(8) . . . 1_565 ?
O2 Mo3 O18 K1 151.1(7) 1_455 . . 1_565 ?
O12 Mo3 O18 K1 -154(5) . . . 1_565 ?
Mo4 Mo3 O18 K1 115.0(4) 1_455 . . 1_565 ?
K1 Mo3 O18 K1 38.3(16) 2_556 . . 1_565 ?
O11 Mo4 O19 Th2 122(2) . . . . ?
O8 Mo4 O19 Th2 -138(2) . . . . ?
O2 Mo4 O19 Th2 15(2) . . . . ?
O1 Mo4 O19 Th2 -35(5) 1_655 . . . ?
O13 Mo4 O19 Th2 -61(2) . . . . ?
Mo3 Mo4 O19 Th2 17(3) 1_655 . . . ?
Th1 Mo4 O19 Th2 -151.7(13) 2_666 . . . ?
Th1 Mo4 O19 Th2 -100(2) . . . . ?
K2 Mo4 O19 Th2 135(2) 2 . . . ?
O11 Mo4 O19 K2 -13.1(10) . . . 2 ?
O8 Mo4 O19 K2 87.3(8) . . . 2 ?
O2 Mo4 O19 K2 -119.4(8) . . . 2 ?
O1 Mo4 O19 K2 -169(3) 1_655 . . 2 ?
O13 Mo4 O19 K2 164.5(8) . . . 2 ?
Mo3 Mo4 O19 K2 -117.5(7) 1_655 . . 2 ?
Th1 Mo4 O19 K2 73.6(13) 2_666 . . 2 ?
Th1 Mo4 O19 K2 124.8(6) . . . 2 ?
O10 Th2 O19 Mo4 -136(2) 2 . . . ?
O16 Th2 O19 Mo4 175.6(17) 1_455 . . . ?
O23 Th2 O19 Mo4 -59(2) 2_655 . . . ?
O7 Th2 O19 Mo4 -14(3) . . . . ?
O21 Th2 O19 Mo4 24(2) . . . . ?
O6 Th2 O19 Mo4 86(2) . . . . ?
O4 Th2 O19 Mo4 136(2) . . . . ?
Mo6 Th2 O19 Mo4 -44(2) . . . . ?
Mo2 Th2 O19 Mo4 103(2) . . . . ?
K2 Th2 O19 Mo4 -134(3) 2 . . . ?
Sr1 Th2 O19 Mo4 111(2) . . . . ?
O10 Th2 O19 K2 -2.8(7) 2 . . 2 ?
O16 Th2 O19 K2 -50.7(17) 1_455 . . 2 ?
O23 Th2 O19 K2 75.0(7) 2_655 . . 2 ?
O7 Th2 O19 K2 119.9(9) . . . 2 ?
O21 Th2 O19 K2 157.7(9) . . . 2 ?
O6 Th2 O19 K2 -140.5(7) . . . 2 ?
O4 Th2 O19 K2 -90.1(8) . . . 2 ?
Mo6 Th2 O19 K2 89.2(7) . . . 2 ?
Mo2 Th2 O19 K2 -122.9(6) . . . 2 ?
Sr1 Th2 O19 K2 -115.0(7) . . . 2 ?
O22 Mo5 O20 Mo6 -80.2(11) . . . . ?
O16 Mo5 O20 Mo6 175.1(11) . . . . ?
O23 Mo5 O20 Mo6 72(2) . . . . ?
O14 Mo5 O20 Mo6 18.9(9) . . . . ?
O14 Mo5 O20 Mo6 93.0(10) 2_655 . . . ?
Sr1 Mo5 O20 Mo6 -147.7(13) 1_655 . . . ?
O22 Mo5 O20 Sr1 67.5(10) . . . 1_655 ?
O16 Mo5 O20 Sr1 -37.2(9) . . . 1_655 ?
O23 Mo5 O20 Sr1 -140.5(17) . . . 1_655 ?
O14 Mo5 O20 Sr1 166.6(10) . . . 1_655 ?
O14 Mo5 O20 Sr1 -119.3(8) 2_655 . . 1_655 ?
Mo6 Mo5 O20 Sr1 147.7(13) . . . 1_655 ?
O17 Mo6 O20 Mo5 83.8(11) . . . . ?
O10 Mo6 O20 Mo5 -47(3) . . . . ?
O7 Mo6 O20 Mo5 -175.5(10) . . . . ?
O14 Mo6 O20 Mo5 -18.3(9) . . . . ?
O23 Mo6 O20 Mo5 -96.6(10) 2_655 . . . ?
Th2 Mo6 O20 Mo5 -136.0(8) . . . . ?
K2 Mo6 O20 Mo5 86.8(14) . . . . ?
K2 Mo6 O20 Mo5 154.2(10) 2_545 . . . ?
Sr1 Mo6 O20 Mo5 62.3(8) 2_545 . . . ?
O17 Mo6 O20 Sr1 -40.7(18) . . . 1_655 ?
O10 Mo6 O20 Sr1 -171.5(16) . . . 1_655 ?
O7 Mo6 O20 Sr1 60.0(16) . . . 1_655 ?
O14 Mo6 O20 Sr1 -142.8(18) . . . 1_655 ?
O23 Mo6 O20 Sr1 138.9(17) 2_655 . . 1_655 ?
Mo5 Mo6 O20 Sr1 -125(2) . . . 1_655 ?
Th2 Mo6 O20 Sr1 99.5(15) . . . 1_655 ?
K2 Mo6 O20 Sr1 -38(2) . . . 1_655 ?
K2 Mo6 O20 Sr1 29.7(14) 2_545 . . 1_655 ?
Sr1 Mo6 O20 Sr1 -62.2(15) 2_545 . . 1_655 ?
O5 Mo1 O21 Th2 131(2) . . . . ?
O3 Mo1 O21 Th2 -127(2) . . . . ?
O13 Mo1 O21 Th2 26(2) . . . . ?
O12 Mo1 O21 Th2 -65(3) 1_655 . . . ?
O2 Mo1 O21 Th2 -46(2) . . . . ?
Mo2 Mo1 O21 Th2 -124(2) 1_655 . . . ?
K1 Mo1 O21 Th2 32(3) 2_656 . . . ?
K1 Mo1 O21 Th2 115(2) . . . . ?
O10 Th2 O21 Mo1 42(3) 2 . . . ?
O16 Th2 O21 Mo1 -155(2) 1_455 . . . ?
O19 Th2 O21 Mo1 4(2) . . . . ?
O23 Th2 O21 Mo1 89(2) 2_655 . . . ?
O7 Th2 O21 Mo1 158(3) . . . . ?
O6 Th2 O21 Mo1 -116(2) . . . . ?
O4 Th2 O21 Mo1 -60(2) . . . . ?
Mo6 Th2 O21 Mo1 130(2) . . . . ?
Mo2 Th2 O21 Mo1 -88(2) . . . . ?
K2 Th2 O21 Mo1 20(2) 2 . . . ?
Sr1 Th2 O21 Mo1 -137(2) . . . . ?
O16 Mo5 O22 Sr1 134.9(16) . . . 2_545 ?
O23 Mo5 O22 Sr1 -120.6(15) . . . 2_545 ?
O20 Mo5 O22 Sr1 47.6(17) . . . 2_545 ?
O14 Mo5 O22 Sr1 -28.9(17) . . . 2_545 ?
O14 Mo5 O22 Sr1 -49(9) 2_655 . . 2_545 ?
Mo6 Mo5 O22 Sr1 10.4(15) . . . 2_545 ?
Sr1 Mo5 O22 Sr1 92.0(15) 1_655 . . 2_545 ?
O16 Mo5 O22 K2 -64.0(15) . . . 1_655 ?
O23 Mo5 O22 K2 40.5(14) . . . 1_655 ?
O20 Mo5 O22 K2 -151.4(12) . . . 1_655 ?
O14 Mo5 O22 K2 132.2(13) . . . 1_655 ?
O14 Mo5 O22 K2 112(8) 2_655 . . 1_655 ?
Mo6 Mo5 O22 K2 171.5(12) . . . 1_655 ?
Sr1 Mo5 O22 K2 -106.9(12) 1_655 . . 1_655 ?
O22 Mo5 O23 Mo6 -175.7(9) . . . 2_655 ?
O16 Mo5 O23 Mo6 -67.4(11) . . . 2_655 ?
O20 Mo5 O23 Mo6 32(2) . . . 2_655 ?
O14 Mo5 O23 Mo6 82.8(9) . . . 2_655 ?
O14 Mo5 O23 Mo6 10.9(8) 2_655 . . 2_655 ?
Mo6 Mo5 O23 Mo6 81.2(9) . . . 2_655 ?
Sr1 Mo5 O23 Mo6 -84.2(13) 1_655 . . 2_655 ?
O22 Mo5 O23 Th2 -34(2) . . . 2_655 ?
O16 Mo5 O23 Th2 74.4(19) . . . 2_655 ?
O20 Mo5 O23 Th2 174.3(15) . . . 2_655 ?
O14 Mo5 O23 Th2 -135.4(18) . . . 2_655 ?
O14 Mo5 O23 Th2 152.7(19) 2_655 . . 2_655 ?
Mo6 Mo5 O23 Th2 -137.0(14) . . . 2_655 ?
Sr1 Mo5 O23 Th2 58(2) 1_655 . . 2_655 ?
O18 Mo3 O24 Th1 -114(3) . . . . ?
O4 Mo3 O24 Th1 -15(3) . . . . ?
O1 Mo3 O24 Th1 143(2) . . . . ?
O2 Mo3 O24 Th1 80(4) 1_455 . . . ?
O12 Mo3 O24 Th1 58(2) . . . . ?
Mo4 Mo3 O24 Th1 135(2) 1_455 . . . ?
K1 Mo3 O24 Th1 -142(3) 1_565 . . . ?
K1 Mo3 O24 Th1 98(3) 2_556 . . . ?
O18 Mo3 O24 K1 28.2(12) . . . 1_565 ?
O4 Mo3 O24 K1 127.1(9) . . . 1_565 ?
O1 Mo3 O24 K1 -75.4(10) . . . 1_565 ?
O2 Mo3 O24 K1 -138.1(18) 1_455 . . 1_565 ?
O12 Mo3 O24 K1 -159.9(9) . . . 1_565 ?
Mo4 Mo3 O24 K1 -83.1(11) 1_455 . . 1_565 ?
K1 Mo3 O24 K1 -120.4(9) 2_556 . . 1_565 ?
O13 Th1 O24 Mo3 51(3) . . . . ?
O9 Th1 O24 Mo3 -16(2) . . . . ?
O15 Th1 O24 Mo3 -90(3) 2_556 . . . ?
O1 Th1 O24 Mo3 -167(3) 2_566 . . . ?
O8 Th1 O24 Mo3 107(3) . . . . ?
O5 Th1 O24 Mo3 -51(4) 2_656 . . . ?
O8 Th1 O24 Mo3 148(2) 2_666 . . . ?
Mo4 Th1 O24 Mo3 -179(2) 2_666 . . . ?
Mo4 Th1 O24 Mo3 77(3) . . . . ?
K1 Th1 O24 Mo3 97(3) 2_656 . . . ?
K1 Th1 O24 Mo3 143(3) 1_565 . . . ?
O13 Th1 O24 K1 -91.3(8) . . . 1_565 ?
O9 Th1 O24 K1 -158.6(9) . . . 1_565 ?
O15 Th1 O24 K1 127.3(8) 2_556 . . 1_565 ?
O1 Th1 O24 K1 50.1(7) 2_566 . . 1_565 ?
O8 Th1 O24 K1 -35.8(7) . . . 1_565 ?
O5 Th1 O24 K1 166.7(14) 2_656 . . 1_565 ?
O8 Th1 O24 K1 5.5(11) 2_666 . . 1_565 ?
Mo4 Th1 O24 K1 38.6(8) 2_666 . . 1_565 ?
Mo4 Th1 O24 K1 -65.4(6) . . . 1_565 ?
K1 Th1 O24 K1 -45.4(16) 2_656 . . 1_565 ?
Mo2 O6 Sr1 O17 -170.6(9) . . . 2_545 ?
Th2 O6 Sr1 O17 70.9(8) . . . 2_545 ?
K1 O6 Sr1 O17 -89.4(8) . . . 2_545 ?
Mo2 O6 Sr1 O11 -35.7(11) . . . 1_445 ?
Th2 O6 Sr1 O11 -154.2(7) . . . 1_445 ?
K1 O6 Sr1 O11 45.5(9) . . . 1_445 ?
Mo2 O6 Sr1 O3 21.9(8) . . . 1_455 ?
Th2 O6 Sr1 O3 -96.6(9) . . . 1_455 ?
K1 O6 Sr1 O3 103.1(9) . . . 1_455 ?
Mo2 O6 Sr1 O22 -116(4) . . . 2_545 ?
Th2 O6 Sr1 O22 126(4) . . . 2_545 ?
K1 O6 Sr1 O22 -35(4) . . . 2_545 ?
Mo2 O6 Sr1 O20 77.5(10) . . . 1_455 ?
Th2 O6 Sr1 O20 -41.0(9) . . . 1_455 ?
K1 O6 Sr1 O20 158.7(7) . . . 1_455 ?
Mo2 O6 Sr1 O16 111.2(10) . . . 1_455 ?
Th2 O6 Sr1 O16 -7.3(7) . . . 1_455 ?
K1 O6 Sr1 O16 -167.6(10) . . . 1_455 ?
Mo2 O6 Sr1 O18 -102.6(10) . . . 1_545 ?
Th2 O6 Sr1 O18 138.9(9) . . . 1_545 ?
K1 O6 Sr1 O18 -21.4(7) . . . 1_545 ?
Mo2 O6 Sr1 Mo5 107.2(8) . . . 1_455 ?
Th2 O6 Sr1 Mo5 -11.3(7) . . . 1_455 ?
K1 O6 Sr1 Mo5 -171.5(6) . . . 1_455 ?
Th2 O6 Sr1 Mo2 -118.5(12) . . . . ?
K1 O6 Sr1 Mo2 81.2(9) . . . . ?
Mo2 O6 Sr1 Mo6 -160.7(6) . . . 2_545 ?
Th2 O6 Sr1 Mo6 80.8(7) . . . 2_545 ?
K1 O6 Sr1 Mo6 -79.4(7) . . . 2_545 ?
Mo2 O6 Sr1 K2 -153.1(10) . . . 2_545 ?
Th2 O6 Sr1 K2 88.4(7) . . . 2_545 ?
K1 O6 Sr1 K2 -71.9(6) . . . 2_545 ?
O15 Mo2 Sr1 O17 -102.9(9) . . . 2_545 ?
O6 Mo2 Sr1 O17 11.2(11) . . . 2_545 ?
O9 Mo2 Sr1 O17 -4.4(14) . . . 2_545 ?
O12 Mo2 Sr1 O17 161.9(9) . . . 2_545 ?
O3 Mo2 Sr1 O17 156.4(10) 1_455 . . 2_545 ?
O4 Mo2 Sr1 O17 88.2(8) . . . 2_545 ?
Mo1 Mo2 Sr1 O17 171.7(6) 1_455 . . 2_545 ?
K1 Mo2 Sr1 O17 -50.6(6) . . . 2_545 ?
Th2 Mo2 Sr1 O17 48.7(6) . . . 2_545 ?
O15 Mo2 Sr1 O11 32.7(9) . . . 1_445 ?
O6 Mo2 Sr1 O11 146.8(10) . . . 1_445 ?
O9 Mo2 Sr1 O11 131.2(13) . . . 1_445 ?
O12 Mo2 Sr1 O11 -62.6(8) . . . 1_445 ?
O3 Mo2 Sr1 O11 -68.0(9) 1_455 . . 1_445 ?
O4 Mo2 Sr1 O11 -136.3(7) . . . 1_445 ?
Mo1 Mo2 Sr1 O11 -52.8(5) 1_455 . . 1_445 ?
K1 Mo2 Sr1 O11 85.0(5) . . . 1_445 ?
Th2 Mo2 Sr1 O11 -175.7(5) . . . 1_445 ?
O15 Mo2 Sr1 O3 100.7(11) . . . 1_455 ?
O6 Mo2 Sr1 O3 -145.2(12) . . . 1_455 ?
O9 Mo2 Sr1 O3 -160.8(15) . . . 1_455 ?
O12 Mo2 Sr1 O3 5.5(10) . . . 1_455 ?
O4 Mo2 Sr1 O3 -68.3(10) . . . 1_455 ?
Mo1 Mo2 Sr1 O3 15.3(8) 1_455 . . 1_455 ?
K1 Mo2 Sr1 O3 153.0(8) . . . 1_455 ?
Th2 Mo2 Sr1 O3 -107.7(8) . . . 1_455 ?
O15 Mo2 Sr1 O22 44.4(15) . . . 2_545 ?
O6 Mo2 Sr1 O22 158.6(16) . . . 2_545 ?
O9 Mo2 Sr1 O22 142.9(18) . . . 2_545 ?
O12 Mo2 Sr1 O22 -50.8(15) . . . 2_545 ?
O3 Mo2 Sr1 O22 -56.3(15) 1_455 . . 2_545 ?
O4 Mo2 Sr1 O22 -124.5(14) . . . 2_545 ?
Mo1 Mo2 Sr1 O22 -41.0(13) 1_455 . . 2_545 ?
K1 Mo2 Sr1 O22 96.7(13) . . . 2_545 ?
Th2 Mo2 Sr1 O22 -164.0(13) . . . 2_545 ?
O15 Mo2 Sr1 O20 136.4(9) . . . 1_455 ?
O6 Mo2 Sr1 O20 -109.5(10) . . . 1_455 ?
O9 Mo2 Sr1 O20 -125.1(13) . . . 1_455 ?
O12 Mo2 Sr1 O20 41.2(8) . . . 1_455 ?
O3 Mo2 Sr1 O20 35.7(9) 1_455 . . 1_455 ?
O4 Mo2 Sr1 O20 -32.5(7) . . . 1_455 ?
Mo1 Mo2 Sr1 O20 51.0(5) 1_455 . . 1_455 ?
K1 Mo2 Sr1 O20 -171.3(5) . . . 1_455 ?
Th2 Mo2 Sr1 O20 -72.0(5) . . . 1_455 ?
O15 Mo2 Sr1 O16 -173.2(9) . . . 1_455 ?
O6 Mo2 Sr1 O16 -59.1(10) . . . 1_455 ?
O9 Mo2 Sr1 O16 -74.7(13) . . . 1_455 ?
O12 Mo2 Sr1 O16 91.6(8) . . . 1_455 ?
O3 Mo2 Sr1 O16 86.1(9) 1_455 . . 1_455 ?
O4 Mo2 Sr1 O16 17.8(7) . . . 1_455 ?
Mo1 Mo2 Sr1 O16 101.4(5) 1_455 . . 1_455 ?
K1 Mo2 Sr1 O16 -120.9(5) . . . 1_455 ?
Th2 Mo2 Sr1 O16 -21.6(5) . . . 1_455 ?
O15 Mo2 Sr1 O6 -114.1(11) . . . . ?
O9 Mo2 Sr1 O6 -15.6(15) . . . . ?
O12 Mo2 Sr1 O6 150.6(11) . . . . ?
O3 Mo2 Sr1 O6 145.2(12) 1_455 . . . ?
O4 Mo2 Sr1 O6 76.9(10) . . . . ?
Mo1 Mo2 Sr1 O6 160.4(9) 1_455 . . . ?
K1 Mo2 Sr1 O6 -61.8(9) . . . . ?
Th2 Mo2 Sr1 O6 37.5(9) . . . . ?
O15 Mo2 Sr1 O18 -45.3(9) . . . 1_545 ?
O6 Mo2 Sr1 O18 68.8(10) . . . 1_545 ?
O9 Mo2 Sr1 O18 53.2(13) . . . 1_545 ?
O12 Mo2 Sr1 O18 -140.6(8) . . . 1_545 ?
O3 Mo2 Sr1 O18 -146.0(9) 1_455 . . 1_545 ?
O4 Mo2 Sr1 O18 145.7(7) . . . 1_545 ?
Mo1 Mo2 Sr1 O18 -130.8(5) 1_455 . . 1_545 ?
K1 Mo2 Sr1 O18 7.0(5) . . . 1_545 ?
Th2 Mo2 Sr1 O18 106.2(5) . . . 1_545 ?
O15 Mo2 Sr1 Mo5 170.0(7) . . . 1_455 ?
O6 Mo2 Sr1 Mo5 -75.9(9) . . . 1_455 ?
O9 Mo2 Sr1 Mo5 -91.5(12) . . . 1_455 ?
O12 Mo2 Sr1 Mo5 74.7(7) . . . 1_455 ?
O3 Mo2 Sr1 Mo5 69.3(8) 1_455 . . 1_455 ?
O4 Mo2 Sr1 Mo5 1.0(5) . . . 1_455 ?
Mo1 Mo2 Sr1 Mo5 84.55(12) 1_455 . . 1_455 ?
K1 Mo2 Sr1 Mo5 -137.70(17) . . . 1_455 ?
Th2 Mo2 Sr1 Mo5 -38.42(9) . . . 1_455 ?
O15 Mo2 Sr1 Mo6 -87.6(7) . . . 2_545 ?
O6 Mo2 Sr1 Mo6 26.6(9) . . . 2_545 ?
O9 Mo2 Sr1 Mo6 10.9(13) . . . 2_545 ?
O12 Mo2 Sr1 Mo6 177.2(7) . . . 2_545 ?
O3 Mo2 Sr1 Mo6 171.7(8) 1_455 . . 2_545 ?
O4 Mo2 Sr1 Mo6 103.5(6) . . . 2_545 ?
Mo1 Mo2 Sr1 Mo6 -173.0(2) 1_455 . . 2_545 ?
K1 Mo2 Sr1 Mo6 -35.3(3) . . . 2_545 ?
Th2 Mo2 Sr1 Mo6 64.0(2) . . . 2_545 ?
O15 Mo2 Sr1 K2 -91.6(7) . . . 2_545 ?
O6 Mo2 Sr1 K2 22.5(9) . . . 2_545 ?
O9 Mo2 Sr1 K2 6.9(12) . . . 2_545 ?
O12 Mo2 Sr1 K2 173.2(7) . . . 2_545 ?
O3 Mo2 Sr1 K2 167.7(8) 1_455 . . 2_545 ?
O4 Mo2 Sr1 K2 99.4(5) . . . 2_545 ?
Mo1 Mo2 Sr1 K2 -177.04(15) 1_455 . . 2_545 ?
K1 Mo2 Sr1 K2 -39.3(2) . . . 2_545 ?
Th2 Mo2 Sr1 K2 59.99(14) . . . 2_545 ?
Mo2 O15 K1 O12 105.8(8) . . . 2_556 ?
Th1 O15 K1 O12 -56.4(8) 2_556 . . 2_556 ?
Mo2 O15 K1 O8 -122.8(13) . . . 1_545 ?
Th1 O15 K1 O8 75.0(16) 2_556 . . 1_545 ?
Mo2 O15 K1 O5 10.7(12) . . . . ?
Th1 O15 K1 O5 -151.5(7) 2_556 . . . ?
Mo2 O15 K1 O24 -149.1(8) . . . 1_545 ?
Th1 O15 K1 O24 48.7(9) 2_556 . . 1_545 ?
Mo2 O15 K1 O9 28.1(6) . . . . ?
Th1 O15 K1 O9 -134.1(10) 2_556 . . . ?
Mo2 O15 K1 O1 155.1(7) . . . 2_556 ?
Th1 O15 K1 O1 -7.1(10) 2_556 . . 2_556 ?
Mo2 O15 K1 O13 98.3(10) . . . 2_656 ?
Th1 O15 K1 O13 -63.8(12) 2_556 . . 2_656 ?
Mo2 O15 K1 O18 -101.4(9) . . . 1_545 ?
Th1 O15 K1 O18 96.4(9) 2_556 . . 1_545 ?
Mo2 O15 K1 O6 -35.2(6) . . . . ?
Th1 O15 K1 O6 162.7(11) 2_556 . . . ?
Th1 O15 K1 Mo2 -162.2(13) 2_556 . . . ?
Mo2 O15 K1 Mo3 -130.6(8) . . . 1_545 ?
Th1 O15 K1 Mo3 67.2(7) 2_556 . . 1_545 ?
Mo1 O5 K1 O12 -109.2(11) . . . 2_556 ?
Th1 O5 K1 O12 81.6(7) 2_656 . . 2_556 ?
Mo1 O5 K1 O8 135.6(12) . . . 1_545 ?
Th1 O5 K1 O8 -33.5(6) 2_656 . . 1_545 ?
Mo1 O5 K1 O15 -22.5(15) . . . . ?
Th1 O5 K1 O15 168.4(7) 2_656 . . . ?
Mo1 O5 K1 O24 129.8(11) . . . 1_545 ?
Th1 O5 K1 O24 -39.4(10) 2_656 . . 1_545 ?
Mo1 O5 K1 O9 -37.3(10) . . . . ?
Th1 O5 K1 O9 153.5(7) 2_656 . . . ?
Mo1 O5 K1 O1 -168.4(10) . . . 2_556 ?
Th1 O5 K1 O1 22.5(7) 2_656 . . 2_556 ?
Mo1 O5 K1 O13 -149.2(13) . . . 2_656 ?
Th1 O5 K1 O13 41.6(5) 2_656 . . 2_656 ?
Mo1 O5 K1 O18 62.7(13) . . . 1_545 ?
Th1 O5 K1 O18 -106.5(7) 2_656 . . 1_545 ?
Mo1 O5 K1 O6 11.9(11) . . . . ?
Th1 O5 K1 O6 -157.3(6) 2_656 . . . ?
Mo1 O5 K1 Mo2 -16.9(11) . . . . ?
Th1 O5 K1 Mo2 174.0(4) 2_656 . . . ?
Mo1 O5 K1 Mo3 91.0(12) . . . 1_545 ?
Th1 O5 K1 Mo3 -78.2(8) 2_656 . . 1_545 ?
Mo2 O9 K1 O12 -117.2(8) . . . 2_556 ?
Th1 O9 K1 O12 52.3(9) . . . 2_556 ?
Mo2 O9 K1 O8 126.7(11) . . . 1_545 ?
Th1 O9 K1 O8 -63.8(15) . . . 1_545 ?
Mo2 O9 K1 O15 -28.1(7) . . . . ?
Th1 O9 K1 O15 141.4(11) . . . . ?
Mo2 O9 K1 O5 138.8(8) . . . . ?
Th1 O9 K1 O5 -51.7(9) . . . . ?
Mo2 O9 K1 O24 -22.8(16) . . . 1_545 ?
Th1 O9 K1 O24 146.7(11) . . . 1_545 ?
Mo2 O9 K1 O1 -119.1(8) . . . 2_556 ?
Th1 O9 K1 O1 50.3(12) . . . 2_556 ?
Mo2 O9 K1 O13 -166.6(7) . . . 2_656 ?
Th1 O9 K1 O13 2.9(10) . . . 2_656 ?
Mo2 O9 K1 O18 18.6(8) . . . 1_545 ?
Th1 O9 K1 O18 -171.9(8) . . . 1_545 ?
Mo2 O9 K1 O6 37.5(6) . . . . ?
Th1 O9 K1 O6 -153.0(12) . . . . ?
Th1 O9 K1 Mo2 169.5(14) . . . . ?
Mo2 O9 K1 Mo3 -3.8(9) . . . 1_545 ?
Th1 O9 K1 Mo3 165.7(6) . . . 1_545 ?
Mo2 O6 K1 O12 -10.0(9) . . . 2_556 ?
Th2 O6 K1 O12 96.1(11) . . . 2_556 ?
Sr1 O6 K1 O12 -108.9(8) . . . 2_556 ?
Mo2 O6 K1 O8 -178.3(7) . . . 1_545 ?
Th2 O6 K1 O8 -72.2(11) . . . 1_545 ?
Sr1 O6 K1 O8 82.8(9) . . . 1_545 ?
Mo2 O6 K1 O15 36.1(7) . . . . ?
Th2 O6 K1 O15 142.2(12) . . . . ?
Sr1 O6 K1 O15 -62.8(8) . . . . ?
Mo2 O6 K1 O5 -112.0(7) . . . . ?
Th2 O6 K1 O5 -5.9(10) . . . . ?
Sr1 O6 K1 O5 149.1(8) . . . . ?
Mo2 O6 K1 O24 112.4(8) . . . 1_545 ?
Th2 O6 K1 O24 -141.5(10) . . . 1_545 ?
Sr1 O6 K1 O24 13.5(10) . . . 1_545 ?
Mo2 O6 K1 O9 -38.6(6) . . . . ?
Th2 O6 K1 O9 67.5(10) . . . . ?
Sr1 O6 K1 O9 -137.5(10) . . . . ?
Mo2 O6 K1 O1 69(2) . . . 2_556 ?
Th2 O6 K1 O1 174.9(15) . . . 2_556 ?
Sr1 O6 K1 O1 -30(2) . . . 2_556 ?
Mo2 O6 K1 O13 -82.9(11) . . . 2_656 ?
Th2 O6 K1 O13 23.3(16) . . . 2_656 ?
Sr1 O6 K1 O13 178.3(7) . . . 2_656 ?
Mo2 O6 K1 O18 119.5(9) . . . 1_545 ?
Th2 O6 K1 O18 -134.4(12) . . . 1_545 ?
Sr1 O6 K1 O18 20.6(7) . . . 1_545 ?
Th2 O6 K1 Mo2 106.1(12) . . . . ?
Sr1 O6 K1 Mo2 -98.9(9) . . . . ?
Mo2 O6 K1 Mo3 107.7(6) . . . 1_545 ?
Th2 O6 K1 Mo3 -146.1(9) . . . 1_545 ?
Sr1 O6 K1 Mo3 8.8(6) . . . 1_545 ?
O15 Mo2 K1 O12 -71.8(9) . . . 2_556 ?
O6 Mo2 K1 O12 171.4(8) . . . 2_556 ?
O9 Mo2 K1 O12 59.1(8) . . . 2_556 ?
O12 Mo2 K1 O12 -4.6(12) . . . 2_556 ?
O3 Mo2 K1 O12 -118.2(9) 1_455 . . 2_556 ?
O4 Mo2 K1 O12 112.1(8) . . . 2_556 ?
Mo1 Mo2 K1 O12 -66.1(5) 1_455 . . 2_556 ?
Th2 Mo2 K1 O12 140.2(4) . . . 2_556 ?
Sr1 Mo2 K1 O12 -145.6(5) . . . 2_556 ?
O15 Mo2 K1 O8 119.9(13) . . . 1_545 ?
O6 Mo2 K1 O8 3.1(12) . . . 1_545 ?
O9 Mo2 K1 O8 -109.2(13) . . . 1_545 ?
O12 Mo2 K1 O8 -172.9(12) . . . 1_545 ?
O3 Mo2 K1 O8 73.5(14) 1_455 . . 1_545 ?
O4 Mo2 K1 O8 -56.2(13) . . . 1_545 ?
Mo1 Mo2 K1 O8 125.6(10) 1_455 . . 1_545 ?
Th2 Mo2 K1 O8 -28.1(11) . . . 1_545 ?
Sr1 Mo2 K1 O8 46.1(11) . . . 1_545 ?
O6 Mo2 K1 O15 -116.8(10) . . . . ?
O9 Mo2 K1 O15 131.0(11) . . . . ?
O12 Mo2 K1 O15 67.3(11) . . . . ?
O3 Mo2 K1 O15 -46.4(12) 1_455 . . . ?
O4 Mo2 K1 O15 -176.1(11) . . . . ?
Mo1 Mo2 K1 O15 5.7(8) 1_455 . . . ?
Th2 Mo2 K1 O15 -148.0(8) . . . . ?
Sr1 Mo2 K1 O15 -73.8(8) . . . . ?
O15 Mo2 K1 O5 -172.0(9) . . . . ?
O6 Mo2 K1 O5 71.2(8) . . . . ?
O9 Mo2 K1 O5 -41.0(8) . . . . ?
O12 Mo2 K1 O5 -104.8(9) . . . . ?
O3 Mo2 K1 O5 141.6(9) 1_455 . . . ?
O4 Mo2 K1 O5 11.9(9) . . . . ?
Mo1 Mo2 K1 O5 -166.3(4) 1_455 . . . ?
Th2 Mo2 K1 O5 40.0(4) . . . . ?
Sr1 Mo2 K1 O5 114.2(4) . . . . ?
O15 Mo2 K1 O24 35.7(10) . . . 1_545 ?
O6 Mo2 K1 O24 -81.1(9) . . . 1_545 ?
O9 Mo2 K1 O24 166.7(10) . . . 1_545 ?
O12 Mo2 K1 O24 102.9(9) . . . 1_545 ?
O3 Mo2 K1 O24 -10.7(10) 1_455 . . 1_545 ?
O4 Mo2 K1 O24 -140.4(9) . . . 1_545 ?
Mo1 Mo2 K1 O24 41.4(7) 1_455 . . 1_545 ?
Th2 Mo2 K1 O24 -112.3(6) . . . 1_545 ?
Sr1 Mo2 K1 O24 -38.1(6) . . . 1_545 ?
O15 Mo2 K1 O9 -131.0(11) . . . . ?
O6 Mo2 K1 O9 112.2(10) . . . . ?
O12 Mo2 K1 O9 -63.7(10) . . . . ?
O3 Mo2 K1 O9 -177.3(11) 1_455 . . . ?
O4 Mo2 K1 O9 53.0(10) . . . . ?
Mo1 Mo2 K1 O9 -125.3(7) 1_455 . . . ?
Th2 Mo2 K1 O9 81.0(7) . . . . ?
Sr1 Mo2 K1 O9 155.3(7) . . . . ?
O15 Mo2 K1 O1 -37.0(10) . . . 2_556 ?
O6 Mo2 K1 O1 -153.8(10) . . . 2_556 ?
O9 Mo2 K1 O1 94.0(10) . . . 2_556 ?
O12 Mo2 K1 O1 30.3(11) . . . 2_556 ?
O3 Mo2 K1 O1 -83.4(11) 1_455 . . 2_556 ?
O4 Mo2 K1 O1 147.0(9) . . . 2_556 ?
Mo1 Mo2 K1 O1 -31.3(8) 1_455 . . 2_556 ?
Th2 Mo2 K1 O1 175.0(7) . . . 2_556 ?
Sr1 Mo2 K1 O1 -110.8(7) . . . 2_556 ?
O15 Mo2 K1 O13 -113.1(10) . . . 2_656 ?
O6 Mo2 K1 O13 130.1(9) . . . 2_656 ?
O9 Mo2 K1 O13 17.9(9) . . . 2_656 ?
O12 Mo2 K1 O13 -45.8(10) . . . 2_656 ?
O3 Mo2 K1 O13 -159.5(9) 1_455 . . 2_656 ?
O4 Mo2 K1 O13 70.9(9) . . . 2_656 ?
Mo1 Mo2 K1 O13 -107.4(6) 1_455 . . 2_656 ?
Th2 Mo2 K1 O13 98.9(6) . . . 2_656 ?
Sr1 Mo2 K1 O13 173.1(6) . . . 2_656 ?
O15 Mo2 K1 O18 67.6(9) . . . 1_545 ?
O6 Mo2 K1 O18 -49.1(8) . . . 1_545 ?
O9 Mo2 K1 O18 -161.4(8) . . . 1_545 ?
O12 Mo2 K1 O18 134.9(9) . . . 1_545 ?
O3 Mo2 K1 O18 21.3(9) 1_455 . . 1_545 ?
O4 Mo2 K1 O18 -108.4(8) . . . 1_545 ?
Mo1 Mo2 K1 O18 73.4(5) 1_455 . . 1_545 ?
Th2 Mo2 K1 O18 -80.4(4) . . . 1_545 ?
Sr1 Mo2 K1 O18 -6.1(4) . . . 1_545 ?
O15 Mo2 K1 O6 116.8(10) . . . . ?
O9 Mo2 K1 O6 -112.2(10) . . . . ?
O12 Mo2 K1 O6 -176.0(10) . . . . ?
O3 Mo2 K1 O6 70.4(10) 1_455 . . . ?
O4 Mo2 K1 O6 -59.3(10) . . . . ?
Mo1 Mo2 K1 O6 122.5(7) 1_455 . . . ?
Th2 Mo2 K1 O6 -31.2(7) . . . . ?
Sr1 Mo2 K1 O6 43.0(7) . . . . ?
O15 Mo2 K1 Mo3 45.9(8) . . . 1_545 ?
O6 Mo2 K1 Mo3 -70.9(7) . . . 1_545 ?
O9 Mo2 K1 Mo3 176.9(7) . . . 1_545 ?
O12 Mo2 K1 Mo3 113.2(7) . . . 1_545 ?
O3 Mo2 K1 Mo3 -0.5(8) 1_455 . . 1_545 ?
O4 Mo2 K1 Mo3 -130.1(7) . . . 1_545 ?
Mo1 Mo2 K1 Mo3 51.6(3) 1_455 . . 1_545 ?
Th2 Mo2 K1 Mo3 -102.11(13) . . . 1_545 ?
Sr1 Mo2 K1 Mo3 -27.86(17) . . . 1_545 ?
Mo6 O17 K2 O7 -132.4(10) . . . 2_545 ?
Sr1 O17 K2 O7 82.4(7) 2_545 . . 2_545 ?
Mo6 O17 K2 O11 31(7) . . . 2 ?
Sr1 O17 K2 O11 -115(6) 2_545 . . 2 ?
Mo6 O17 K2 O10 14.7(7) . . . . ?
Sr1 O17 K2 O10 -130.5(9) 2_545 . . . ?
Mo6 O17 K2 O19 45.5(11) . . . 2 ?
Sr1 O17 K2 O19 -99.7(8) 2_545 . . 2 ?
Mo6 O17 K2 O22 -42.5(11) . . . 1_455 ?
Sr1 O17 K2 O22 172.3(7) 2_545 . . 1_455 ?
Mo6 O17 K2 O18 101.4(10) . . . 2 ?
Sr1 O17 K2 O18 -43.8(7) 2_545 . . 2 ?
Sr1 O17 K2 Mo6 -145.2(13) 2_545 . . . ?
Mo6 O17 K2 Mo4 51.9(14) . . . 2 ?
Sr1 O17 K2 Mo4 -93.2(9) 2_545 . . 2 ?
Mo6 O17 K2 Mo6 -110.0(8) . . . 2_545 ?
Sr1 O17 K2 Mo6 104.9(6) 2_545 . . 2_545 ?
Mo6 O17 K2 Sr1 145.2(13) . . . 2_545 ?
Mo6 O17 K2 Sr1 -80.3(12) . . . 2_445 ?
Sr1 O17 K2 Sr1 134.5(7) 2_545 . . 2_445 ?
Mo6 O10 K2 O7 25.7(11) . . . 2_545 ?
Th2 O10 K2 O7 -167.9(7) 2 . . 2_545 ?
Mo6 O10 K2 O17 -13.7(7) . . . . ?
Th2 O10 K2 O17 152.7(10) 2 . . . ?
Mo6 O10 K2 O11 168.4(8) . . . 2 ?
Th2 O10 K2 O11 -25.2(10) 2 . . 2 ?
Mo6 O10 K2 O19 -163.8(10) . . . 2 ?
Th2 O10 K2 O19 2.6(7) 2 . . 2 ?
Mo6 O10 K2 O22 116.8(9) . . . 1_455 ?
Th2 O10 K2 O22 -76.8(8) 2 . . 1_455 ?
Mo6 O10 K2 O18 -87.1(8) . . . 2 ?
Th2 O10 K2 O18 79.2(8) 2 . . 2 ?
Th2 O10 K2 Mo6 166.4(13) 2 . . . ?
Mo6 O10 K2 Mo4 -173.6(7) . . . 2 ?
Th2 O10 K2 Mo4 -7.2(7) 2 . . 2 ?
Mo6 O10 K2 Mo6 49.7(8) . . . 2_545 ?
Th2 O10 K2 Mo6 -143.9(5) 2 . . 2_545 ?
Mo6 O10 K2 Sr1 -41.6(7) . . . 2_545 ?
Th2 O10 K2 Sr1 124.8(7) 2 . . 2_545 ?
Mo6 O10 K2 Sr1 125.8(6) . . . 2_445 ?
Th2 O10 K2 Sr1 -67.8(8) 2 . . 2_445 ?
O17 Mo6 K2 O7 46.2(10) . . . 2_545 ?
O10 Mo6 K2 O7 -158.7(10) . . . 2_545 ?
O7 Mo6 K2 O7 -55.9(9) . . . 2_545 ?
O20 Mo6 K2 O7 42.3(13) . . . 2_545 ?
O14 Mo6 K2 O7 134.5(8) . . . 2_545 ?
O23 Mo6 K2 O7 -132.9(8) 2_655 . . 2_545 ?
Mo5 Mo6 K2 O7 94.1(5) . . . 2_545 ?
Th2 Mo6 K2 O7 -92.3(5) . . . 2_545 ?
K2 Mo6 K2 O7 -23.0(4) 2_545 . . 2_545 ?
Sr1 Mo6 K2 O7 69.4(5) 2_545 . . 2_545 ?
O10 Mo6 K2 O17 155.1(12) . . . . ?
O7 Mo6 K2 O17 -102.1(11) . . . . ?
O20 Mo6 K2 O17 -3.9(15) . . . . ?
O14 Mo6 K2 O17 88.3(11) . . . . ?
O23 Mo6 K2 O17 -179.1(12) 2_655 . . . ?
Mo5 Mo6 K2 O17 47.9(9) . . . . ?
Th2 Mo6 K2 O17 -138.5(9) . . . . ?
K2 Mo6 K2 O17 -69.2(9) 2_545 . . . ?
Sr1 Mo6 K2 O17 23.2(9) 2_545 . . . ?
O17 Mo6 K2 O11 -173.8(14) . . . 2 ?
O10 Mo6 K2 O11 -18.7(12) . . . 2 ?
O7 Mo6 K2 O11 84.1(11) . . . 2 ?
O20 Mo6 K2 O11 -177.7(15) . . . 2 ?
O14 Mo6 K2 O11 -85.5(12) . . . 2 ?
O23 Mo6 K2 O11 7.1(13) 2_655 . . 2 ?
Mo5 Mo6 K2 O11 -125.9(10) . . . 2 ?
Th2 Mo6 K2 O11 47.7(10) . . . 2 ?
K2 Mo6 K2 O11 117.1(10) 2_545 . . 2 ?
Sr1 Mo6 K2 O11 -150.5(10) 2_545 . . 2 ?
O17 Mo6 K2 O10 -155.1(12) . . . . ?
O7 Mo6 K2 O10 102.8(10) . . . . ?
O20 Mo6 K2 O10 -159.0(14) . . . . ?
O14 Mo6 K2 O10 -66.8(10) . . . . ?
O23 Mo6 K2 O10 25.8(11) 2_655 . . . ?
Mo5 Mo6 K2 O10 -107.2(8) . . . . ?
Th2 Mo6 K2 O10 66.4(8) . . . . ?
K2 Mo6 K2 O10 135.7(8) 2_545 . . . ?
Sr1 Mo6 K2 O10 -131.9(8) 2_545 . . . ?
O17 Mo6 K2 O19 -140.2(11) . . . 2 ?
O10 Mo6 K2 O19 14.9(9) . . . 2 ?
O7 Mo6 K2 O19 117.7(7) . . . 2 ?
O20 Mo6 K2 O19 -144.1(13) . . . 2 ?
O14 Mo6 K2 O19 -51.8(8) . . . 2 ?
O23 Mo6 K2 O19 40.7(9) 2_655 . . 2 ?
Mo5 Mo6 K2 O19 -92.3(5) . . . 2 ?
Th2 Mo6 K2 O19 81.3(5) . . . 2 ?
K2 Mo6 K2 O19 150.7(5) 2_545 . . 2 ?
Sr1 Mo6 K2 O19 -116.9(5) 2_545 . . 2 ?
O17 Mo6 K2 O22 142.7(11) . . . 1_455 ?
O10 Mo6 K2 O22 -62.2(9) . . . 1_455 ?
O7 Mo6 K2 O22 40.5(8) . . . 1_455 ?
O20 Mo6 K2 O22 138.7(13) . . . 1_455 ?
O14 Mo6 K2 O22 -129.0(8) . . . 1_455 ?
O23 Mo6 K2 O22 -36.5(9) 2_655 . . 1_455 ?
Mo5 Mo6 K2 O22 -169.4(5) . . . 1_455 ?
Th2 Mo6 K2 O22 4.2(5) . . . 1_455 ?
K2 Mo6 K2 O22 73.5(5) 2_545 . . 1_455 ?
Sr1 Mo6 K2 O22 165.9(5) 2_545 . . 1_455 ?
O17 Mo6 K2 O18 -69.9(10) . . . 2 ?
O10 Mo6 K2 O18 85.2(9) . . . 2 ?
O7 Mo6 K2 O18 -172.1(8) . . . 2 ?
O20 Mo6 K2 O18 -73.9(13) . . . 2 ?
O14 Mo6 K2 O18 18.4(8) . . . 2 ?
O23 Mo6 K2 O18 110.9(9) 2_655 . . 2 ?
Mo5 Mo6 K2 O18 -22.0(5) . . . 2 ?
Th2 Mo6 K2 O18 151.6(5) . . . 2 ?
K2 Mo6 K2 O18 -139.1(5) 2_545 . . 2 ?
Sr1 Mo6 K2 O18 -46.7(5) 2_545 . . 2 ?
O17 Mo6 K2 Mo4 -147.4(10) . . . 2 ?
O10 Mo6 K2 Mo4 7.7(8) . . . 2 ?
O7 Mo6 K2 Mo4 110.5(6) . . . 2 ?
O20 Mo6 K2 Mo4 -151.3(12) . . . 2 ?
O14 Mo6 K2 Mo4 -59.1(7) . . . 2 ?
O23 Mo6 K2 Mo4 33.5(8) 2_655 . . 2 ?
Mo5 Mo6 K2 Mo4 -99.5(3) . . . 2 ?
Th2 Mo6 K2 Mo4 74.1(3) . . . 2 ?
K2 Mo6 K2 Mo4 143.5(4) 2_545 . . 2 ?
Sr1 Mo6 K2 Mo4 -124.1(3) 2_545 . . 2 ?
O17 Mo6 K2 Mo6 69.2(9) . . . 2_545 ?
O10 Mo6 K2 Mo6 -135.7(8) . . . 2_545 ?
O7 Mo6 K2 Mo6 -32.9(6) . . . 2_545 ?
O20 Mo6 K2 Mo6 65.2(12) . . . 2_545 ?
O14 Mo6 K2 Mo6 157.5(6) . . . 2_545 ?
O23 Mo6 K2 Mo6 -110.0(7) 2_655 . . 2_545 ?
Mo5 Mo6 K2 Mo6 117.07(16) . . . 2_545 ?
Th2 Mo6 K2 Mo6 -69.33(16) . . . 2_545 ?
K2 Mo6 K2 Mo6 0.0 2_545 . . 2_545 ?
Sr1 Mo6 K2 Mo6 92.41(17) 2_545 . . 2_545 ?
O17 Mo6 K2 Sr1 -23.2(9) . . . 2_545 ?
O10 Mo6 K2 Sr1 131.9(8) . . . 2_545 ?
O7 Mo6 K2 Sr1 -125.4(6) . . . 2_545 ?
O20 Mo6 K2 Sr1 -27.2(12) . . . 2_545 ?
O14 Mo6 K2 Sr1 65.1(7) . . . 2_545 ?
O23 Mo6 K2 Sr1 157.6(7) 2_655 . . 2_545 ?
Mo5 Mo6 K2 Sr1 24.7(2) . . . 2_545 ?
Th2 Mo6 K2 Sr1 -161.75(10) . . . 2_545 ?
K2 Mo6 K2 Sr1 -92.42(17) 2_545 . . 2_545 ?
O17 Mo6 K2 Sr1 130.1(10) . . . 2_445 ?
O10 Mo6 K2 Sr1 -74.8(8) . . . 2_445 ?
O7 Mo6 K2 Sr1 28.0(7) . . . 2_445 ?
O20 Mo6 K2 Sr1 126.2(12) . . . 2_445 ?
O14 Mo6 K2 Sr1 -141.6(7) . . . 2_445 ?
O23 Mo6 K2 Sr1 -49.0(8) 2_655 . . 2_445 ?
Mo5 Mo6 K2 Sr1 178.0(2) . . . 2_445 ?
Th2 Mo6 K2 Sr1 -8.4(3) . . . 2_445 ?
K2 Mo6 K2 Sr1 60.9(3) 2_545 . . 2_445 ?
Sr1 Mo6 K2 Sr1 153.3(4) 2_545 . . 2_445 ?

_diffrn_measured_fraction_theta_max 0.979
_diffrn_reflns_theta_full        26.37
_diffrn_measured_fraction_theta_full 0.979
_refine_diff_density_max         4.429
_refine_diff_density_min         -5.567
_refine_diff_density_rms         0.848
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Mo9Nd2O36Th3
_database_code_depnum_ccdc_archive 'CCDC 1430751'
_audit_update_record             
;
2015-10-16 deposited with the CCDC.
2015-11-12 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Mo18 Nd4 O72 Th6'
_chemical_formula_weight         4848.12

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nd Nd -0.1943 3.0179 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Th Th -7.2400 8.8979 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Hexagonal
_symmetry_space_group_name_H-M   'P 63/m'
_symmetry_space_group_name_Hall  '-P 6c'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'

_cell_length_a                   17.556(3)
_cell_length_b                   17.556(3)
_cell_length_c                   6.2713(10)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_volume                     1673.9(5)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    2817
_cell_measurement_theta_min      3.2471
_cell_measurement_theta_max      34.7471

_exptl_crystal_description       
;
'Wed Jul 17 08:54:07 2013'
;
_exptl_crystal_colour            
;
'Wed Jul 17 08:54:07 2013'
;
_exptl_crystal_size_max          0.7
_exptl_crystal_size_mid          0.6
_exptl_crystal_size_min          0.4
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.809
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2112
_exptl_absorpt_coefficient_mu    19.663
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.30311
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   
;
'Wed Jul 17 08:54:07 2013'
;

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Eos'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean 15.9834
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            19895
_diffrn_reflns_av_R_equivalents  0.1405
_diffrn_reflns_av_sigmaI/netI    0.0446
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_theta_min         3.51
_diffrn_reflns_theta_max         28.27
_reflns_number_total             1506
_reflns_number_gt                512
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       
;
'Wed Jul 17 08:54:07 2013'
;
_computing_cell_refinement       
;
'Wed Jul 17 08:54:07 2013'
;
_computing_data_reduction        
;
'Wed Jul 17 08:54:07 2013'
;
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0509P)²+0.3353P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    .
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         1506
_refine_ls_number_parameters     95
_refine_ls_number_restraints     54
_refine_ls_R_factor_all          0.0914
_refine_ls_R_factor_gt           0.0414
_refine_ls_wR_factor_ref         0.1435
_refine_ls_wR_factor_gt          0.1117
_refine_ls_goodness_of_fit_ref   1.140
_refine_ls_restrained_S_all      1.124
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Nd1 Nd 0.0000 0.0000 0.5000 0.0233(14) Uani 0.672(10) 6 d SP . .
Nd2 Nd 0.6667 0.3333 0.5023(6) 0.0242(8) Uani 0.683(6) 3 d SP . .
Th1 Th 0.33347(7) 0.00030(7) 0.7500 0.0145(2) Uani 1 2 d S . .
Mo1 Mo 0.59974(15) 0.10199(15) 0.7500 0.0181(5) Uani 1 2 d S . .
Mo2 Mo -0.23156(14) -0.16485(15) 0.2500 0.0151(5) Uani 1 2 d S . .
Mo3 Mo 0.43546(16) 0.16935(14) 0.2500 0.0168(5) Uani 1 2 d S . .
O1 O -0.2482(10) -0.2285(9) 0.473(3) 0.043(4) Uani 1 1 d U . .
O2 O 0.4228(10) 0.1103(9) 0.487(2) 0.043(4) Uani 1 1 d U . .
O3 O -0.3044(10) -0.1244(11) 0.2500 0.020(4) Uani 1 2 d SU . .
O4 O 0.4873(13) 0.0305(13) 0.7500 0.035(5) Uani 1 2 d SU . .
O5 O 0.6476(10) 0.0867(11) 0.525(2) 0.051(4) Uani 1 1 d U . .
O6 O 0.3634(13) 0.2082(13) 0.2500 0.039(5) Uani 1 2 d SU . .
O7 O -0.1245(14) -0.0809(16) 0.2500 0.053(6) Uani 1 2 d SU . .
O8 O 0.6225(14) 0.2150(13) 0.7500 0.041(5) Uani 1 2 d SU . .
O9 O 0.5471(12) 0.2602(13) 0.2500 0.035(5) Uani 1 2 d SU . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Nd1 O7 2.480(17) 9_556 ?
Nd1 O7 2.480(17) 3 ?
Nd1 O7 2.480(17) 8_556 ?
Nd1 O7 2.480(17) . ?
Nd1 O7 2.480(17) 7_556 ?
Nd1 O7 2.480(17) 2 ?
Nd1 Nd1 3.1356(5) 4 ?
Nd1 Nd1 3.1356(5) 4_554 ?
Nd2 O8 2.391(15) 2_655 ?
Nd2 O8 2.391(15) . ?
Nd2 O8 2.391(15) 3_665 ?
Nd2 O9 2.421(14) 2_655 ?
Nd2 O9 2.421(15) . ?
Nd2 O9 2.422(14) 3_665 ?
Nd2 Nd2 3.106(7) 10_557 ?
Nd2 Nd2 3.165(7) 10_556 ?
Th1 O2 2.424(14) 10_557 ?
Th1 O2 2.424(14) . ?
Th1 O1 2.428(15) 2 ?
Th1 O1 2.428(15) 11_557 ?
Th1 O5 2.435(16) 7_656 ?
Th1 O5 2.435(16) 4_655 ?
Th1 O3 2.474(16) 7_556 ?
Th1 O4 2.48(2) . ?
Th1 O6 2.51(2) 8_556 ?
Mo1 O5 1.730(15) . ?
Mo1 O5 1.730(15) 10_557 ?
Mo1 O4 1.73(2) . ?
Mo1 O8 1.82(2) . ?
Mo2 O1 1.721(15) 10_556 ?
Mo2 O1 1.721(15) . ?
Mo2 O7 1.71(2) . ?
Mo2 O3 1.746(16) . ?
Mo3 O6 1.71(2) . ?
Mo3 O2 1.762(14) 10_556 ?
Mo3 O2 1.762(14) . ?
Mo3 O9 1.806(19) . ?
O1 Th1 2.428(15) 3 ?
O3 Th1 2.473(16) 7_556 ?
O5 Th1 2.435(16) 7_656 ?
O6 Th1 2.51(2) 9_556 ?
O7 Nd1 2.480(17) 4_554 ?
O8 Nd2 2.391(15) 10_557 ?
O9 Nd2 2.422(14) 10_556 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O7 Nd1 O7 179.998(1) 9_556 3 ?
O7 Nd1 O7 84.3(5) 9_556 8_556 ?
O7 Nd1 O7 95.7(5) 3 8_556 ?
O7 Nd1 O7 95.7(5) 9_556 . ?
O7 Nd1 O7 84.3(5) 3 . ?
O7 Nd1 O7 95.7(5) 8_556 . ?
O7 Nd1 O7 84.3(5) 9_556 7_556 ?
O7 Nd1 O7 95.7(5) 3 7_556 ?
O7 Nd1 O7 84.3(5) 8_556 7_556 ?
O7 Nd1 O7 179.998(1) . 7_556 ?
O7 Nd1 O7 95.7(5) 9_556 2 ?
O7 Nd1 O7 84.3(5) 3 2 ?
O7 Nd1 O7 179.999(1) 8_556 2 ?
O7 Nd1 O7 84.3(5) . 2 ?
O7 Nd1 O7 95.7(5) 7_556 2 ?
O7 Nd1 Nd1 50.8(3) 9_556 4 ?
O7 Nd1 Nd1 129.2(3) 3 4 ?
O7 Nd1 Nd1 50.8(3) 8_556 4 ?
O7 Nd1 Nd1 129.2(3) . 4 ?
O7 Nd1 Nd1 50.8(3) 7_556 4 ?
O7 Nd1 Nd1 129.2(3) 2 4 ?
O7 Nd1 Nd1 129.2(3) 9_556 4_554 ?
O7 Nd1 Nd1 50.8(3) 3 4_554 ?
O7 Nd1 Nd1 129.2(3) 8_556 4_554 ?
O7 Nd1 Nd1 50.8(3) . 4_554 ?
O7 Nd1 Nd1 129.2(3) 7_556 4_554 ?
O7 Nd1 Nd1 50.8(3) 2 4_554 ?
Nd1 Nd1 Nd1 180.0 4 4_554 ?
O8 Nd2 O8 82.4(5) 2_655 . ?
O8 Nd2 O8 82.4(5) 2_655 3_665 ?
O8 Nd2 O8 82.4(5) . 3_665 ?
O8 Nd2 O9 98.4(6) 2_655 2_655 ?
O8 Nd2 O9 97.4(6) . 2_655 ?
O8 Nd2 O9 179.2(8) 3_665 2_655 ?
O8 Nd2 O9 179.2(8) 2_655 . ?
O8 Nd2 O9 98.4(6) . . ?
O8 Nd2 O9 97.4(6) 3_665 . ?
O9 Nd2 O9 81.9(5) 2_655 . ?
O8 Nd2 O9 97.4(6) 2_655 3_665 ?
O8 Nd2 O9 179.2(8) . 3_665 ?
O8 Nd2 O9 98.4(6) 3_665 3_665 ?
O9 Nd2 O9 81.9(5) 2_655 3_665 ?
O9 Nd2 O9 81.9(5) . 3_665 ?
O8 Nd2 Nd2 49.5(3) 2_655 10_557 ?
O8 Nd2 Nd2 49.5(3) . 10_557 ?
O8 Nd2 Nd2 49.5(3) 3_665 10_557 ?
O9 Nd2 Nd2 130.8(3) 2_655 10_557 ?
O9 Nd2 Nd2 130.8(3) . 10_557 ?
O9 Nd2 Nd2 130.8(3) 3_665 10_557 ?
O8 Nd2 Nd2 130.5(3) 2_655 10_556 ?
O8 Nd2 Nd2 130.5(3) . 10_556 ?
O8 Nd2 Nd2 130.5(3) 3_665 10_556 ?
O9 Nd2 Nd2 49.2(3) 2_655 10_556 ?
O9 Nd2 Nd2 49.2(3) . 10_556 ?
O9 Nd2 Nd2 49.2(3) 3_665 10_556 ?
Nd2 Nd2 Nd2 180.0 10_557 10_556 ?
O2 Th1 O2 85.7(7) 10_557 . ?
O2 Th1 O1 138.0(5) 10_557 2 ?
O2 Th1 O1 76.7(5) . 2 ?
O2 Th1 O1 76.7(5) 10_557 11_557 ?
O2 Th1 O1 138.0(5) . 11_557 ?
O1 Th1 O1 91.5(7) 2 11_557 ?
O2 Th1 O5 138.1(6) 10_557 7_656 ?
O2 Th1 O5 77.4(5) . 7_656 ?
O1 Th1 O5 74.5(5) 2 7_656 ?
O1 Th1 O5 138.5(5) 11_557 7_656 ?
O2 Th1 O5 77.4(5) 10_557 4_655 ?
O2 Th1 O5 138.1(6) . 4_655 ?
O1 Th1 O5 138.5(5) 2 4_655 ?
O1 Th1 O5 74.5(5) 11_557 4_655 ?
O5 Th1 O5 90.3(7) 7_656 4_655 ?
O2 Th1 O3 68.5(4) 10_557 7_556 ?
O2 Th1 O3 68.5(4) . 7_556 ?
O1 Th1 O3 69.6(4) 2 7_556 ?
O1 Th1 O3 69.6(4) 11_557 7_556 ?
O5 Th1 O3 134.9(4) 7_656 7_556 ?
O5 Th1 O3 134.9(4) 4_655 7_556 ?
O2 Th1 O4 68.2(5) 10_557 . ?
O2 Th1 O4 68.2(5) . . ?
O1 Th1 O4 134.3(4) 2 . ?
O1 Th1 O4 134.3(4) 11_557 . ?
O5 Th1 O4 70.0(5) 7_656 . ?
O5 Th1 O4 70.0(5) 4_655 . ?
O3 Th1 O4 119.6(7) 7_556 . ?
O2 Th1 O6 137.2(3) 10_557 8_556 ?
O2 Th1 O6 137.2(3) . 8_556 ?
O1 Th1 O6 69.7(4) 2 8_556 ?
O1 Th1 O6 69.7(4) 11_557 8_556 ?
O5 Th1 O6 68.8(5) 7_656 8_556 ?
O5 Th1 O6 68.8(5) 4_655 8_556 ?
O3 Th1 O6 120.3(7) 7_556 8_556 ?
O4 Th1 O6 120.1(7) . 8_556 ?
O5 Mo1 O5 109.2(10) . 10_557 ?
O5 Mo1 O4 110.7(6) . . ?
O5 Mo1 O4 110.7(6) 10_557 . ?
O5 Mo1 O8 108.1(7) . . ?
O5 Mo1 O8 108.1(7) 10_557 . ?
O4 Mo1 O8 109.9(10) . . ?
O1 Mo2 O1 108.6(10) 10_556 . ?
O1 Mo2 O7 108.4(7) 10_556 . ?
O1 Mo2 O7 108.4(7) . . ?
O1 Mo2 O3 110.1(5) 10_556 . ?
O1 Mo2 O3 110.1(5) . . ?
O7 Mo2 O3 111.2(10) . . ?
O6 Mo3 O2 109.5(6) . 10_556 ?
O6 Mo3 O2 109.5(6) . . ?
O2 Mo3 O2 115.1(9) 10_556 . ?
O6 Mo3 O9 109.9(10) . . ?
O2 Mo3 O9 106.4(6) 10_556 . ?
O2 Mo3 O9 106.4(6) . . ?
Mo2 O1 Th1 156.2(8) . 3 ?
Mo3 O2 Th1 152.1(9) . . ?
Mo2 O3 Th1 150.9(9) . 7_556 ?
Mo1 O4 Th1 151.8(11) . . ?
Mo1 O5 Th1 154.7(9) . 7_656 ?
Mo3 O6 Th1 150.7(11) . 9_556 ?
Mo2 O7 Nd1 140.0(4) . 4_554 ?
Mo2 O7 Nd1 140.0(4) . . ?
Nd1 O7 Nd1 78.4(6) 4_554 . ?
Mo1 O8 Nd2 138.3(4) . 10_557 ?
Mo1 O8 Nd2 138.3(4) . . ?
Nd2 O8 Nd2 81.0(6) 10_557 . ?
Mo3 O9 Nd2 137.6(4) . . ?
Mo3 O9 Nd2 137.6(4) . 10_556 ?
Nd2 O9 Nd2 81.6(6) . 10_556 ?

_diffrn_measured_fraction_theta_max 0.994
_diffrn_reflns_theta_full        28.27
_diffrn_measured_fraction_theta_full 0.994
_refine_diff_density_max         3.201
_refine_diff_density_min         -1.998
_refine_diff_density_rms         0.364
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Rb2MgTh3Mo8O32
_database_code_depnum_ccdc_archive 'CCDC 1430752'
_audit_update_record             
;
2015-10-16 deposited with the CCDC.
2015-11-12 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        Rb2MgTh3(MoO4)8
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Mg Mo8 O32 Rb2 Th3'
_chemical_formula_weight         2170.89

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Th Th -7.2400 8.8979 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_symmetry_space_group_name_Hall  '-C 2yc'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   18.6792(4)
_cell_length_b                   18.0812(5)
_cell_length_c                   9.4616(3)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.230(2)
_cell_angle_gamma                90.00
_cell_volume                     3195.55(15)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    2604
_cell_measurement_theta_min      3.0563
_cell_measurement_theta_max      30.6650
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.512
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3792
_exptl_absorpt_coefficient_mu    20.079
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.79714
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   
;
'Wed Oct 16 13:51:03 2013'
;

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Eos'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean 15.9834
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            10641
_diffrn_reflns_av_R_equivalents  0.0607
_diffrn_reflns_av_sigmaI/netI    0.0660
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_theta_min         3.12
_diffrn_reflns_theta_max         26.37
_reflns_number_total             3222
_reflns_number_gt                2617
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       
;
'Wed Oct 16 13:51:03 2013'
;
_computing_cell_refinement       
;
'Wed Oct 16 13:51:03 2013'
;
_computing_data_reduction        
;
'Wed Oct 16 13:51:03 2013'
;
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0105P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    .
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.000115(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         3222
_refine_ls_number_parameters     210
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0482
_refine_ls_R_factor_gt           0.0342
_refine_ls_wR_factor_ref         0.0611
_refine_ls_wR_factor_gt          0.0559
_refine_ls_goodness_of_fit_ref   0.996
_refine_ls_restrained_S_all      0.996
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Th1 Th 0.0000 0.13010(3) 0.2500 0.00854(13) Uani 1 2 d S . .
Th2 Th 0.249572(19) 0.11910(2) -0.33905(3) 0.00854(10) Uani 1 1 d . . .
Mo1 Mo 0.11845(4) 0.02537(5) -0.04803(8) 0.00828(18) Uani 1 1 d . . .
Mo2 Mo 0.09058(4) 0.26019(5) 0.52925(8) 0.00984(19) Uani 1 1 d . . .
Mo3 Mo 0.21296(4) 0.17831(5) 0.24584(8) 0.0109(2) Uani 1 1 d . . .
Mo4 Mo 0.37951(4) 0.03257(5) -0.03552(8) 0.00900(19) Uani 1 1 d . . .
Mg1 Mg 0.5000 0.0896(2) 0.2500 0.0084(10) Uani 1 2 d S . .
Rb1 Rb 0.11818(6) 0.25876(7) -0.06204(11) 0.0271(3) Uani 1 1 d . . .
O1 O 0.2345(4) 0.1524(4) 0.4189(7) 0.032(2) Uani 1 1 d . . .
O2 O 0.0183(3) 0.2197(4) 0.4318(7) 0.0190(17) Uani 1 1 d . . .
O3 O 0.3286(3) 0.0888(4) -0.1532(6) 0.0170(16) Uani 1 1 d . . .
O4 O 0.1508(4) 0.3033(4) 0.4127(7) 0.0218(17) Uani 1 1 d . . .
O5 O 0.1725(4) 0.0867(4) -0.1441(6) 0.0193(17) Uani 1 1 d . . .
O6 O 0.4249(3) 0.0901(4) 0.0847(6) 0.0137(15) Uani 1 1 d . . .
O7 O 0.1685(4) -0.0247(4) 0.0781(7) 0.0218(17) Uani 1 1 d . . .
O8 O 0.2479(4) 0.2672(4) 0.2052(7) 0.0185(16) Uani 1 1 d . . .
O9 O 0.0551(4) 0.3216(4) 0.6511(7) 0.0212(17) Uani 1 1 d . . .
O10 O 0.1189(4) 0.1776(4) 0.2138(7) 0.0262(19) Uani 1 1 d . . .
O11 O 0.4419(3) -0.0137(4) -0.1362(6) 0.0169(16) Uani 1 1 d . . .
O12 O 0.0514(3) 0.0766(4) 0.0350(7) 0.0194(17) Uani 1 1 d . . .
O13 O 0.0784(4) -0.0384(4) -0.1658(7) 0.0270(19) Uani 1 1 d . . .
O14 O 0.3249(4) -0.0321(4) 0.0532(7) 0.0239(18) Uani 1 1 d . . .
O15 O 0.1363(4) 0.1912(4) 0.6254(7) 0.0239(18) Uani 1 1 d . . .
O16 O 0.2535(4) 0.1194(4) 0.1314(7) 0.034(2) Uani 1 1 d . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Th1 O13 2.349(7) 6_556 ?
Th1 O13 2.349(7) 5 ?
Th1 O2 2.387(6) 2 ?
Th1 O2 2.387(6) . ?
Th1 O10 2.407(7) 2 ?
Th1 O10 2.407(7) . ?
Th1 O12 2.452(6) 2 ?
Th1 O12 2.452(6) . ?
Th1 Rb1 4.3651(11) . ?
Th1 Rb1 4.3651(11) 2 ?
Th2 O14 2.346(7) 6 ?
Th2 O3 2.355(6) . ?
Th2 O1 2.384(7) 1_554 ?
Th2 O7 2.410(7) 6 ?
Th2 O8 2.415(7) 7 ?
Th2 O5 2.416(6) . ?
Th2 O4 2.435(7) 7 ?
Th2 O15 2.506(7) 1_554 ?
Th2 Rb1 4.3957(12) . ?
Mo1 O12 1.747(6) . ?
Mo1 O5 1.756(6) . ?
Mo1 O7 1.764(6) . ?
Mo1 O13 1.768(6) . ?
Mo1 Rb1 4.2222(15) . ?
Mo2 O9 1.735(7) . ?
Mo2 O4 1.760(7) . ?
Mo2 O15 1.763(7) . ?
Mo2 O2 1.788(6) . ?
Mo2 Rb1 3.8992(13) 1_556 ?
Mo2 Rb1 3.9132(14) 2 ?
Mo3 O16 1.699(7) . ?
Mo3 O1 1.748(7) . ?
Mo3 O8 1.777(6) . ?
Mo3 O10 1.782(7) . ?
Mo3 Rb1 3.7008(13) . ?
Mo3 Rb1 3.7830(14) 7 ?
Mo4 O11 1.724(6) . ?
Mo4 O6 1.757(6) . ?
Mo4 O14 1.766(7) . ?
Mo4 O3 1.781(6) . ?
Mo4 Rb1 3.8844(15) 7 ?
Mg1 O11 2.056(7) 6_556 ?
Mg1 O11 2.056(7) 5_655 ?
Mg1 O6 2.096(6) 2_655 ?
Mg1 O6 2.096(6) . ?
Mg1 O9 2.126(8) 7_556 ?
Mg1 O9 2.126(8) 8 ?
Mg1 Rb1 3.940(3) 8_556 ?
Mg1 Rb1 3.940(3) 7 ?
Rb1 O6 2.857(7) 7 ?
Rb1 O8 2.888(7) 7 ?
Rb1 O2 2.923(7) 2 ?
Rb1 O10 2.995(7) . ?
Rb1 O9 3.166(7) 1_554 ?
Rb1 O15 3.219(7) 1_554 ?
Rb1 O16 3.323(8) 7 ?
Rb1 O5 3.364(7) . ?
Rb1 O8 3.498(7) . ?
Rb1 O9 3.528(7) 2 ?
Rb1 O3 3.567(7) 7 ?
O1 Th2 2.384(7) 1_556 ?
O2 Rb1 2.923(7) 2 ?
O3 Rb1 3.567(7) 7 ?
O4 Th2 2.435(7) 7 ?
O6 Rb1 2.857(7) 7 ?
O7 Th2 2.410(7) 6_556 ?
O8 Th2 2.415(7) 7 ?
O8 Rb1 2.888(7) 7 ?
O9 Mg1 2.126(8) 7_556 ?
O9 Rb1 3.166(7) 1_556 ?
O9 Rb1 3.529(7) 2 ?
O11 Mg1 2.056(7) 5_655 ?
O13 Th1 2.349(7) 5 ?
O14 Th2 2.346(7) 6_556 ?
O15 Th2 2.506(7) 1_556 ?
O15 Rb1 3.218(7) 1_556 ?
O16 Rb1 3.323(8) 7 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O13 Th1 O13 90.2(4) 6_556 5 ?
O13 Th1 O2 144.2(2) 6_556 2 ?
O13 Th1 O2 98.5(2) 5 2 ?
O13 Th1 O2 98.5(2) 6_556 . ?
O13 Th1 O2 144.2(2) 5 . ?
O2 Th1 O2 94.5(3) 2 . ?
O13 Th1 O10 141.1(2) 6_556 2 ?
O13 Th1 O10 74.1(2) 5 2 ?
O2 Th1 O10 74.4(2) 2 2 ?
O2 Th1 O10 77.6(2) . 2 ?
O13 Th1 O10 74.1(2) 6_556 . ?
O13 Th1 O10 141.1(2) 5 . ?
O2 Th1 O10 77.6(2) 2 . ?
O2 Th1 O10 74.4(2) . . ?
O10 Th1 O10 138.2(4) 2 . ?
O13 Th1 O12 71.7(2) 6_556 2 ?
O13 Th1 O12 76.0(2) 5 2 ?
O2 Th1 O12 144.1(2) 2 2 ?
O2 Th1 O12 74.1(2) . 2 ?
O10 Th1 O12 70.0(2) 2 2 ?
O10 Th1 O12 128.5(2) . 2 ?
O13 Th1 O12 76.0(2) 6_556 . ?
O13 Th1 O12 71.7(2) 5 . ?
O2 Th1 O12 74.1(2) 2 . ?
O2 Th1 O12 144.1(2) . . ?
O10 Th1 O12 128.5(2) 2 . ?
O10 Th1 O12 70.0(2) . . ?
O12 Th1 O12 133.5(3) 2 . ?
O13 Th1 Rb1 106.82(17) 6_556 . ?
O13 Th1 Rb1 117.57(17) 5 . ?
O2 Th1 Rb1 38.94(16) 2 . ?
O2 Th1 Rb1 93.10(16) . . ?
O10 Th1 Rb1 112.07(18) 2 . ?
O10 Th1 Rb1 40.92(16) . . ?
O12 Th1 Rb1 166.46(16) 2 . ?
O12 Th1 Rb1 56.52(17) . . ?
O13 Th1 Rb1 117.58(17) 6_556 2 ?
O13 Th1 Rb1 106.82(17) 5 2 ?
O2 Th1 Rb1 93.10(16) 2 2 ?
O2 Th1 Rb1 38.94(16) . 2 ?
O10 Th1 Rb1 40.92(16) 2 2 ?
O10 Th1 Rb1 112.07(18) . 2 ?
O12 Th1 Rb1 56.52(17) 2 2 ?
O12 Th1 Rb1 166.46(16) . 2 ?
Rb1 Th1 Rb1 115.59(3) . 2 ?
O14 Th2 O3 78.1(2) 6 . ?
O14 Th2 O1 79.7(3) 6 1_554 ?
O3 Th2 O1 147.9(2) . 1_554 ?
O14 Th2 O7 76.2(2) 6 6 ?
O3 Th2 O7 118.0(2) . 6 ?
O1 Th2 O7 78.1(2) 1_554 6 ?
O14 Th2 O8 142.0(2) 6 7 ?
O3 Th2 O8 78.2(2) . 7 ?
O1 Th2 O8 106.9(2) 1_554 7 ?
O7 Th2 O8 141.6(2) 6 7 ?
O14 Th2 O5 121.9(2) 6 . ?
O3 Th2 O5 75.3(2) . . ?
O1 Th2 O5 136.6(2) 1_554 . ?
O7 Th2 O5 72.6(2) 6 . ?
O8 Th2 O5 79.4(2) 7 . ?
O14 Th2 O4 78.6(2) 6 7 ?
O3 Th2 O4 82.5(2) . 7 ?
O1 Th2 O4 70.6(2) 1_554 7 ?
O7 Th2 O4 142.6(2) 6 7 ?
O8 Th2 O4 69.3(2) 7 7 ?
O5 Th2 O4 144.7(2) . 7 ?
O14 Th2 O15 142.9(2) 6 1_554 ?
O3 Th2 O15 138.3(2) . 1_554 ?
O1 Th2 O15 69.1(2) 1_554 1_554 ?
O7 Th2 O15 78.2(2) 6 1_554 ?
O8 Th2 O15 69.0(2) 7 1_554 ?
O5 Th2 O15 74.0(2) . 1_554 ?
O4 Th2 O15 107.9(2) 7 1_554 ?
O14 Th2 Rb1 168.94(17) 6 . ?
O3 Th2 Rb1 92.19(16) . . ?
O1 Th2 Rb1 111.32(19) 1_554 . ?
O7 Th2 Rb1 104.42(17) 6 . ?
O8 Th2 Rb1 37.63(16) 7 . ?
O5 Th2 Rb1 49.34(17) . . ?
O4 Th2 Rb1 105.61(16) 7 . ?
O15 Th2 Rb1 46.22(16) 1_554 . ?
O12 Mo1 O5 108.2(3) . . ?
O12 Mo1 O7 110.3(3) . . ?
O5 Mo1 O7 111.7(3) . . ?
O12 Mo1 O13 109.1(3) . . ?
O5 Mo1 O13 109.2(3) . . ?
O7 Mo1 O13 108.3(3) . . ?
O12 Mo1 Rb1 58.9(2) . . ?
O5 Mo1 Rb1 49.7(2) . . ?
O7 Mo1 Rb1 122.4(2) . . ?
O13 Mo1 Rb1 129.2(3) . . ?
O9 Mo2 O4 112.3(3) . . ?
O9 Mo2 O15 107.2(3) . . ?
O4 Mo2 O15 109.1(3) . . ?
O9 Mo2 O2 108.3(3) . . ?
O4 Mo2 O2 109.9(3) . . ?
O15 Mo2 O2 109.9(3) . . ?
O9 Mo2 Rb1 52.7(2) . 1_556 ?
O4 Mo2 Rb1 122.8(2) . 1_556 ?
O15 Mo2 Rb1 54.7(2) . 1_556 ?
O2 Mo2 Rb1 127.2(2) . 1_556 ?
O9 Mo2 Rb1 64.4(2) . 2 ?
O4 Mo2 Rb1 133.8(2) . 2 ?
O15 Mo2 Rb1 115.8(2) . 2 ?
O2 Mo2 Rb1 44.6(2) . 2 ?
Rb1 Mo2 Rb1 92.82(3) 1_556 2 ?
O16 Mo3 O1 109.1(4) . . ?
O16 Mo3 O8 105.3(4) . . ?
O1 Mo3 O8 111.2(3) . . ?
O16 Mo3 O10 109.2(4) . . ?
O1 Mo3 O10 112.3(3) . . ?
O8 Mo3 O10 109.4(3) . . ?
O16 Mo3 Rb1 87.6(3) . . ?
O1 Mo3 Rb1 161.8(3) . . ?
O8 Mo3 Rb1 69.4(2) . . ?
O10 Mo3 Rb1 53.2(2) . . ?
O16 Mo3 Rb1 61.4(3) . 7 ?
O1 Mo3 Rb1 108.8(3) . 7 ?
O8 Mo3 Rb1 47.2(2) . 7 ?
O10 Mo3 Rb1 138.4(2) . 7 ?
Rb1 Mo3 Rb1 85.24(3) . 7 ?
O11 Mo4 O6 108.6(3) . . ?
O11 Mo4 O14 109.5(3) . . ?
O6 Mo4 O14 111.2(3) . . ?
O11 Mo4 O3 107.0(3) . . ?
O6 Mo4 O3 108.8(3) . . ?
O14 Mo4 O3 111.5(3) . . ?
O11 Mo4 Rb1 126.6(2) . 7 ?
O6 Mo4 Rb1 42.8(2) . 7 ?
O14 Mo4 Rb1 122.4(2) . 7 ?
O3 Mo4 Rb1 66.4(2) . 7 ?
O11 Mg1 O11 96.3(4) 6_556 5_655 ?
O11 Mg1 O6 88.0(3) 6_556 2_655 ?
O11 Mg1 O6 92.3(3) 5_655 2_655 ?
O11 Mg1 O6 92.3(3) 6_556 . ?
O11 Mg1 O6 88.0(3) 5_655 . ?
O6 Mg1 O6 179.5(4) 2_655 . ?
O11 Mg1 O9 90.9(3) 6_556 7_556 ?
O11 Mg1 O9 172.6(3) 5_655 7_556 ?
O6 Mg1 O9 89.5(3) 2_655 7_556 ?
O6 Mg1 O9 90.1(3) . 7_556 ?
O11 Mg1 O9 172.6(3) 6_556 8 ?
O11 Mg1 O9 90.9(3) 5_655 8 ?
O6 Mg1 O9 90.1(3) 2_655 8 ?
O6 Mg1 O9 89.5(3) . 8 ?
O9 Mg1 O9 81.9(4) 7_556 8 ?
O11 Mg1 Rb1 121.60(18) 6_556 8_556 ?
O11 Mg1 Rb1 113.86(18) 5_655 8_556 ?
O6 Mg1 Rb1 44.62(19) 2_655 8_556 ?
O6 Mg1 Rb1 134.9(2) . 8_556 ?
O9 Mg1 Rb1 63.0(2) 7_556 8_556 ?
O9 Mg1 Rb1 53.26(19) 8 8_556 ?
O11 Mg1 Rb1 113.86(18) 6_556 7 ?
O11 Mg1 Rb1 121.60(18) 5_655 7 ?
O6 Mg1 Rb1 134.9(2) 2_655 7 ?
O6 Mg1 Rb1 44.62(19) . 7 ?
O9 Mg1 Rb1 53.26(19) 7_556 7 ?
O9 Mg1 Rb1 63.0(2) 8 7 ?
Rb1 Mg1 Rb1 91.78(10) 8_556 7 ?
O6 Rb1 O8 111.39(18) 7 7 ?
O6 Rb1 O2 90.95(19) 7 2 ?
O8 Rb1 O2 156.5(2) 7 2 ?
O6 Rb1 O10 122.33(19) 7 . ?
O8 Rb1 O10 109.15(19) 7 . ?
O2 Rb1 O10 60.99(18) 2 . ?
O6 Rb1 O9 59.23(17) 7 1_554 ?
O8 Rb1 O9 88.67(18) 7 1_554 ?
O2 Rb1 O9 97.22(18) 2 1_554 ?
O10 Rb1 O9 157.46(18) . 1_554 ?
O6 Rb1 O15 108.95(17) 7 1_554 ?
O8 Rb1 O15 54.05(18) 7 1_554 ?
O2 Rb1 O15 113.02(18) 2 1_554 ?
O10 Rb1 O15 127.91(19) . 1_554 ?
O9 Rb1 O15 52.33(17) 1_554 1_554 ?
O6 Rb1 O16 63.53(19) 7 7 ?
O8 Rb1 O16 52.28(18) 7 7 ?
O2 Rb1 O16 150.99(19) 2 7 ?
O10 Rb1 O16 119.76(18) . 7 ?
O9 Rb1 O16 81.90(18) 1_554 7 ?
O15 Rb1 O16 89.51(17) 1_554 7 ?
O6 Rb1 O5 162.27(16) 7 . ?
O8 Rb1 O5 58.58(17) 7 . ?
O2 Rb1 O5 97.97(18) 2 . ?
O10 Rb1 O5 75.36(18) . . ?
O9 Rb1 O5 104.24(17) 1_554 . ?
O15 Rb1 O5 53.42(16) 1_554 . ?
O16 Rb1 O5 110.42(17) 7 . ?
O6 Rb1 O8 101.93(16) 7 . ?
O8 Rb1 O8 75.35(19) 7 . ?
O2 Rb1 O8 107.98(17) 2 . ?
O10 Rb1 O8 52.46(17) . . ?
O9 Rb1 O8 149.15(17) 1_554 . ?
O15 Rb1 O8 127.25(17) 1_554 . ?
O16 Rb1 O8 67.40(17) 7 . ?
O5 Rb1 O8 89.90(16) . . ?
O6 Rb1 O9 54.27(17) 7 2 ?
O8 Rb1 O9 137.37(17) 7 2 ?
O2 Rb1 O9 51.52(17) 2 2 ?
O10 Rb1 O9 111.53(17) . 2 ?
O9 Rb1 O9 48.8(2) 1_554 2 ?
O15 Rb1 O9 90.16(16) 1_554 2 ?
O16 Rb1 O9 113.63(18) 7 2 ?
O5 Rb1 O9 121.34(16) . 2 ?
O8 Rb1 O9 142.22(16) . 2 ?
O6 Rb1 O3 51.79(15) 7 7 ?
O8 Rb1 O3 98.81(17) 7 7 ?
O2 Rb1 O3 100.81(18) 2 7 ?
O10 Rb1 O3 83.16(17) . 7 ?
O9 Rb1 O3 108.31(16) 1_554 7 ?
O15 Rb1 O3 141.98(16) 1_554 7 ?
O16 Rb1 O3 53.17(16) 7 7 ?
O5 Rb1 O3 139.70(16) . 7 ?
O8 Rb1 O3 50.41(15) . 7 ?
O9 Rb1 O3 98.10(16) 2 7 ?
O6 Rb1 Mo3 124.68(12) 7 . ?
O8 Rb1 Mo3 83.83(13) 7 . ?
O2 Rb1 Mo3 89.34(12) 2 . ?
O10 Rb1 Mo3 28.44(13) . . ?
O9 Rb1 Mo3 172.44(13) 1_554 . ?
O15 Rb1 Mo3 121.48(12) 1_554 . ?
O16 Rb1 Mo3 94.18(13) 7 . ?
O5 Rb1 Mo3 70.98(11) . . ?
O8 Rb1 Mo3 28.41(11) . . ?
O9 Rb1 Mo3 138.59(11) 2 . ?
O3 Rb1 Mo3 73.91(10) 7 . ?
Mo3 O1 Th2 173.4(4) . 1_556 ?
Mo2 O2 Th1 139.0(4) . . ?
Mo2 O2 Rb1 110.0(3) . 2 ?
Th1 O2 Rb1 110.2(2) . 2 ?
Mo4 O3 Th2 158.6(4) . . ?
Mo4 O3 Rb1 86.4(2) . 7 ?
Th2 O3 Rb1 114.8(2) . 7 ?
Mo2 O4 Th2 157.7(3) . 7 ?
Mo1 O5 Th2 153.4(4) . . ?
Mo1 O5 Rb1 106.9(3) . . ?
Th2 O5 Rb1 97.6(2) . . ?
Mo4 O6 Mg1 143.1(4) . . ?
Mo4 O6 Rb1 112.5(3) . 7 ?
Mg1 O6 Rb1 104.4(3) . 7 ?
Mo1 O7 Th2 156.1(4) . 6_556 ?
Mo3 O8 Th2 131.5(3) . 7 ?
Mo3 O8 Rb1 105.9(3) . 7 ?
Th2 O8 Rb1 111.7(2) 7 7 ?
Mo3 O8 Rb1 82.1(2) . . ?
Th2 O8 Rb1 115.4(2) 7 . ?
Rb1 O8 Rb1 104.65(19) 7 . ?
Mo2 O9 Mg1 164.4(4) . 7_556 ?
Mo2 O9 Rb1 101.4(3) . 1_556 ?
Mg1 O9 Rb1 94.2(2) 7_556 1_556 ?
Mo2 O9 Rb1 89.3(3) . 2 ?
Mg1 O9 Rb1 84.5(2) 7_556 2 ?
Rb1 O9 Rb1 115.3(2) 1_556 2 ?
Mo3 O10 Th1 152.7(4) . . ?
Mo3 O10 Rb1 98.4(3) . . ?
Th1 O10 Rb1 107.3(2) . . ?
Mo4 O11 Mg1 166.5(4) . 5_655 ?
Mo1 O12 Th1 150.0(4) . . ?
Mo1 O13 Th1 159.4(4) . 5 ?
Mo4 O14 Th2 177.3(4) . 6_556 ?
Mo2 O15 Th2 147.6(4) . 1_556 ?
Mo2 O15 Rb1 98.8(3) . 1_556 ?
Th2 O15 Rb1 99.6(2) 1_556 1_556 ?
Mo3 O16 Rb1 91.9(3) . 7 ?

_diffrn_measured_fraction_theta_max 0.986
_diffrn_reflns_theta_full        26.37
_diffrn_measured_fraction_theta_full 0.986
_refine_diff_density_max         1.291
_refine_diff_density_min         -1.507
_refine_diff_density_rms         0.331
